# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2018

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_exp_3141
_database_code_depnum_ccdc_archive 'CCDC 1419125'
_audit_update_record             
;
2015-08-17 deposited with the CCDC.
2018-04-06 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         '0.666667(C4.5 F1.5 Na4.5 O13.5 Zn3)'
_chemical_formula_sum            'C3 F Na3 O9 Zn2'
_chemical_formula_weight         398.74

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_H-M_alt        'C 1 2/c 1'
_space_group_name_Hall           '-C 2yc'

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   14.6090(15)
_cell_length_b                   8.5274(7)
_cell_length_c                   20.1877(13)
_cell_angle_alpha                90.00
_cell_angle_beta                 102.426(7)
_cell_angle_gamma                90.00
_cell_volume                     2456.0(4)
_cell_formula_units_Z            12
_cell_measurement_reflns_used    1737
_cell_measurement_temperature    103.5
_cell_measurement_theta_max      29.5298
_cell_measurement_theta_min      3.0948

_exptl_crystal_description       plate
_exptl_crystal_colour            colorless
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.05
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    3.235
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             2304
_exptl_absorpt_coefficient_mu    6.081
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.29658
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
CrysAlisPro, Agilent Technologies,
Version 1.171.35.11 (release 16-05-2011 CrysAlis171 .NET)
(compiled May 16 2011,17:55:39)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;

_diffrn_ambient_temperature      103(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Xcalibur, Eos, Gemini'
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            5589
_diffrn_reflns_av_R_equivalents  0.0321
_diffrn_reflns_av_sigmaI/netI    0.0417
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_theta_min         3.14
_diffrn_reflns_theta_max         25.99
_reflns_number_total             2421
_reflns_number_gt                1982
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    ?
_computing_publication_material  ?

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0555P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    none
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         2421
_refine_ls_number_parameters     255
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0526
_refine_ls_R_factor_gt           0.0438
_refine_ls_wR_factor_ref         0.1150
_refine_ls_wR_factor_gt          0.1084
_refine_ls_goodness_of_fit_ref   1.132
_refine_ls_restrained_S_all      1.132
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Zn1 Zn 0.19292(4) 0.27228(7) 0.34666(2) 0.00792(19) Uani 1 1 d . . .
Zn2 Zn 0.13619(3) 0.27578(6) 0.14991(2) 0.00641(18) Uani 1 1 d . . .
Zn3 Zn 0.02503(3) -0.23285(6) 0.34978(2) 0.00618(18) Uani 1 1 d . . .
Na1 Na 0.14639(12) -0.0414(2) 0.24981(8) 0.0107(4) Uani 1 1 d . . .
Na2 Na 0.0000 0.4090(3) 0.2500 0.0103(5) Uani 1 2 d S . .
Na3 Na 0.23474(11) -0.0571(2) 0.43302(8) 0.0096(4) Uani 1 1 d . . .
Na4 Na 0.05478(13) 0.4409(2) 0.44546(10) 0.0191(5) Uani 1 1 d . . .
Na5 Na 0.38170(12) 0.4047(2) 0.42984(9) 0.0117(4) Uani 1 1 d . . .
F1 F 0.0000 -0.1682(4) 0.2500 0.0111(8) Uani 1 2 d S . .
C5 C 0.2500 0.2500 0.5000 0.0114(15) Uani 1 2 d S . .
C4 C 0.0887(3) 0.7585(5) 0.49889(19) 0.0096(11) Uani 1 1 d . . .
O5 O 0.4392(2) 0.0803(4) 0.32556(15) 0.0091(6) Uani 1 1 d . . .
O6 O 0.29826(19) -0.0155(3) 0.32687(14) 0.0070(6) Uani 1 1 d . . .
O2 O -0.02241(19) -0.0139(3) 0.36109(14) 0.0075(6) Uani 1 1 d . . .
O8 O 0.21966(19) 0.0886(4) 0.15592(14) 0.0065(6) Uani 1 1 d . . .
O7 O 0.3381(2) 0.2437(4) 0.14555(16) 0.0098(7) Uani 1 1 d . . .
O3 O 0.0038(2) 0.2423(4) 0.36927(16) 0.0123(7) Uani 1 1 d . . .
F2 F 0.12599(17) 0.2377(3) 0.24805(11) 0.0102(6) Uani 1 1 d . . .
O12 O 0.1143(2) 0.6575(4) 0.54814(14) 0.0111(7) Uani 1 1 d . . .
O4 O 0.3210(2) 0.2432(3) 0.32628(16) 0.0106(7) Uani 1 1 d . . .
O1 O 0.1195(2) 0.0800(3) 0.36144(14) 0.0089(6) Uani 1 1 d . . .
O11 O 0.1258(2) 0.8903(4) 0.49899(14) 0.0136(7) Uani 1 1 d . . .
O10 O 0.0209(2) 0.7103(4) 0.44987(14) 0.0112(7) Uani 1 1 d . . .
O9 O 0.3603(2) -0.0130(4) 0.1576(2) 0.0251(9) Uani 1 1 d . . .
C1 C 0.0338(3) 0.1027(5) 0.3640(2) 0.0074(9) Uani 1 1 d . . .
C3 C 0.3062(3) 0.1066(5) 0.1533(2) 0.0091(10) Uani 1 1 d . . .
C2 C 0.3529(3) 0.1019(5) 0.3261(2) 0.0067(9) Uiso 1 1 d . . .
O13 O 0.1813(4) 0.3367(7) 0.5097(3) 0.0096(13) Uani 0.50 1 d P . -1
O15 O 0.2847(4) 0.1522(7) 0.5514(3) 0.0125(14) Uani 0.50 1 d P . -1
O14 O 0.2746(4) 0.2314(7) 0.4457(3) 0.0078(13) Uani 0.50 1 d P . -1


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Zn1 O9 1.984(4) 4 ?
Zn1 O4 2.015(3) . ?
Zn1 O1 2.016(3) . ?
Zn1 F2 2.041(2) . ?
Zn1 O15 2.114(6) 7_556 ?
Zn1 O14 2.125(6) . ?
Zn1 Na5 3.1158(18) . ?
Zn1 Na2 3.2777(11) . ?
Zn1 Na3 3.2931(19) . ?
Zn1 Na1 3.2966(19) . ?
Zn1 Na4 3.4426(18) . ?
Zn2 O8 1.996(3) . ?
Zn2 O3 2.019(3) 2 ?
Zn2 O6 2.028(3) 4 ?
Zn2 F2 2.045(2) . ?
Zn2 O12 2.089(3) 6_565 ?
Zn2 Na3 3.1220(17) 4 ?
Zn2 Na2 3.3260(10) . ?
Zn2 Na4 3.341(2) 2 ?
Zn2 Na1 3.3581(19) . ?
Zn2 Na5 3.5341(19) 4_545 ?
Zn3 O7 1.992(3) 4_545 ?
Zn3 O2 2.022(3) . ?
Zn3 O5 2.022(3) 3_445 ?
Zn3 F1 2.0440(11) . ?
Zn3 O10 2.092(3) 1_545 ?
Zn3 Na5 3.1353(17) 3_445 ?
Zn3 Na1 3.2882(18) 2 ?
Zn3 Na4 3.361(2) 1_545 ?
Zn3 Na1 3.3795(18) . ?
Zn3 Na3 3.4985(18) . ?
Zn3 Na2 3.633(2) 1_545 ?
Na1 F1 2.397(2) . ?
Na1 F2 2.398(3) . ?
Na1 O6 2.430(3) . ?
Na1 O4 2.505(3) 4_545 ?
Na1 O2 2.570(3) 2 ?
Na1 O1 2.585(3) . ?
Na1 O8 2.615(3) . ?
Na1 O7 2.769(4) 4_545 ?
Na1 Zn3 3.2882(18) 2 ?
Na2 F2 2.357(3) 2 ?
Na2 F2 2.357(3) . ?
Na2 O5 2.415(3) 3_455 ?
Na2 O5 2.415(3) 4 ?
Na2 O9 2.540(4) 4 ?
Na2 O9 2.540(4) 3_455 ?
Na2 O3 2.786(3) 2 ?
Na2 O3 2.786(3) . ?
Na2 Zn1 3.2777(11) 2 ?
Na2 Zn2 3.3260(10) 2 ?
Na3 O1 2.289(3) . ?
Na3 O12 2.319(3) 7_556 ?
Na3 O11 2.328(3) 1_545 ?
Na3 O13 2.401(6) 7_556 ?
Na3 O7 2.410(3) 4_545 ?
Na3 O14 2.529(6) . ?
Na3 O6 2.537(3) . ?
Na3 C5 2.9338(18) . ?
Na3 O15 2.946(6) . ?
Na3 Zn2 3.1220(17) 4_545 ?
Na4 O13 2.203(6) . ?
Na4 O3 2.302(4) . ?
Na4 O10 2.355(4) . ?
Na4 O15 2.463(6) 7_556 ?
Na4 O12 2.639(3) 5_566 ?
Na4 O9 2.671(4) 4 ?
Na4 O12 2.773(4) . ?
Na4 O10 2.890(4) 5_566 ?
Na4 O5 2.892(4) 3_455 ?
Na4 C4 2.917(5) . ?
Na4 C4 3.092(5) 5_566 ?
Na4 Na4 3.153(4) 5_566 ?
Na5 O14 2.224(6) . ?
Na5 O11 2.280(3) 7_566 ?
Na5 O2 2.282(3) 3 ?
Na5 O4 2.501(3) . ?
Na5 O8 2.558(3) 4 ?
Na5 O15 2.586(6) 7_556 ?
Na5 O10 2.587(4) 3_545 ?
Na5 O13 2.657(6) 7_556 ?
Na5 C5 2.9362(17) . ?
Na5 Zn3 3.1353(17) 3 ?
Na5 Zn2 3.5341(19) 4 ?
F1 Zn3 2.0440(11) 2 ?
F1 Na1 2.397(2) 2 ?
C5 O14 1.236(6) 7_556 ?
C5 O14 1.236(6) . ?
C5 O13 1.295(6) 7_556 ?
C5 O13 1.295(6) . ?
C5 O15 1.342(6) . ?
C5 O15 1.342(6) 7_556 ?
C5 Na3 2.9338(18) 7_556 ?
C5 Na5 2.9362(17) 7_556 ?
C4 O11 1.248(5) . ?
C4 O10 1.307(5) . ?
C4 O12 1.307(5) . ?
C4 Na4 3.092(5) 5_566 ?
O5 C2 1.276(5) . ?
O5 Zn3 2.022(3) 3 ?
O5 Na2 2.415(3) 3_545 ?
O5 Na4 2.892(4) 3_545 ?
O6 C2 1.282(5) . ?
O6 Zn2 2.028(3) 4_545 ?
O2 C1 1.282(5) . ?
O2 Na5 2.282(3) 3_445 ?
O2 Na1 2.570(3) 2 ?
O8 C3 1.286(5) . ?
O8 Na5 2.558(3) 4_545 ?
O7 C3 1.280(5) . ?
O7 Zn3 1.992(3) 4 ?
O7 Na3 2.410(3) 4 ?
O7 Na1 2.769(4) 4 ?
O3 C1 1.281(5) . ?
O3 Zn2 2.019(3) 2 ?
O12 Zn2 2.089(3) 6_566 ?
O12 Na3 2.319(3) 7_556 ?
O12 Na4 2.639(3) 5_566 ?
O4 C2 1.293(5) . ?
O4 Na1 2.505(3) 4 ?
O1 C1 1.280(5) . ?
O11 Na5 2.280(3) 7_566 ?
O11 Na3 2.328(3) 1_565 ?
O10 Zn3 2.092(3) 1_565 ?
O10 Na5 2.587(4) 3_455 ?
O10 Na4 2.890(4) 5_566 ?
O9 C3 1.281(5) . ?
O9 Zn1 1.984(4) 4_545 ?
O9 Na2 2.540(4) 3_545 ?
O9 Na4 2.671(4) 4_545 ?
O13 Na3 2.401(6) 7_556 ?
O13 Na5 2.657(6) 7_556 ?
O15 Zn1 2.114(6) 7_556 ?
O15 Na4 2.463(6) 7_556 ?
O15 Na5 2.586(6) 7_556 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O9 Zn1 O4 118.48(13) 4 . ?
O9 Zn1 O1 122.77(12) 4 . ?
O4 Zn1 O1 118.47(12) . . ?
O9 Zn1 F2 89.42(13) 4 . ?
O4 Zn1 F2 93.10(11) . . ?
O1 Zn1 F2 82.44(11) . . ?
O9 Zn1 O15 74.8(2) 4 7_556 ?
O4 Zn1 O15 106.30(18) . 7_556 ?
O1 Zn1 O15 94.54(18) . 7_556 ?
F2 Zn1 O15 159.16(18) . 7_556 ?
O9 Zn1 O14 109.14(19) 4 . ?
O4 Zn1 O14 79.25(18) . . ?
O1 Zn1 O14 86.36(18) . . ?
F2 Zn1 O14 161.41(18) . . ?
O15 Zn1 O14 36.5(2) 7_556 . ?
O9 Zn1 Na5 88.96(11) 4 . ?
O4 Zn1 Na5 53.26(9) . . ?
O1 Zn1 Na5 130.71(9) . . ?
F2 Zn1 Na5 139.51(8) . . ?
O15 Zn1 Na5 55.36(16) 7_556 . ?
O14 Zn1 Na5 45.53(16) . . ?
O9 Zn1 Na2 50.74(11) 4 . ?
O4 Zn1 Na2 129.74(9) . . ?
O1 Zn1 Na2 87.76(9) . . ?
F2 Zn1 Na2 45.64(7) . . ?
O15 Zn1 Na2 113.83(17) 7_556 . ?
O14 Zn1 Na2 148.81(15) . . ?
Na5 Zn1 Na2 137.72(6) . . ?
O9 Zn1 Na3 146.79(11) 4 . ?
O4 Zn1 Na3 85.90(9) . . ?
O1 Zn1 Na3 43.27(9) . . ?
F2 Zn1 Na3 112.85(8) . . ?
O15 Zn1 Na3 76.82(17) 7_556 . ?
O14 Zn1 Na3 50.17(16) . . ?
Na5 Zn1 Na3 88.97(5) . . ?
Na2 Zn1 Na3 131.02(5) . . ?
O9 Zn1 Na1 133.97(11) 4 . ?
O4 Zn1 Na1 82.02(9) . . ?
O1 Zn1 Na1 51.65(9) . . ?
F2 Zn1 Na1 46.38(8) . . ?
O15 Zn1 Na1 142.51(17) 7_556 . ?
O14 Zn1 Na1 115.29(16) . . ?
Na5 Zn1 Na1 131.26(5) . . ?
Na2 Zn1 Na1 83.94(5) . . ?
Na3 Zn1 Na1 67.23(4) . . ?
O9 Zn1 Na4 50.70(11) 4 . ?
O4 Zn1 Na4 148.79(9) . . ?
O1 Zn1 Na4 81.80(9) . . ?
F2 Zn1 Na4 114.07(8) . . ?
O15 Zn1 Na4 45.21(17) 7_556 . ?
O14 Zn1 Na4 78.71(16) . . ?
Na5 Zn1 Na4 95.59(4) . . ?
Na2 Zn1 Na4 70.13(4) . . ?
Na3 Zn1 Na4 96.59(5) . . ?
Na1 Zn1 Na4 127.65(5) . . ?
O8 Zn2 O3 118.62(12) . 2 ?
O8 Zn2 O6 115.84(12) . 4 ?
O3 Zn2 O6 125.25(12) 2 4 ?
O8 Zn2 F2 89.14(11) . . ?
O3 Zn2 F2 83.18(12) 2 . ?
O6 Zn2 F2 92.55(10) 4 . ?
O8 Zn2 O12 103.86(12) . 6_565 ?
O3 Zn2 O12 85.17(12) 2 6_565 ?
O6 Zn2 O12 87.31(11) 4 6_565 ?
F2 Zn2 O12 165.63(11) . 6_565 ?
O8 Zn2 Na3 88.06(9) . 4 ?
O3 Zn2 Na3 131.74(10) 2 4 ?
O6 Zn2 Na3 54.11(8) 4 4 ?
F2 Zn2 Na3 140.40(8) . 4 ?
O12 Zn2 Na3 47.97(9) 6_565 4 ?
O8 Zn2 Na2 132.34(9) . . ?
O3 Zn2 Na2 56.69(9) 2 . ?
O6 Zn2 Na2 82.77(9) 4 . ?
F2 Zn2 Na2 44.57(7) . . ?
O12 Zn2 Na2 121.31(9) 6_565 . ?
Na3 Zn2 Na2 132.78(6) 4 . ?
O8 Zn2 Na4 142.70(9) . 2 ?
O3 Zn2 Na4 42.53(9) 2 2 ?
O6 Zn2 Na4 93.29(9) 4 2 ?
F2 Zn2 Na4 113.54(8) . 2 ?
O12 Zn2 Na4 52.16(9) 6_565 2 ?
Na3 Zn2 Na4 91.40(5) 4 2 ?
Na2 Zn2 Na4 70.83(4) . 2 ?
O8 Zn2 Na1 51.09(8) . . ?
O3 Zn2 Na1 85.03(9) 2 . ?
O6 Zn2 Na1 127.62(8) 4 . ?
F2 Zn2 Na1 45.02(8) . . ?
O12 Zn2 Na1 141.96(9) 6_565 . ?
Na3 Zn2 Na1 137.38(5) 4 . ?
Na2 Zn2 Na1 82.26(5) . . ?
Na4 Zn2 Na1 127.54(5) 2 . ?
O8 Zn2 Na5 45.27(9) . 4_545 ?
O3 Zn2 Na5 79.25(9) 2 4_545 ?
O6 Zn2 Na5 151.18(8) 4 4_545 ?
F2 Zn2 Na5 106.60(8) . 4_545 ?
O12 Zn2 Na5 79.34(9) 6_565 4_545 ?
Na3 Zn2 Na5 99.11(4) 4 4_545 ?
Na2 Zn2 Na5 125.96(5) . 4_545 ?
Na4 Zn2 Na5 98.29(5) 2 4_545 ?
Na1 Zn2 Na5 62.73(4) . 4_545 ?
O7 Zn3 O2 116.91(12) 4_545 . ?
O7 Zn3 O5 119.77(12) 4_545 3_445 ?
O2 Zn3 O5 123.04(12) . 3_445 ?
O7 Zn3 F1 92.22(9) 4_545 . ?
O2 Zn3 F1 82.49(12) . . ?
O5 Zn3 F1 90.23(12) 3_445 . ?
O7 Zn3 O10 99.70(12) 4_545 1_545 ?
O2 Zn3 O10 91.33(12) . 1_545 ?
O5 Zn3 O10 84.58(12) 3_445 1_545 ?
F1 Zn3 O10 168.06(9) . 1_545 ?
O7 Zn3 Na5 142.03(10) 4_545 3_445 ?
O2 Zn3 Na5 46.60(9) . 3_445 ?
O5 Zn3 Na5 88.35(9) 3_445 3_445 ?
F1 Zn3 Na5 114.17(7) . 3_445 ?
O10 Zn3 Na5 55.06(9) 1_545 3_445 ?
O7 Zn3 Na1 134.73(10) 4_545 2 ?
O2 Zn3 Na1 51.39(9) . 2 ?
O5 Zn3 Na1 83.81(9) 3_445 2 ?
F1 Zn3 Na1 46.56(5) . 2 ?
O10 Zn3 Na1 121.96(9) 1_545 2 ?
Na5 Zn3 Na1 67.92(4) 3_445 2 ?
O7 Zn3 Na4 83.40(9) 4_545 1_545 ?
O2 Zn3 Na4 134.80(9) . 1_545 ?
O5 Zn3 Na4 58.90(9) 3_445 1_545 ?
F1 Zn3 Na4 139.73(11) . 1_545 ?
O10 Zn3 Na4 43.94(9) 1_545 1_545 ?
Na5 Zn3 Na4 91.81(5) 3_445 1_545 ?
Na1 Zn3 Na4 138.56(5) 2 1_545 ?
O7 Zn3 Na1 55.00(9) 4_545 . ?
O2 Zn3 Na1 81.83(9) . . ?
O5 Zn3 Na1 127.89(9) 3_445 . ?
F1 Zn3 Na1 44.51(5) . . ?
O10 Zn3 Na1 144.78(9) 1_545 . ?
Na5 Zn3 Na1 128.42(5) 3_445 . ?
Na1 Zn3 Na1 79.83(6) 2 . ?
Na4 Zn3 Na1 136.33(5) 1_545 . ?
O7 Zn3 Na3 41.74(9) 4_545 . ?
O2 Zn3 Na3 80.57(9) . . ?
O5 Zn3 Na3 152.55(9) 3_445 . ?
F1 Zn3 Na3 108.08(7) . . ?
O10 Zn3 Na3 80.78(9) 1_545 . ?
Na5 Zn3 Na3 101.83(5) 3_445 . ?
Na1 Zn3 Na3 123.65(5) 2 . ?
Na4 Zn3 Na3 94.98(5) 1_545 . ?
Na1 Zn3 Na3 64.04(4) . . ?
O7 Zn3 Na2 85.52(9) 4_545 1_545 ?
O2 Zn3 Na2 147.45(8) . 1_545 ?
O5 Zn3 Na2 38.76(8) 3_445 1_545 ?
F1 Zn3 Na2 72.84(10) . 1_545 ?
O10 Zn3 Na2 108.68(9) 1_545 1_545 ?
Na5 Zn3 Na2 126.99(4) 3_445 1_545 ?
Na1 Zn3 Na2 96.07(4) 2 1_545 ?
Na4 Zn3 Na2 66.92(4) 1_545 1_545 ?
Na1 Zn3 Na2 94.48(4) . 1_545 ?
Na3 Zn3 Na2 126.84(3) . 1_545 ?
F1 Na1 F2 109.86(12) . . ?
F1 Na1 O6 137.05(10) . . ?
F2 Na1 O6 90.72(11) . . ?
F1 Na1 O4 87.58(11) . 4_545 ?
F2 Na1 O4 139.29(11) . 4_545 ?
O6 Na1 O4 101.02(11) . 4_545 ?
F1 Na1 O2 65.22(8) . 2 ?
F2 Na1 O2 80.46(10) . 2 ?
O6 Na1 O2 157.61(12) . 2 ?
O4 Na1 O2 73.99(10) 4_545 2 ?
F1 Na1 O1 82.91(9) . . ?
F2 Na1 O1 64.77(9) . . ?
O6 Na1 O1 72.21(10) . . ?
O4 Na1 O1 155.88(12) 4_545 . ?
O2 Na1 O1 120.80(11) 2 . ?
F1 Na1 O8 134.16(9) . . ?
F2 Na1 O8 68.75(10) . . ?
O6 Na1 O8 88.03(10) . . ?
O4 Na1 O8 72.83(10) 4_545 . ?
O2 Na1 O8 69.60(9) 2 . ?
O1 Na1 O8 128.64(13) . . ?
F1 Na1 O7 68.09(9) . 4_545 ?
F2 Na1 O7 131.13(10) . 4_545 ?
O6 Na1 O7 70.02(10) . 4_545 ?
O4 Na1 O7 89.27(11) 4_545 4_545 ?
O2 Na1 O7 130.68(11) 2 4_545 ?
O1 Na1 O7 66.61(10) . 4_545 ?
O8 Na1 O7 148.69(12) . 4_545 ?
F1 Na1 Zn3 38.25(3) . 2 ?
F2 Na1 Zn3 114.07(8) . 2 ?
O6 Na1 Zn3 155.07(10) . 2 ?
O4 Na1 Zn3 58.76(8) 4_545 2 ?
O2 Na1 Zn3 37.94(7) 2 2 ?
O1 Na1 Zn3 119.56(9) . 2 ?
O8 Na1 Zn3 98.27(8) . 2 ?
O7 Na1 Zn3 93.70(8) 4_545 2 ?
F1 Na1 Zn1 115.81(8) . . ?
F2 Na1 Zn1 38.05(6) . . ?
O6 Na1 Zn1 60.21(8) . . ?
O4 Na1 Zn1 156.41(10) 4_545 . ?
O2 Na1 Zn1 117.34(9) 2 . ?
O1 Na1 Zn1 37.70(7) . . ?
O8 Na1 Zn1 91.23(8) . . ?
O7 Na1 Zn1 96.44(8) 4_545 . ?
Zn3 Na1 Zn1 142.96(6) 2 . ?
F1 Na1 Zn2 116.10(9) . . ?
F2 Na1 Zn2 37.09(6) . . ?
O6 Na1 Zn2 103.16(9) . . ?
O4 Na1 Zn2 102.24(8) 4_545 . ?
O2 Na1 Zn2 58.08(7) 2 . ?
O1 Na1 Zn2 101.86(9) . . ?
O8 Na1 Zn2 36.44(7) . . ?
O7 Na1 Zn2 167.72(9) 4_545 . ?
Zn3 Na1 Zn2 95.92(4) 2 . ?
Zn1 Na1 Zn2 71.30(4) . . ?
F1 Na1 Zn3 36.71(3) . . ?
F2 Na1 Zn3 114.13(8) . . ?
O6 Na1 Zn3 100.70(8) . . ?
O4 Na1 Zn3 101.86(9) 4_545 . ?
O2 Na1 Zn3 101.68(8) 2 . ?
O1 Na1 Zn3 58.36(7) . . ?
O8 Na1 Zn3 170.62(9) . . ?
O7 Na1 Zn3 36.10(7) 4_545 . ?
Zn3 Na1 Zn3 72.36(4) 2 . ?
Zn1 Na1 Zn3 96.06(4) . . ?
Zn2 Na1 Zn3 141.87(6) . . ?
F2 Na2 F2 103.40(15) 2 . ?
F2 Na2 O5 88.25(9) 2 3_455 ?
F2 Na2 O5 141.28(9) . 3_455 ?
F2 Na2 O5 141.28(9) 2 4 ?
F2 Na2 O5 88.25(9) . 4 ?
O5 Na2 O5 105.58(17) 3_455 4 ?
F2 Na2 O9 131.10(11) 2 4 ?
F2 Na2 O9 70.58(9) . 4 ?
O5 Na2 O9 74.01(10) 3_455 4 ?
O5 Na2 O9 87.62(12) 4 4 ?
F2 Na2 O9 70.58(9) 2 3_455 ?
F2 Na2 O9 131.10(11) . 3_455 ?
O5 Na2 O9 87.62(12) 3_455 3_455 ?
O5 Na2 O9 74.01(10) 4 3_455 ?
O9 Na2 O9 149.6(2) 4 3_455 ?
F2 Na2 O3 80.08(10) 2 2 ?
F2 Na2 O3 62.61(9) . 2 ?
O5 Na2 O3 155.87(10) 3_455 2 ?
O5 Na2 O3 72.81(9) 4 2 ?
O9 Na2 O3 129.18(10) 4 2 ?
O9 Na2 O3 68.63(11) 3_455 2 ?
F2 Na2 O3 62.61(9) 2 . ?
F2 Na2 O3 80.08(10) . . ?
O5 Na2 O3 72.81(9) 3_455 . ?
O5 Na2 O3 155.87(10) 4 . ?
O9 Na2 O3 68.63(11) 4 . ?
O9 Na2 O3 129.18(10) 3_455 . ?
O3 Na2 O3 118.64(16) 2 . ?
F2 Na2 Zn1 38.27(6) 2 2 ?
F2 Na2 Zn1 110.13(9) . 2 ?
O5 Na2 Zn1 101.83(7) 3_455 2 ?
O5 Na2 Zn1 103.02(7) 4 2 ?
O9 Na2 Zn1 169.33(10) 4 2 ?
O9 Na2 Zn1 37.22(8) 3_455 2 ?
O3 Na2 Zn1 56.58(7) 2 2 ?
O3 Na2 Zn1 100.82(8) . 2 ?
F2 Na2 Zn1 110.13(9) 2 . ?
F2 Na2 Zn1 38.27(6) . . ?
O5 Na2 Zn1 103.02(7) 3_455 . ?
O5 Na2 Zn1 101.83(7) 4 . ?
O9 Na2 Zn1 37.22(8) 4 . ?
O9 Na2 Zn1 169.33(10) 3_455 . ?
O3 Na2 Zn1 100.82(8) 2 . ?
O3 Na2 Zn1 56.58(7) . . ?
Zn1 Na2 Zn1 138.33(9) 2 . ?
F2 Na2 Zn2 111.71(9) 2 . ?
F2 Na2 Zn2 37.51(6) . . ?
O5 Na2 Zn2 160.01(10) 3_455 . ?
O5 Na2 Zn2 58.22(7) 4 . ?
O9 Na2 Zn2 92.54(7) 4 . ?
O9 Na2 Zn2 97.74(8) 3_455 . ?
O3 Na2 Zn2 37.26(7) 2 . ?
O3 Na2 Zn2 116.57(9) . . ?
Zn1 Na2 Zn2 93.84(4) 2 . ?
Zn1 Na2 Zn2 71.94(3) . . ?
F2 Na2 Zn2 37.51(6) 2 2 ?
F2 Na2 Zn2 111.71(9) . 2 ?
O5 Na2 Zn2 58.22(7) 3_455 2 ?
O5 Na2 Zn2 160.01(10) 4 2 ?
O9 Na2 Zn2 97.74(8) 4 2 ?
O9 Na2 Zn2 92.54(7) 3_455 2 ?
O3 Na2 Zn2 116.57(9) 2 2 ?
O3 Na2 Zn2 37.26(7) . 2 ?
Zn1 Na2 Zn2 71.94(3) 2 2 ?
Zn1 Na2 Zn2 93.84(4) . 2 ?
Zn2 Na2 Zn2 140.06(9) . 2 ?
O1 Na3 O12 146.71(13) . 7_556 ?
O1 Na3 O11 87.67(12) . 1_545 ?
O12 Na3 O11 125.31(13) 7_556 1_545 ?
O1 Na3 O13 97.72(17) . 7_556 ?
O12 Na3 O13 80.85(16) 7_556 7_556 ?
O11 Na3 O13 102.49(16) 1_545 7_556 ?
O1 Na3 O7 77.54(12) . 4_545 ?
O12 Na3 O7 96.73(12) 7_556 4_545 ?
O11 Na3 O7 88.94(12) 1_545 4_545 ?
O13 Na3 O7 167.53(17) 7_556 4_545 ?
O1 Na3 O14 71.88(16) . . ?
O12 Na3 O14 98.76(17) 7_556 . ?
O11 Na3 O14 107.50(16) 1_545 . ?
O13 Na3 O14 26.74(18) 7_556 . ?
O7 Na3 O14 144.28(17) 4_545 . ?
O1 Na3 O6 75.41(11) . . ?
O12 Na3 O6 71.49(11) 7_556 . ?
O11 Na3 O6 158.37(12) 1_545 . ?
O13 Na3 O6 93.20(16) 7_556 . ?
O7 Na3 O6 74.49(11) 4_545 . ?
O14 Na3 O6 80.26(15) . . ?
O1 Na3 C5 78.91(9) . . ?
O12 Na3 C5 106.18(10) 7_556 . ?
O11 Na3 C5 84.36(9) 1_545 . ?
O13 Na3 C5 25.69(13) 7_556 . ?
O7 Na3 C5 155.74(10) 4_545 . ?
O14 Na3 C5 24.76(13) . . ?
O6 Na3 C5 105.01(9) . . ?
O1 Na3 O15 102.87(16) . . ?
O12 Na3 O15 91.70(15) 7_556 . ?
O11 Na3 O15 74.54(14) 1_545 . ?
O13 Na3 O15 28.71(17) 7_556 . ?
O7 Na3 O15 163.41(15) 4_545 . ?
O14 Na3 O15 46.92(17) . . ?
O6 Na3 O15 121.90(15) . . ?
C5 Na3 O15 26.39(12) . . ?
O1 Na3 Zn2 109.96(9) . 4_545 ?
O12 Na3 Zn2 42.00(8) 7_556 4_545 ?
O11 Na3 Zn2 141.72(11) 1_545 4_545 ?
O13 Na3 Zn2 108.11(14) 7_556 4_545 ?
O7 Na3 Zn2 63.73(8) 4_545 4_545 ?
O14 Na3 Zn2 110.21(14) . 4_545 ?
O6 Na3 Zn2 40.36(7) . 4_545 ?
C5 Na3 Zn2 131.28(6) . 4_545 ?
O15 Na3 Zn2 129.68(13) . 4_545 ?
O1 Na3 Zn1 37.13(8) . . ?
O12 Na3 Zn1 117.60(9) 7_556 . ?
O11 Na3 Zn1 113.29(10) 1_545 . ?
O13 Na3 Zn1 66.72(14) 7_556 . ?
O7 Na3 Zn1 104.33(9) 4_545 . ?
O14 Na3 Zn1 40.18(14) . . ?
O6 Na3 Zn1 59.55(8) . . ?
C5 Na3 Zn1 57.97(3) . . ?
O15 Na3 Zn1 84.14(13) . . ?
Zn2 Na3 Zn1 99.79(5) 4_545 . ?
O1 Na3 Zn3 57.78(8) . . ?
O12 Na3 Zn3 128.61(10) 7_556 . ?
O11 Na3 Zn3 63.67(8) 1_545 . ?
O13 Na3 Zn3 150.52(15) 7_556 . ?
O7 Na3 Zn3 33.38(8) 4_545 . ?
O14 Na3 Zn3 128.63(15) . . ?
O6 Na3 Zn3 95.50(8) . . ?
C5 Na3 Zn3 125.14(5) . . ?
O15 Na3 Zn3 133.46(13) . . ?
Zn2 Na3 Zn3 96.57(5) 4_545 . ?
Zn1 Na3 Zn3 93.87(4) . . ?
O13 Na4 O3 101.88(19) . . ?
O13 Na4 O10 121.86(19) . . ?
O3 Na4 O10 134.64(14) . . ?
O13 Na4 O15 35.05(19) . 7_556 ?
O3 Na4 O15 87.09(17) . 7_556 ?
O10 Na4 O15 121.35(17) . 7_556 ?
O13 Na4 O12 121.23(18) . 5_566 ?
O3 Na4 O12 68.09(11) . 5_566 ?
O10 Na4 O12 95.84(12) . 5_566 ?
O15 Na4 O12 142.37(19) 7_556 5_566 ?
O13 Na4 O9 92.64(17) . 4 ?
O3 Na4 O9 74.06(12) . 4 ?
O10 Na4 O9 91.30(12) . 4 ?
O15 Na4 O9 57.90(16) 7_556 4 ?
O12 Na4 O9 132.98(13) 5_566 4 ?
O13 Na4 O12 74.96(17) . . ?
O3 Na4 O12 173.83(13) . . ?
O10 Na4 O12 49.98(10) . . ?
O15 Na4 O12 92.96(17) 7_556 . ?
O12 Na4 O12 108.77(10) 5_566 . ?
O9 Na4 O12 111.14(12) 4 . ?
O13 Na4 O10 78.13(16) . 5_566 ?
O3 Na4 O10 92.33(12) . 5_566 ?
O10 Na4 O10 106.90(10) . 5_566 ?
O15 Na4 O10 110.40(17) 7_556 5_566 ?
O12 Na4 O10 46.60(9) 5_566 5_566 ?
O9 Na4 O10 161.79(13) 4 5_566 ?
O12 Na4 O10 81.87(10) . 5_566 ?
O13 Na4 O5 157.36(17) . 3_455 ?
O3 Na4 O5 72.33(11) . 3_455 ?
O10 Na4 O5 62.70(10) . 3_455 ?
O15 Na4 O5 122.38(16) 7_556 3_455 ?
O12 Na4 O5 77.72(10) 5_566 3_455 ?
O9 Na4 O5 64.73(11) 4 3_455 ?
O12 Na4 O5 112.63(11) . 3_455 ?
O10 Na4 O5 123.28(11) 5_566 3_455 ?
O13 Na4 C4 95.90(18) . . ?
O3 Na4 C4 159.24(15) . . ?
O10 Na4 C4 26.01(10) . . ?
O15 Na4 C4 101.82(17) 7_556 . ?
O12 Na4 C4 111.32(12) 5_566 . ?
O9 Na4 C4 94.65(12) 4 . ?
O12 Na4 C4 26.41(10) . . ?
O10 Na4 C4 101.83(11) 5_566 . ?
O5 Na4 C4 87.15(11) 3_455 . ?
O13 Na4 C4 96.48(17) . 5_566 ?
O3 Na4 C4 72.00(12) . 5_566 ?
O10 Na4 C4 110.98(12) . 5_566 ?
O15 Na4 C4 121.94(17) 7_556 5_566 ?
O12 Na4 C4 24.79(10) 5_566 5_566 ?
O9 Na4 C4 145.98(12) 4 5_566 ?
O12 Na4 C4 102.88(11) . 5_566 ?
O10 Na4 C4 24.94(9) 5_566 5_566 ?
O5 Na4 C4 102.15(11) 3_455 5_566 ?
C4 Na4 C4 116.78(11) . 5_566 ?
O13 Na4 Na4 101.87(17) . 5_566 ?
O3 Na4 Na4 124.20(13) . 5_566 ?
O10 Na4 Na4 61.29(9) . 5_566 ?
O15 Na4 Na4 135.09(18) 7_556 5_566 ?
O12 Na4 Na4 56.37(8) 5_566 5_566 ?
O9 Na4 Na4 152.59(14) 4 5_566 ?
O12 Na4 Na4 52.41(8) . 5_566 ?
O10 Na4 Na4 45.62(8) 5_566 5_566 ?
O5 Na4 Na4 99.23(11) 3_455 5_566 ?
C4 Na4 Na4 61.09(10) . 5_566 ?
C4 Na4 Na4 55.68(9) 5_566 5_566 ?
O14 Na5 O11 106.76(17) . 7_566 ?
O14 Na5 O2 146.32(18) . 3 ?
O11 Na5 O2 105.61(13) 7_566 3 ?
O14 Na5 O4 67.69(17) . . ?
O11 Na5 O4 153.17(13) 7_566 . ?
O2 Na5 O4 79.21(11) 3 . ?
O14 Na5 O8 100.49(18) . 4 ?
O11 Na5 O8 81.80(12) 7_566 4 ?
O2 Na5 O8 75.15(11) 3 4 ?
O4 Na5 O8 73.88(10) . 4 ?
O14 Na5 O15 30.9(2) . 7_556 ?
O11 Na5 O15 82.96(16) 7_566 7_556 ?
O2 Na5 O15 149.98(17) 3 7_556 ?
O4 Na5 O15 81.01(15) . 7_556 ?
O8 Na5 O15 77.81(16) 4 7_556 ?
O14 Na5 O10 96.02(18) . 3_545 ?
O11 Na5 O10 122.38(12) 7_566 3_545 ?
O2 Na5 O10 74.06(11) 3 3_545 ?
O4 Na5 O10 84.44(11) . 3_545 ?
O8 Na5 O10 145.04(11) 4 3_545 ?
O15 Na5 O10 126.07(17) 7_556 3_545 ?
O14 Na5 O13 25.23(18) . 7_556 ?
O11 Na5 O13 103.65(15) 7_566 7_556 ?
O2 Na5 O13 146.50(16) 3 7_556 ?
O4 Na5 O13 82.06(15) . 7_556 ?
O8 Na5 O13 125.35(15) 4 7_556 ?
O15 Na5 O13 50.03(18) 7_556 7_556 ?
O10 Na5 O13 76.69(15) 3_545 7_556 ?
O14 Na5 C5 22.80(14) . . ?
O11 Na5 C5 85.14(9) 7_566 . ?
O2 Na5 C5 169.05(11) 3 . ?
O4 Na5 C5 90.25(9) . . ?
O8 Na5 C5 104.95(8) 4 . ?
O15 Na5 C5 27.20(14) 7_556 . ?
O10 Na5 C5 102.18(9) 3_545 . ?
O13 Na5 C5 26.16(12) 7_556 . ?
O14 Na5 Zn1 42.98(15) . . ?
O11 Na5 Zn1 117.43(10) 7_566 . ?
O2 Na5 Zn1 111.74(10) 3 . ?
O4 Na5 Zn1 40.21(7) . . ?
O8 Na5 Zn1 62.69(8) 4 . ?
O15 Na5 Zn1 42.26(13) 7_556 . ?
O10 Na5 Zn1 115.25(9) 3_545 . ?
O13 Na5 Zn1 67.23(12) 7_556 . ?
C5 Na5 Zn1 60.08(3) . . ?
O14 Na5 Zn3 113.18(16) . 3 ?
O11 Na5 Zn3 137.70(10) 7_566 3 ?
O2 Na5 Zn3 40.07(8) 3 3 ?
O4 Na5 Zn3 61.26(8) . 3 ?
O8 Na5 Zn3 103.53(8) 4 3 ?
O15 Na5 Zn3 139.34(15) 7_556 3 ?
O10 Na5 Zn3 41.51(7) 3_545 3 ?
O13 Na5 Zn3 106.43(13) 7_556 3 ?
C5 Na5 Zn3 131.31(6) . 3 ?
Zn1 Na5 Zn3 101.44(5) . 3 ?
O14 Na5 Zn2 132.45(17) . 4 ?
O11 Na5 Zn2 65.91(9) 7_566 4 ?
O2 Na5 Zn2 56.32(8) 3 4 ?
O4 Na5 Zn2 97.71(9) . 4 ?
O8 Na5 Zn2 33.67(7) 4 4 ?
O15 Na5 Zn2 104.79(15) 7_556 4 ?
O10 Na5 Zn2 128.58(9) 3_545 4 ?
O13 Na5 Zn2 154.70(13) 7_556 4 ?
C5 Na5 Zn2 129.06(6) . 4 ?
Zn1 Na5 Zn2 96.25(5) . 4 ?
Zn3 Na5 Zn2 95.30(4) 3 4 ?
Zn3 F1 Zn3 148.7(2) 2 . ?
Zn3 F1 Na1 95.20(5) 2 . ?
Zn3 F1 Na1 98.78(5) . . ?
Zn3 F1 Na1 98.78(5) 2 2 ?
Zn3 F1 Na1 95.20(5) . 2 ?
Na1 F1 Na1 126.37(18) . 2 ?
O14 C5 O14 180.00(17) 7_556 . ?
O14 C5 O13 126.2(3) 7_556 7_556 ?
O14 C5 O13 53.8(3) . 7_556 ?
O14 C5 O13 53.8(3) 7_556 . ?
O14 C5 O13 126.2(3) . . ?
O13 C5 O13 180.0(5) 7_556 . ?
O14 C5 O15 61.8(4) 7_556 . ?
O14 C5 O15 118.2(4) . . ?
O13 C5 O15 65.5(4) 7_556 . ?
O13 C5 O15 114.5(4) . . ?
O14 C5 O15 118.2(4) 7_556 7_556 ?
O14 C5 O15 61.8(4) . 7_556 ?
O13 C5 O15 114.5(4) 7_556 7_556 ?
O13 C5 O15 65.5(4) . 7_556 ?
O15 C5 O15 180.0(4) . 7_556 ?
O14 C5 Na3 121.0(3) 7_556 . ?
O14 C5 Na3 59.0(3) . . ?
O13 C5 Na3 53.5(3) 7_556 . ?
O13 C5 Na3 126.5(3) . . ?
O15 C5 Na3 77.3(3) . . ?
O15 C5 Na3 102.7(3) 7_556 . ?
O14 C5 Na3 59.0(3) 7_556 7_556 ?
O14 C5 Na3 121.0(3) . 7_556 ?
O13 C5 Na3 126.5(3) 7_556 7_556 ?
O13 C5 Na3 53.5(3) . 7_556 ?
O15 C5 Na3 102.7(3) . 7_556 ?
O15 C5 Na3 77.3(3) 7_556 7_556 ?
Na3 C5 Na3 180.0 . 7_556 ?
O14 C5 Na5 44.2(3) 7_556 7_556 ?
O14 C5 Na5 135.8(3) . 7_556 ?
O13 C5 Na5 115.2(3) 7_556 7_556 ?
O13 C5 Na5 64.8(3) . 7_556 ?
O15 C5 Na5 61.7(3) . 7_556 ?
O15 C5 Na5 118.3(3) 7_556 7_556 ?
Na3 C5 Na5 80.12(5) . 7_556 ?
Na3 C5 Na5 99.88(5) 7_556 7_556 ?
O14 C5 Na5 135.8(3) 7_556 . ?
O14 C5 Na5 44.2(3) . . ?
O13 C5 Na5 64.8(3) 7_556 . ?
O13 C5 Na5 115.2(3) . . ?
O15 C5 Na5 118.3(3) . . ?
O15 C5 Na5 61.7(3) 7_556 . ?
Na3 C5 Na5 99.88(5) . . ?
Na3 C5 Na5 80.12(5) 7_556 . ?
Na5 C5 Na5 180.0 7_556 . ?
O11 C4 O10 122.9(4) . . ?
O11 C4 O12 122.6(4) . . ?
O10 C4 O12 114.5(4) . . ?
O11 C4 Na4 151.2(3) . . ?
O10 C4 Na4 52.2(2) . . ?
O12 C4 Na4 70.6(2) . . ?
O11 C4 Na4 145.4(3) . 5_566 ?
O10 C4 Na4 68.9(2) . 5_566 ?
O12 C4 Na4 57.8(2) . 5_566 ?
Na4 C4 Na4 63.22(10) . 5_566 ?
C2 O5 Zn3 116.5(3) . 3 ?
C2 O5 Na2 126.2(3) . 3_545 ?
Zn3 O5 Na2 109.63(13) 3 3_545 ?
C2 O5 Na4 116.9(3) . 3_545 ?
Zn3 O5 Na4 84.33(10) 3 3_545 ?
Na2 O5 Na4 92.98(10) 3_545 3_545 ?
C2 O6 Zn2 115.0(3) . 4_545 ?
C2 O6 Na1 123.3(3) . . ?
Zn2 O6 Na1 112.88(13) 4_545 . ?
C2 O6 Na3 117.5(2) . . ?
Zn2 O6 Na3 85.54(11) 4_545 . ?
Na1 O6 Na3 94.50(11) . . ?
C1 O2 Zn3 119.3(3) . . ?
C1 O2 Na5 132.7(3) . 3_445 ?
Zn3 O2 Na5 93.32(13) . 3_445 ?
C1 O2 Na1 115.8(3) . 2 ?
Zn3 O2 Na1 90.67(11) . 2 ?
Na5 O2 Na1 95.29(11) 3_445 2 ?
C3 O8 Zn2 119.7(3) . . ?
C3 O8 Na5 118.4(3) . 4_545 ?
Zn2 O8 Na5 101.06(12) . 4_545 ?
C3 O8 Na1 129.8(3) . . ?
Zn2 O8 Na1 92.47(11) . . ?
Na5 O8 Na1 87.89(10) 4_545 . ?
C3 O7 Zn3 118.3(3) . 4 ?
C3 O7 Na3 127.1(3) . 4 ?
Zn3 O7 Na3 104.88(13) 4 4 ?
C3 O7 Na1 118.9(3) . 4 ?
Zn3 O7 Na1 88.89(11) 4 4 ?
Na3 O7 Na1 89.29(11) 4 4 ?
C1 O3 Zn2 117.8(3) . 2 ?
C1 O3 Na4 132.3(3) . . ?
Zn2 O3 Na4 101.11(14) 2 . ?
C1 O3 Na2 110.3(3) . . ?
Zn2 O3 Na2 86.05(11) 2 . ?
Na4 O3 Na2 98.36(13) . . ?
Zn1 F2 Zn2 143.37(13) . . ?
Zn1 F2 Na2 96.09(9) . . ?
Zn2 F2 Na2 97.92(10) . . ?
Zn1 F2 Na1 95.57(10) . . ?
Zn2 F2 Na1 97.89(10) . . ?
Na2 F2 Na1 135.23(13) . . ?
C4 O12 Zn2 121.8(3) . 6_566 ?
C4 O12 Na3 118.3(3) . 7_556 ?
Zn2 O12 Na3 90.03(11) 6_566 7_556 ?
C4 O12 Na4 97.4(2) . 5_566 ?
Zn2 O12 Na4 89.14(11) 6_566 5_566 ?
Na3 O12 Na4 137.87(15) 7_556 5_566 ?
C4 O12 Na4 83.0(2) . . ?
Zn2 O12 Na4 150.87(14) 6_566 . ?
Na3 O12 Na4 90.63(11) 7_556 . ?
Na4 O12 Na4 71.23(10) 5_566 . ?
C2 O4 Zn1 117.8(3) . . ?
C2 O4 Na5 116.9(3) . . ?
Zn1 O4 Na5 86.53(11) . . ?
C2 O4 Na1 124.4(3) . 4 ?
Zn1 O4 Na1 110.03(13) . 4 ?
Na5 O4 Na1 91.65(11) . 4 ?
C1 O1 Zn1 116.1(3) . . ?
C1 O1 Na3 130.1(3) . . ?
Zn1 O1 Na3 99.60(13) . . ?
C1 O1 Na1 115.4(3) . . ?
Zn1 O1 Na1 90.65(11) . . ?
Na3 O1 Na1 96.71(11) . . ?
C4 O11 Na5 127.7(2) . 7_566 ?
C4 O11 Na3 121.5(2) . 1_565 ?
Na5 O11 Na3 110.14(14) 7_566 1_565 ?
C4 O10 Zn3 118.9(3) . 1_565 ?
C4 O10 Na4 101.8(3) . . ?
Zn3 O10 Na4 98.02(12) 1_565 . ?
C4 O10 Na5 111.0(3) . 3_455 ?
Zn3 O10 Na5 83.43(11) 1_565 3_455 ?
Na4 O10 Na5 141.60(14) . 3_455 ?
C4 O10 Na4 86.2(2) . 5_566 ?
Zn3 O10 Na4 154.80(14) 1_565 5_566 ?
Na4 O10 Na4 73.10(10) . 5_566 ?
Na5 O10 Na4 89.36(10) 3_455 5_566 ?
C3 O9 Zn1 120.1(3) . 4_545 ?
C3 O9 Na2 130.2(3) . 3_545 ?
Zn1 O9 Na2 92.04(14) 4_545 3_545 ?
C3 O9 Na4 116.5(3) . 4_545 ?
Zn1 O9 Na4 94.22(15) 4_545 4_545 ?
Na2 O9 Na4 95.67(11) 3_545 4_545 ?
O1 C1 O3 119.9(4) . . ?
O1 C1 O2 120.3(4) . . ?
O3 C1 O2 119.8(4) . . ?
O7 C3 O9 120.0(4) . . ?
O7 C3 O8 120.0(4) . . ?
O9 C3 O8 120.0(4) . . ?
O5 C2 O6 120.4(4) . . ?
O5 C2 O4 119.5(4) . . ?
O6 C2 O4 120.1(4) . . ?
C5 O13 Na4 136.2(4) . . ?
C5 O13 Na3 100.8(3) . 7_556 ?
Na4 O13 Na3 104.1(2) . 7_556 ?
C5 O13 Na5 89.0(3) . 7_556 ?
Na4 O13 Na5 104.7(2) . 7_556 ?
Na3 O13 Na5 125.2(2) 7_556 7_556 ?
C5 O15 Zn1 121.1(4) . 7_556 ?
C5 O15 Na4 114.8(3) . 7_556 ?
Zn1 O15 Na4 97.3(2) 7_556 7_556 ?
C5 O15 Na5 91.1(3) . 7_556 ?
Zn1 O15 Na5 82.4(2) 7_556 7_556 ?
Na4 O15 Na5 148.8(3) 7_556 7_556 ?
C5 O15 Na3 76.3(3) . . ?
Zn1 O15 Na3 159.0(3) 7_556 . ?
Na4 O15 Na3 83.93(19) 7_556 . ?
Na5 O15 Na3 85.88(17) 7_556 . ?
C5 O14 Zn1 127.0(4) . . ?
C5 O14 Na5 113.0(3) . . ?
Zn1 O14 Na5 91.5(2) . . ?
C5 O14 Na3 96.3(3) . . ?
Zn1 O14 Na3 89.6(2) . . ?
Na5 O14 Na3 141.8(3) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O9 Zn1 Na1 F1 -69.49(17) 4 . . . ?
O4 Zn1 Na1 F1 168.25(12) . . . . ?
O1 Zn1 Na1 F1 31.80(12) . . . . ?
F2 Zn1 Na1 F1 -89.68(13) . . . . ?
O15 Zn1 Na1 F1 61.8(3) 7_556 . . . ?
O14 Zn1 Na1 F1 94.19(19) . . . . ?
Na5 Zn1 Na1 F1 146.15(8) . . . . ?
Na2 Zn1 Na1 F1 -60.14(8) . . . . ?
Na3 Zn1 Na1 F1 79.36(9) . . . . ?
Na4 Zn1 Na1 F1 -1.04(11) . . . . ?
O9 Zn1 Na1 F2 20.19(17) 4 . . . ?
O4 Zn1 Na1 F2 -102.06(13) . . . . ?
O1 Zn1 Na1 F2 121.48(15) . . . . ?
O15 Zn1 Na1 F2 151.5(3) 7_556 . . . ?
O14 Zn1 Na1 F2 -176.13(19) . . . . ?
Na5 Zn1 Na1 F2 -124.16(11) . . . . ?
Na2 Zn1 Na1 F2 29.55(10) . . . . ?
Na3 Zn1 Na1 F2 169.05(11) . . . . ?
Na4 Zn1 Na1 F2 88.64(11) . . . . ?
O9 Zn1 Na1 O6 159.21(17) 4 . . . ?
O4 Zn1 Na1 O6 36.95(12) . . . . ?
O1 Zn1 Na1 O6 -99.50(13) . . . . ?
F2 Zn1 Na1 O6 139.02(13) . . . . ?
O15 Zn1 Na1 O6 -69.5(3) 7_556 . . . ?
O14 Zn1 Na1 O6 -37.11(19) . . . . ?
Na5 Zn1 Na1 O6 14.85(10) . . . . ?
Na2 Zn1 Na1 O6 168.56(8) . . . . ?
Na3 Zn1 Na1 O6 -51.94(8) . . . . ?
Na4 Zn1 Na1 O6 -132.34(9) . . . . ?
O9 Zn1 Na1 O4 118.7(3) 4 . . 4_545 ?
O4 Zn1 Na1 O4 -3.6(3) . . . 4_545 ?
O1 Zn1 Na1 O4 -140.0(3) . . . 4_545 ?
F2 Zn1 Na1 O4 98.5(3) . . . 4_545 ?
O15 Zn1 Na1 O4 -110.0(4) 7_556 . . 4_545 ?
O14 Zn1 Na1 O4 -77.6(3) . . . 4_545 ?
Na5 Zn1 Na1 O4 -25.7(3) . . . 4_545 ?
Na2 Zn1 Na1 O4 128.0(2) . . . 4_545 ?
Na3 Zn1 Na1 O4 -92.5(2) . . . 4_545 ?
Na4 Zn1 Na1 O4 -172.9(2) . . . 4_545 ?
O9 Zn1 Na1 O2 4.60(18) 4 . . 2 ?
O4 Zn1 Na1 O2 -117.66(13) . . . 2 ?
O1 Zn1 Na1 O2 105.89(14) . . . 2 ?
F2 Zn1 Na1 O2 -15.60(12) . . . 2 ?
O15 Zn1 Na1 O2 135.9(3) 7_556 . . 2 ?
O14 Zn1 Na1 O2 168.28(19) . . . 2 ?
Na5 Zn1 Na1 O2 -139.76(9) . . . 2 ?
Na2 Zn1 Na1 O2 13.95(9) . . . 2 ?
Na3 Zn1 Na1 O2 153.45(10) . . . 2 ?
Na4 Zn1 Na1 O2 73.05(11) . . . 2 ?
O9 Zn1 Na1 O1 -101.29(17) 4 . . . ?
O4 Zn1 Na1 O1 136.45(14) . . . . ?
F2 Zn1 Na1 O1 -121.48(15) . . . . ?
O15 Zn1 Na1 O1 30.0(3) 7_556 . . . ?
O14 Zn1 Na1 O1 62.4(2) . . . . ?
Na5 Zn1 Na1 O1 114.35(12) . . . . ?
Na2 Zn1 Na1 O1 -91.94(11) . . . . ?
Na3 Zn1 Na1 O1 47.56(11) . . . . ?
Na4 Zn1 Na1 O1 -32.84(12) . . . . ?
O9 Zn1 Na1 O8 72.18(16) 4 . . . ?
O4 Zn1 Na1 O8 -50.07(11) . . . . ?
O1 Zn1 Na1 O8 173.47(13) . . . . ?
F2 Zn1 Na1 O8 51.99(12) . . . . ?
O15 Zn1 Na1 O8 -156.5(3) 7_556 . . . ?
O14 Zn1 Na1 O8 -124.14(18) . . . . ?
Na5 Zn1 Na1 O8 -72.18(9) . . . . ?
Na2 Zn1 Na1 O8 81.54(8) . . . . ?
Na3 Zn1 Na1 O8 -138.96(9) . . . . ?
Na4 Zn1 Na1 O8 140.63(8) . . . . ?
O9 Zn1 Na1 O7 -138.23(15) 4 . . 4_545 ?
O4 Zn1 Na1 O7 99.51(12) . . . 4_545 ?
O1 Zn1 Na1 O7 -36.94(13) . . . 4_545 ?
F2 Zn1 Na1 O7 -158.43(13) . . . 4_545 ?
O15 Zn1 Na1 O7 -6.9(3) 7_556 . . 4_545 ?
O14 Zn1 Na1 O7 25.45(19) . . . 4_545 ?
Na5 Zn1 Na1 O7 77.41(9) . . . 4_545 ?
Na2 Zn1 Na1 O7 -128.88(8) . . . 4_545 ?
Na3 Zn1 Na1 O7 10.62(7) . . . 4_545 ?
Na4 Zn1 Na1 O7 -69.78(10) . . . 4_545 ?
O9 Zn1 Na1 Zn3 -33.33(18) 4 . . 2 ?
O4 Zn1 Na1 Zn3 -155.59(13) . . . 2 ?
O1 Zn1 Na1 Zn3 67.96(13) . . . 2 ?
F2 Zn1 Na1 Zn3 -53.53(12) . . . 2 ?
O15 Zn1 Na1 Zn3 98.0(3) 7_556 . . 2 ?
O14 Zn1 Na1 Zn3 130.35(19) . . . 2 ?
Na5 Zn1 Na1 Zn3 -177.69(8) . . . 2 ?
Na2 Zn1 Na1 Zn3 -23.98(9) . . . 2 ?
Na3 Zn1 Na1 Zn3 115.52(10) . . . 2 ?
Na4 Zn1 Na1 Zn3 35.12(12) . . . 2 ?
O9 Zn1 Na1 Zn2 41.14(14) 4 . . . ?
O4 Zn1 Na1 Zn2 -81.12(9) . . . . ?
O1 Zn1 Na1 Zn2 142.43(11) . . . . ?
F2 Zn1 Na1 Zn2 20.95(9) . . . . ?
O15 Zn1 Na1 Zn2 172.4(3) 7_556 . . . ?
O14 Zn1 Na1 Zn2 -155.18(17) . . . . ?
Na5 Zn1 Na1 Zn2 -103.22(6) . . . . ?
Na2 Zn1 Na1 Zn2 50.49(3) . . . . ?
Na3 Zn1 Na1 Zn2 -170.01(5) . . . . ?
Na4 Zn1 Na1 Zn2 109.59(6) . . . . ?
O9 Zn1 Na1 Zn3 -101.91(14) 4 . . . ?
O4 Zn1 Na1 Zn3 135.84(10) . . . . ?
O1 Zn1 Na1 Zn3 -0.62(10) . . . . ?
F2 Zn1 Na1 Zn3 -122.10(11) . . . . ?
O15 Zn1 Na1 Zn3 29.4(3) 7_556 . . . ?
O14 Zn1 Na1 Zn3 61.77(17) . . . . ?
Na5 Zn1 Na1 Zn3 113.73(6) . . . . ?
Na2 Zn1 Na1 Zn3 -92.56(4) . . . . ?
Na3 Zn1 Na1 Zn3 46.95(4) . . . . ?
Na4 Zn1 Na1 Zn3 -33.46(7) . . . . ?
O8 Zn2 Na1 F1 -129.98(14) . . . . ?
O3 Zn2 Na1 F1 3.49(12) 2 . . . ?
O6 Zn2 Na1 F1 135.13(12) 4 . . . ?
F2 Zn2 Na1 F1 88.81(14) . . . . ?
O12 Zn2 Na1 F1 -72.13(17) 6_565 . . . ?
Na3 Zn2 Na1 F1 -149.68(8) 4 . . . ?
Na2 Zn2 Na1 F1 60.51(8) . . . . ?
Na4 Zn2 Na1 F1 2.01(11) 2 . . . ?
Na5 Zn2 Na1 F1 -76.96(8) 4_545 . . . ?
O8 Zn2 Na1 F2 141.20(15) . . . . ?
O3 Zn2 Na1 F2 -85.32(14) 2 . . . ?
O6 Zn2 Na1 F2 46.32(15) 4 . . . ?
O12 Zn2 Na1 F2 -160.94(17) 6_565 . . . ?
Na3 Zn2 Na1 F2 121.51(12) 4 . . . ?
Na2 Zn2 Na1 F2 -28.30(10) . . . . ?
Na4 Zn2 Na1 F2 -86.81(11) 2 . . . ?
Na5 Zn2 Na1 F2 -165.77(11) 4_545 . . . ?
O8 Zn2 Na1 O6 67.92(13) . . . . ?
O3 Zn2 Na1 O6 -158.60(13) 2 . . . ?
O6 Zn2 Na1 O6 -26.96(16) 4 . . . ?
F2 Zn2 Na1 O6 -73.28(13) . . . . ?
O12 Zn2 Na1 O6 125.78(15) 6_565 . . . ?
Na3 Zn2 Na1 O6 48.22(11) 4 . . . ?
Na2 Zn2 Na1 O6 -101.59(9) . . . . ?
Na4 Zn2 Na1 O6 -160.09(8) 2 . . . ?
Na5 Zn2 Na1 O6 120.95(9) 4_545 . . . ?
O8 Zn2 Na1 O4 -36.65(13) . . . 4_545 ?
O3 Zn2 Na1 O4 96.83(12) 2 . . 4_545 ?
O6 Zn2 Na1 O4 -131.54(13) 4 . . 4_545 ?
F2 Zn2 Na1 O4 -177.86(14) . . . 4_545 ?
O12 Zn2 Na1 O4 21.20(17) 6_565 . . 4_545 ?
Na3 Zn2 Na1 O4 -56.35(11) 4 . . 4_545 ?
Na2 Zn2 Na1 O4 153.84(9) . . . 4_545 ?
Na4 Zn2 Na1 O4 95.34(10) 2 . . 4_545 ?
Na5 Zn2 Na1 O4 16.37(8) 4_545 . . 4_545 ?
O8 Zn2 Na1 O2 -98.77(13) . . . 2 ?
O3 Zn2 Na1 O2 34.71(12) 2 . . 2 ?
O6 Zn2 Na1 O2 166.34(13) 4 . . 2 ?
F2 Zn2 Na1 O2 120.02(13) . . . 2 ?
O12 Zn2 Na1 O2 -40.92(16) 6_565 . . 2 ?
Na3 Zn2 Na1 O2 -118.47(9) 4 . . 2 ?
Na2 Zn2 Na1 O2 91.72(8) . . . 2 ?
Na4 Zn2 Na1 O2 33.22(10) 2 . . 2 ?
Na5 Zn2 Na1 O2 -45.75(8) 4_545 . . 2 ?
O8 Zn2 Na1 O1 142.17(13) . . . . ?
O3 Zn2 Na1 O1 -84.35(12) 2 . . . ?
O6 Zn2 Na1 O1 47.29(13) 4 . . . ?
F2 Zn2 Na1 O1 0.97(12) . . . . ?
O12 Zn2 Na1 O1 -159.98(15) 6_565 . . . ?
Na3 Zn2 Na1 O1 122.47(9) 4 . . . ?
Na2 Zn2 Na1 O1 -27.34(8) . . . . ?
Na4 Zn2 Na1 O1 -85.84(9) 2 . . . ?
Na5 Zn2 Na1 O1 -164.80(9) 4_545 . . . ?
O3 Zn2 Na1 O8 133.48(14) 2 . . . ?
O6 Zn2 Na1 O8 -94.88(15) 4 . . . ?
F2 Zn2 Na1 O8 -141.20(15) . . . . ?
O12 Zn2 Na1 O8 57.85(18) 6_565 . . . ?
Na3 Zn2 Na1 O8 -19.70(13) 4 . . . ?
Na2 Zn2 Na1 O8 -169.51(11) . . . . ?
Na4 Zn2 Na1 O8 131.99(11) 2 . . . ?
Na5 Zn2 Na1 O8 53.03(11) 4_545 . . . ?
O8 Zn2 Na1 O7 122.7(5) . . . 4_545 ?
O3 Zn2 Na1 O7 -103.8(4) 2 . . 4_545 ?
O6 Zn2 Na1 O7 27.8(5) 4 . . 4_545 ?
F2 Zn2 Na1 O7 -18.5(4) . . . 4_545 ?
O12 Zn2 Na1 O7 -179.4(4) 6_565 . . 4_545 ?
Na3 Zn2 Na1 O7 103.0(4) 4 . . 4_545 ?
Na2 Zn2 Na1 O7 -46.8(4) . . . 4_545 ?
Na4 Zn2 Na1 O7 -105.3(4) 2 . . 4_545 ?
Na5 Zn2 Na1 O7 175.7(4) 4_545 . . 4_545 ?
O8 Zn2 Na1 Zn3 -95.92(11) . . . 2 ?
O3 Zn2 Na1 Zn3 37.56(10) 2 . . 2 ?
O6 Zn2 Na1 Zn3 169.19(10) 4 . . 2 ?
F2 Zn2 Na1 Zn3 122.87(11) . . . 2 ?
O12 Zn2 Na1 Zn3 -38.07(15) 6_565 . . 2 ?
Na3 Zn2 Na1 Zn3 -115.62(6) 4 . . 2 ?
Na2 Zn2 Na1 Zn3 94.57(4) . . . 2 ?
Na4 Zn2 Na1 Zn3 36.07(7) 2 . . 2 ?
Na5 Zn2 Na1 Zn3 -42.90(4) 4_545 . . 2 ?
O8 Zn2 Na1 Zn1 119.78(11) . . . . ?
O3 Zn2 Na1 Zn1 -106.75(10) 2 . . . ?
O6 Zn2 Na1 Zn1 24.89(11) 4 . . . ?
F2 Zn2 Na1 Zn1 -21.43(10) . . . . ?
O12 Zn2 Na1 Zn1 177.63(14) 6_565 . . . ?
Na3 Zn2 Na1 Zn1 100.08(7) 4 . . . ?
Na2 Zn2 Na1 Zn1 -49.73(3) . . . . ?
Na4 Zn2 Na1 Zn1 -108.23(6) 2 . . . ?
Na5 Zn2 Na1 Zn1 172.80(5) 4_545 . . . ?
O8 Zn2 Na1 Zn3 -164.74(15) . . . . ?
O3 Zn2 Na1 Zn3 -31.26(12) 2 . . . ?
O6 Zn2 Na1 Zn3 100.38(13) 4 . . . ?
F2 Zn2 Na1 Zn3 54.06(12) . . . . ?
O12 Zn2 Na1 Zn3 -106.88(16) 6_565 . . . ?
Na3 Zn2 Na1 Zn3 175.57(7) 4 . . . ?
Na2 Zn2 Na1 Zn3 25.75(8) . . . . ?
Na4 Zn2 Na1 Zn3 -32.75(12) 2 . . . ?
Na5 Zn2 Na1 Zn3 -111.71(10) 4_545 . . . ?
O7 Zn3 Na1 F1 141.22(17) 4_545 . . . ?
O2 Zn3 Na1 F1 -87.57(16) . . . . ?
O5 Zn3 Na1 F1 38.32(17) 3_445 . . . ?
O10 Zn3 Na1 F1 -168.2(2) 1_545 . . . ?
Na5 Zn3 Na1 F1 -86.48(14) 3_445 . . . ?
Na1 Zn3 Na1 F1 -35.50(14) 2 . . . ?
Na4 Zn3 Na1 F1 120.71(14) 1_545 . . . ?
Na3 Zn3 Na1 F1 -171.02(14) . . . . ?
Na2 Zn3 Na1 F1 59.87(13) 1_545 . . . ?
O7 Zn3 Na1 F2 -127.52(14) 4_545 . . . ?
O2 Zn3 Na1 F2 3.69(11) . . . . ?
O5 Zn3 Na1 F2 129.58(13) 3_445 . . . ?
F1 Zn3 Na1 F2 91.26(16) . . . . ?
O10 Zn3 Na1 F2 -76.95(18) 1_545 . . . ?
Na5 Zn3 Na1 F2 4.78(11) 3_445 . . . ?
Na1 Zn3 Na1 F2 55.76(8) 2 . . . ?
Na4 Zn3 Na1 F2 -148.03(9) 1_545 . . . ?
Na3 Zn3 Na1 F2 -79.76(9) . . . . ?
Na2 Zn3 Na1 F2 151.13(8) 1_545 . . . ?
O7 Zn3 Na1 O6 -31.85(13) 4_545 . . . ?
O2 Zn3 Na1 O6 99.35(12) . . . . ?
O5 Zn3 Na1 O6 -134.75(13) 3_445 . . . ?
F1 Zn3 Na1 O6 -173.07(16) . . . . ?
O10 Zn3 Na1 O6 18.72(19) 1_545 . . . ?
Na5 Zn3 Na1 O6 100.45(10) 3_445 . . . ?
Na1 Zn3 Na1 O6 151.42(8) 2 . . . ?
Na4 Zn3 Na1 O6 -52.37(12) 1_545 . . . ?
Na3 Zn3 Na1 O6 15.91(9) . . . . ?
Na2 Zn3 Na1 O6 -113.20(9) 1_545 . . . ?
O7 Zn3 Na1 O4 71.95(14) 4_545 . . 4_545 ?
O2 Zn3 Na1 O4 -156.85(12) . . . 4_545 ?
O5 Zn3 Na1 O4 -30.95(15) 3_445 . . 4_545 ?
F1 Zn3 Na1 O4 -69.27(15) . . . 4_545 ?
O10 Zn3 Na1 O4 122.52(17) 1_545 . . 4_545 ?
Na5 Zn3 Na1 O4 -155.75(8) 3_445 . . 4_545 ?
Na1 Zn3 Na1 O4 -104.78(10) 2 . . 4_545 ?
Na4 Zn3 Na1 O4 51.43(11) 1_545 . . 4_545 ?
Na3 Zn3 Na1 O4 119.71(9) . . . 4_545 ?
Na2 Zn3 Na1 O4 -9.40(8) 1_545 . . 4_545 ?
O7 Zn3 Na1 O2 147.80(14) 4_545 . . 2 ?
O2 Zn3 Na1 O2 -80.99(11) . . . 2 ?
O5 Zn3 Na1 O2 44.91(14) 3_445 . . 2 ?
F1 Zn3 Na1 O2 6.58(14) . . . 2 ?
O10 Zn3 Na1 O2 -161.63(17) 1_545 . . 2 ?
Na5 Zn3 Na1 O2 -79.89(9) 3_445 . . 2 ?
Na1 Zn3 Na1 O2 -28.92(10) 2 . . 2 ?
Na4 Zn3 Na1 O2 127.29(9) 1_545 . . 2 ?
Na3 Zn3 Na1 O2 -164.44(10) . . . 2 ?
Na2 Zn3 Na1 O2 66.46(9) 1_545 . . 2 ?
O7 Zn3 Na1 O1 -93.07(14) 4_545 . . . ?
O2 Zn3 Na1 O1 38.14(11) . . . . ?
O5 Zn3 Na1 O1 164.04(13) 3_445 . . . ?
F1 Zn3 Na1 O1 125.71(16) . . . . ?
O10 Zn3 Na1 O1 -42.49(18) 1_545 . . . ?
Na5 Zn3 Na1 O1 39.24(10) 3_445 . . . ?
Na1 Zn3 Na1 O1 90.21(8) 2 . . . ?
Na4 Zn3 Na1 O1 -113.58(10) 1_545 . . . ?
Na3 Zn3 Na1 O1 -45.30(8) . . . . ?
Na2 Zn3 Na1 O1 -174.41(8) 1_545 . . . ?
O7 Zn3 Na1 O8 126.5(6) 4_545 . . . ?
O2 Zn3 Na1 O8 -102.3(6) . . . . ?
O5 Zn3 Na1 O8 23.6(6) 3_445 . . . ?
F1 Zn3 Na1 O8 -14.7(6) . . . . ?
O10 Zn3 Na1 O8 177.1(6) 1_545 . . . ?
Na5 Zn3 Na1 O8 -101.2(6) 3_445 . . . ?
Na1 Zn3 Na1 O8 -50.2(6) 2 . . . ?
Na4 Zn3 Na1 O8 106.0(6) 1_545 . . . ?
Na3 Zn3 Na1 O8 174.3(6) . . . . ?
Na2 Zn3 Na1 O8 45.2(6) 1_545 . . . ?
O2 Zn3 Na1 O7 131.21(14) . . . 4_545 ?
O5 Zn3 Na1 O7 -102.90(15) 3_445 . . 4_545 ?
F1 Zn3 Na1 O7 -141.22(17) . . . 4_545 ?
O10 Zn3 Na1 O7 50.6(2) 1_545 . . 4_545 ?
Na5 Zn3 Na1 O7 132.30(12) 3_445 . . 4_545 ?
Na1 Zn3 Na1 O7 -176.73(11) 2 . . 4_545 ?
Na4 Zn3 Na1 O7 -20.51(13) 1_545 . . 4_545 ?
Na3 Zn3 Na1 O7 47.76(11) . . . 4_545 ?
Na2 Zn3 Na1 O7 -81.35(11) 1_545 . . 4_545 ?
O7 Zn3 Na1 Zn3 123.42(12) 4_545 . . 2 ?
O2 Zn3 Na1 Zn3 -105.37(9) . . . 2 ?
O5 Zn3 Na1 Zn3 20.53(12) 3_445 . . 2 ?
F1 Zn3 Na1 Zn3 -17.80(13) . . . 2 ?
O10 Zn3 Na1 Zn3 173.99(15) 1_545 . . 2 ?
Na5 Zn3 Na1 Zn3 -104.27(5) 3_445 . . 2 ?
Na1 Zn3 Na1 Zn3 -53.30(5) 2 . . 2 ?
Na4 Zn3 Na1 Zn3 102.91(6) 1_545 . . 2 ?
Na3 Zn3 Na1 Zn3 171.18(5) . . . 2 ?
Na2 Zn3 Na1 Zn3 42.08(3) 1_545 . . 2 ?
O7 Zn3 Na1 Zn1 -92.62(11) 4_545 . . . ?
O2 Zn3 Na1 Zn1 38.58(9) . . . . ?
O5 Zn3 Na1 Zn1 164.48(11) 3_445 . . . ?
F1 Zn3 Na1 Zn1 126.16(14) . . . . ?
O10 Zn3 Na1 Zn1 -42.05(17) 1_545 . . . ?
Na5 Zn3 Na1 Zn1 39.68(7) 3_445 . . . ?
Na1 Zn3 Na1 Zn1 90.65(3) 2 . . . ?
Na4 Zn3 Na1 Zn1 -113.13(7) 1_545 . . . ?
Na3 Zn3 Na1 Zn1 -44.86(4) . . . . ?
Na2 Zn3 Na1 Zn1 -173.97(4) 1_545 . . . ?
O7 Zn3 Na1 Zn2 -159.87(15) 4_545 . . . ?
O2 Zn3 Na1 Zn2 -28.66(11) . . . . ?
O5 Zn3 Na1 Zn2 97.24(14) 3_445 . . . ?
F1 Zn3 Na1 Zn2 58.91(15) . . . . ?
O10 Zn3 Na1 Zn2 -109.30(17) 1_545 . . . ?
Na5 Zn3 Na1 Zn2 -27.56(11) 3_445 . . . ?
Na1 Zn3 Na1 Zn2 23.41(9) 2 . . . ?
Na4 Zn3 Na1 Zn2 179.62(7) 1_545 . . . ?
Na3 Zn3 Na1 Zn2 -112.11(9) . . . . ?
Na2 Zn3 Na1 Zn2 118.79(8) 1_545 . . . ?
O9 Zn1 Na2 F2 -132.44(15) 4 . . 2 ?
O4 Zn1 Na2 F2 130.59(12) . . . 2 ?
O1 Zn1 Na2 F2 4.58(11) . . . 2 ?
F2 Zn1 Na2 F2 86.20(16) . . . 2 ?
O15 Zn1 Na2 F2 -89.39(19) 7_556 . . 2 ?
O14 Zn1 Na2 F2 -74.6(3) . . . 2 ?
Na5 Zn1 Na2 F2 -153.42(8) . . . 2 ?
Na3 Zn1 Na2 F2 3.71(9) . . . 2 ?
Na1 Zn1 Na2 F2 56.24(8) . . . 2 ?
Na4 Zn1 Na2 F2 -77.51(7) . . . 2 ?
O9 Zn1 Na2 F2 141.36(17) 4 . . . ?
O4 Zn1 Na2 F2 44.39(16) . . . . ?
O1 Zn1 Na2 F2 -81.62(13) . . . . ?
O15 Zn1 Na2 F2 -175.6(2) 7_556 . . . ?
O14 Zn1 Na2 F2 -160.8(3) . . . . ?
Na5 Zn1 Na2 F2 120.38(12) . . . . ?
Na3 Zn1 Na2 F2 -82.49(10) . . . . ?
Na1 Zn1 Na2 F2 -29.96(10) . . . . ?
Na4 Zn1 Na2 F2 -163.70(11) . . . . ?
O9 Zn1 Na2 O5 -39.50(15) 4 . . 3_455 ?
O4 Zn1 Na2 O5 -136.47(13) . . . 3_455 ?
O1 Zn1 Na2 O5 97.53(12) . . . 3_455 ?
F2 Zn1 Na2 O5 179.14(15) . . . 3_455 ?
O15 Zn1 Na2 O5 3.6(2) 7_556 . . 3_455 ?
O14 Zn1 Na2 O5 18.3(3) . . . 3_455 ?
Na5 Zn1 Na2 O5 -60.48(10) . . . 3_455 ?
Na3 Zn1 Na2 O5 96.65(11) . . . 3_455 ?
Na1 Zn1 Na2 O5 149.19(9) . . . 3_455 ?
Na4 Zn1 Na2 O5 15.44(9) . . . 3_455 ?
O9 Zn1 Na2 O5 69.77(16) 4 . . 4 ?
O4 Zn1 Na2 O5 -27.20(16) . . . 4 ?
O1 Zn1 Na2 O5 -153.21(13) . . . 4 ?
F2 Zn1 Na2 O5 -71.59(12) . . . 4 ?
O15 Zn1 Na2 O5 112.82(19) 7_556 . . 4 ?
O14 Zn1 Na2 O5 127.6(3) . . . 4 ?
Na5 Zn1 Na2 O5 48.79(11) . . . 4 ?
Na3 Zn1 Na2 O5 -154.08(9) . . . 4 ?
Na1 Zn1 Na2 O5 -101.54(10) . . . 4 ?
Na4 Zn1 Na2 O5 124.71(10) . . . 4 ?
O4 Zn1 Na2 O9 -96.97(17) . . . 4 ?
O1 Zn1 Na2 O9 137.02(15) . . . 4 ?
F2 Zn1 Na2 O9 -141.36(17) . . . 4 ?
O15 Zn1 Na2 O9 43.1(2) 7_556 . . 4 ?
O14 Zn1 Na2 O9 57.8(3) . . . 4 ?
Na5 Zn1 Na2 O9 -20.98(14) . . . 4 ?
Na3 Zn1 Na2 O9 136.15(14) . . . 4 ?
Na1 Zn1 Na2 O9 -171.31(13) . . . 4 ?
Na4 Zn1 Na2 O9 54.94(13) . . . 4 ?
O9 Zn1 Na2 O9 135.7(6) 4 . . 3_455 ?
O4 Zn1 Na2 O9 38.7(6) . . . 3_455 ?
O1 Zn1 Na2 O9 -87.3(6) . . . 3_455 ?
F2 Zn1 Na2 O9 -5.7(6) . . . 3_455 ?
O15 Zn1 Na2 O9 178.7(6) 7_556 . . 3_455 ?
O14 Zn1 Na2 O9 -166.5(6) . . . 3_455 ?
Na5 Zn1 Na2 O9 114.7(6) . . . 3_455 ?
Na3 Zn1 Na2 O9 -88.2(6) . . . 3_455 ?
Na1 Zn1 Na2 O9 -35.6(6) . . . 3_455 ?
Na4 Zn1 Na2 O9 -169.4(6) . . . 3_455 ?
O9 Zn1 Na2 O3 144.26(15) 4 . . 2 ?
O4 Zn1 Na2 O3 47.29(15) . . . 2 ?
O1 Zn1 Na2 O3 -78.71(12) . . . 2 ?
F2 Zn1 Na2 O3 2.91(11) . . . 2 ?
O15 Zn1 Na2 O3 -172.68(19) 7_556 . . 2 ?
O14 Zn1 Na2 O3 -157.9(3) . . . 2 ?
Na5 Zn1 Na2 O3 123.29(10) . . . 2 ?
Na3 Zn1 Na2 O3 -79.58(8) . . . 2 ?
Na1 Zn1 Na2 O3 -27.05(9) . . . 2 ?
Na4 Zn1 Na2 O3 -160.80(9) . . . 2 ?
O9 Zn1 Na2 O3 -98.44(15) 4 . . . ?
O4 Zn1 Na2 O3 164.59(14) . . . . ?
O1 Zn1 Na2 O3 38.58(11) . . . . ?
F2 Zn1 Na2 O3 120.20(14) . . . . ?
O15 Zn1 Na2 O3 -55.39(19) 7_556 . . . ?
O14 Zn1 Na2 O3 -40.6(3) . . . . ?
Na5 Zn1 Na2 O3 -119.42(9) . . . . ?
Na3 Zn1 Na2 O3 37.71(10) . . . . ?
Na1 Zn1 Na2 O3 90.25(9) . . . . ?
Na4 Zn1 Na2 O3 -43.50(8) . . . . ?
O9 Zn1 Na2 Zn1 -164.68(13) 4 . . 2 ?
O4 Zn1 Na2 Zn1 98.35(12) . . . 2 ?
O1 Zn1 Na2 Zn1 -27.66(8) . . . 2 ?
F2 Zn1 Na2 Zn1 53.96(10) . . . 2 ?
O15 Zn1 Na2 Zn1 -121.63(18) 7_556 . . 2 ?
O14 Zn1 Na2 Zn1 -106.9(3) . . . 2 ?
Na5 Zn1 Na2 Zn1 174.34(5) . . . 2 ?
Na3 Zn1 Na2 Zn1 -28.53(5) . . . 2 ?
Na1 Zn1 Na2 Zn1 24.01(3) . . . 2 ?
Na4 Zn1 Na2 Zn1 -109.74(4) . . . 2 ?
O9 Zn1 Na2 Zn2 120.41(14) 4 . . . ?
O4 Zn1 Na2 Zn2 23.44(13) . . . . ?
O1 Zn1 Na2 Zn2 -102.57(9) . . . . ?
F2 Zn1 Na2 Zn2 -20.95(10) . . . . ?
O15 Zn1 Na2 Zn2 163.46(17) 7_556 . . . ?
O14 Zn1 Na2 Zn2 178.2(3) . . . . ?
Na5 Zn1 Na2 Zn2 99.43(6) . . . . ?
Na3 Zn1 Na2 Zn2 -103.44(4) . . . . ?
Na1 Zn1 Na2 Zn2 -50.90(4) . . . . ?
Na4 Zn1 Na2 Zn2 175.35(5) . . . . ?
O9 Zn1 Na2 Zn2 -97.75(13) 4 . . 2 ?
O4 Zn1 Na2 Zn2 165.28(11) . . . 2 ?
O1 Zn1 Na2 Zn2 39.28(9) . . . 2 ?
F2 Zn1 Na2 Zn2 120.89(12) . . . 2 ?
O15 Zn1 Na2 Zn2 -54.69(18) 7_556 . . 2 ?
O14 Zn1 Na2 Zn2 -39.9(3) . . . 2 ?
Na5 Zn1 Na2 Zn2 -118.73(6) . . . 2 ?
Na3 Zn1 Na2 Zn2 38.40(7) . . . 2 ?
Na1 Zn1 Na2 Zn2 90.94(5) . . . 2 ?
Na4 Zn1 Na2 Zn2 -42.81(5) . . . 2 ?
O8 Zn2 Na2 F2 -66.24(13) . . . 2 ?
O3 Zn2 Na2 F2 33.94(12) 2 . . 2 ?
O6 Zn2 Na2 F2 175.15(11) 4 . . 2 ?
F2 Zn2 Na2 F2 -83.74(17) . . . 2 ?
O12 Zn2 Na2 F2 92.76(13) 6_565 . . 2 ?
Na3 Zn2 Na2 F2 152.45(8) 4 . . 2 ?
Na4 Zn2 Na2 F2 79.10(8) 2 . . 2 ?
Na1 Zn2 Na2 F2 -55.19(8) . . . 2 ?
Na5 Zn2 Na2 F2 -7.25(9) 4_545 . . 2 ?
O8 Zn2 Na2 F2 17.50(16) . . . . ?
O3 Zn2 Na2 F2 117.67(16) 2 . . . ?
O6 Zn2 Na2 F2 -101.11(13) 4 . . . ?
O12 Zn2 Na2 F2 176.50(14) 6_565 . . . ?
Na3 Zn2 Na2 F2 -123.81(11) 4 . . . ?
Na4 Zn2 Na2 F2 162.84(11) 2 . . . ?
Na1 Zn2 Na2 F2 28.55(11) . . . . ?
Na5 Zn2 Na2 F2 76.49(11) 4_545 . . . ?
O8 Zn2 Na2 O5 117.1(3) . . . 3_455 ?
O3 Zn2 Na2 O5 -142.7(3) 2 . . 3_455 ?
O6 Zn2 Na2 O5 -1.5(3) 4 . . 3_455 ?
F2 Zn2 Na2 O5 99.6(3) . . . 3_455 ?
O12 Zn2 Na2 O5 -83.9(3) 6_565 . . 3_455 ?
Na3 Zn2 Na2 O5 -24.2(3) 4 . . 3_455 ?
Na4 Zn2 Na2 O5 -97.6(3) 2 . . 3_455 ?
Na1 Zn2 Na2 O5 128.2(2) . . . 3_455 ?
Na5 Zn2 Na2 O5 176.1(2) 4_545 . . 3_455 ?
O8 Zn2 Na2 O5 155.92(15) . . . 4 ?
O3 Zn2 Na2 O5 -103.90(13) 2 . . 4 ?
O6 Zn2 Na2 O5 37.31(11) 4 . . 4 ?
F2 Zn2 Na2 O5 138.43(13) . . . 4 ?
O12 Zn2 Na2 O5 -45.07(13) 6_565 . . 4 ?
Na3 Zn2 Na2 O5 14.61(9) 4 . . 4 ?
Na4 Zn2 Na2 O5 -58.74(9) 2 . . 4 ?
Na1 Zn2 Na2 O5 166.97(9) . . . 4 ?
Na5 Zn2 Na2 O5 -145.09(9) 4_545 . . 4 ?
O8 Zn2 Na2 O9 70.30(16) . . . 4 ?
O3 Zn2 Na2 O9 170.48(15) 2 . . 4 ?
O6 Zn2 Na2 O9 -48.30(13) 4 . . 4 ?
F2 Zn2 Na2 O9 52.81(13) . . . 4 ?
O12 Zn2 Na2 O9 -130.69(13) 6_565 . . 4 ?
Na3 Zn2 Na2 O9 -71.01(11) 4 . . 4 ?
Na4 Zn2 Na2 O9 -144.36(11) 2 . . 4 ?
Na1 Zn2 Na2 O9 81.35(11) . . . 4 ?
Na5 Zn2 Na2 O9 129.29(10) 4_545 . . 4 ?
O8 Zn2 Na2 O9 -138.36(14) . . . 3_455 ?
O3 Zn2 Na2 O9 -38.18(14) 2 . . 3_455 ?
O6 Zn2 Na2 O9 103.04(13) 4 . . 3_455 ?
F2 Zn2 Na2 O9 -155.85(15) . . . 3_455 ?
O12 Zn2 Na2 O9 20.65(15) 6_565 . . 3_455 ?
Na3 Zn2 Na2 O9 80.33(11) 4 . . 3_455 ?
Na4 Zn2 Na2 O9 6.98(10) 2 . . 3_455 ?
Na1 Zn2 Na2 O9 -127.31(10) . . . 3_455 ?
Na5 Zn2 Na2 O9 -79.37(11) 4_545 . . 3_455 ?
O8 Zn2 Na2 O3 -100.18(15) . . . 2 ?
O6 Zn2 Na2 O3 141.21(13) 4 . . 2 ?
F2 Zn2 Na2 O3 -117.67(16) . . . 2 ?
O12 Zn2 Na2 O3 58.83(15) 6_565 . . 2 ?
Na3 Zn2 Na2 O3 118.51(12) 4 . . 2 ?
Na4 Zn2 Na2 O3 45.16(11) 2 . . 2 ?
Na1 Zn2 Na2 O3 -89.13(11) . . . 2 ?
Na5 Zn2 Na2 O3 -41.19(12) 4_545 . . 2 ?
O8 Zn2 Na2 O3 2.99(15) . . . . ?
O3 Zn2 Na2 O3 103.17(18) 2 . . . ?
O6 Zn2 Na2 O3 -115.62(12) 4 . . . ?
F2 Zn2 Na2 O3 -14.51(12) . . . . ?
O12 Zn2 Na2 O3 161.99(13) 6_565 . . . ?
Na3 Zn2 Na2 O3 -138.32(10) 4 . . . ?
Na4 Zn2 Na2 O3 148.33(10) 2 . . . ?
Na1 Zn2 Na2 O3 14.04(9) . . . . ?
Na5 Zn2 Na2 O3 61.98(9) 4_545 . . . ?
O8 Zn2 Na2 Zn1 -101.13(11) . . . 2 ?
O3 Zn2 Na2 Zn1 -0.96(11) 2 . . 2 ?
O6 Zn2 Na2 Zn1 140.26(9) 4 . . 2 ?
F2 Zn2 Na2 Zn1 -118.63(12) . . . 2 ?
O12 Zn2 Na2 Zn1 57.87(12) 6_565 . . 2 ?
Na3 Zn2 Na2 Zn1 117.56(6) 4 . . 2 ?
Na4 Zn2 Na2 Zn1 44.21(5) 2 . . 2 ?
Na1 Zn2 Na2 Zn1 -90.08(5) . . . 2 ?
Na5 Zn2 Na2 Zn1 -42.14(7) 4_545 . . 2 ?
O8 Zn2 Na2 Zn1 38.82(12) . . . . ?
O3 Zn2 Na2 Zn1 139.00(12) 2 . . . ?
O6 Zn2 Na2 Zn1 -79.79(9) 4 . . . ?
F2 Zn2 Na2 Zn1 21.33(10) . . . . ?
O12 Zn2 Na2 Zn1 -162.17(10) 6_565 . . . ?
Na3 Zn2 Na2 Zn1 -102.49(6) 4 . . . ?
Na4 Zn2 Na2 Zn1 -175.84(6) 2 . . . ?
Na1 Zn2 Na2 Zn1 49.87(4) . . . . ?
Na5 Zn2 Na2 Zn1 97.81(4) 4_545 . . . ?
O8 Zn2 Na2 Zn2 -34.94(12) . . . 2 ?
O3 Zn2 Na2 Zn2 65.23(11) 2 . . 2 ?
O6 Zn2 Na2 Zn2 -153.55(8) 4 . . 2 ?
F2 Zn2 Na2 Zn2 -52.44(10) . . . 2 ?
O12 Zn2 Na2 Zn2 124.06(10) 6_565 . . 2 ?
Na3 Zn2 Na2 Zn2 -176.25(5) 4 . . 2 ?
Na4 Zn2 Na2 Zn2 110.40(4) 2 . . 2 ?
Na1 Zn2 Na2 Zn2 -23.89(3) . . . 2 ?
Na5 Zn2 Na2 Zn2 24.05(4) 4_545 . . 2 ?
O9 Zn1 Na3 O1 79.6(2) 4 . . . ?
O4 Zn1 Na3 O1 -140.65(15) . . . . ?
F2 Zn1 Na3 O1 -49.01(14) . . . . ?
O15 Zn1 Na3 O1 111.5(2) 7_556 . . . ?
O14 Zn1 Na3 O1 139.9(2) . . . . ?
Na5 Zn1 Na3 O1 166.11(13) . . . . ?
Na2 Zn1 Na3 O1 1.27(13) . . . . ?
Na1 Zn1 Na3 O1 -57.60(12) . . . . ?
Na4 Zn1 Na3 O1 70.60(13) . . . . ?
O9 Zn1 Na3 O12 -129.7(2) 4 . . 7_556 ?
O4 Zn1 Na3 O12 10.06(13) . . . 7_556 ?
O1 Zn1 Na3 O12 150.71(17) . . . 7_556 ?
F2 Zn1 Na3 O12 101.70(13) . . . 7_556 ?
O15 Zn1 Na3 O12 -97.7(2) 7_556 . . 7_556 ?
O14 Zn1 Na3 O12 -69.4(2) . . . 7_556 ?
Na5 Zn1 Na3 O12 -43.17(11) . . . 7_556 ?
Na2 Zn1 Na3 O12 151.98(10) . . . 7_556 ?
Na1 Zn1 Na3 O12 93.12(11) . . . 7_556 ?
Na4 Zn1 Na3 O12 -138.69(10) . . . 7_556 ?
O9 Zn1 Na3 O11 29.5(2) 4 . . 1_545 ?
O4 Zn1 Na3 O11 169.29(13) . . . 1_545 ?
O1 Zn1 Na3 O11 -50.06(15) . . . 1_545 ?
F2 Zn1 Na3 O11 -99.07(12) . . . 1_545 ?
O15 Zn1 Na3 O11 61.48(19) 7_556 . . 1_545 ?
O14 Zn1 Na3 O11 89.9(2) . . . 1_545 ?
Na5 Zn1 Na3 O11 116.05(10) . . . 1_545 ?
Na2 Zn1 Na3 O11 -48.79(11) . . . 1_545 ?
Na1 Zn1 Na3 O11 -107.66(10) . . . 1_545 ?
Na4 Zn1 Na3 O11 20.54(11) . . . 1_545 ?
O9 Zn1 Na3 O13 -64.6(2) 4 . . 7_556 ?
O4 Zn1 Na3 O13 75.21(17) . . . 7_556 ?
O1 Zn1 Na3 O13 -144.14(19) . . . 7_556 ?
F2 Zn1 Na3 O13 166.85(16) . . . 7_556 ?
O15 Zn1 Na3 O13 -32.6(2) 7_556 . . 7_556 ?
O14 Zn1 Na3 O13 -4.2(3) . . . 7_556 ?
Na5 Zn1 Na3 O13 21.97(14) . . . 7_556 ?
Na2 Zn1 Na3 O13 -142.87(14) . . . 7_556 ?
Na1 Zn1 Na3 O13 158.26(15) . . . 7_556 ?
Na4 Zn1 Na3 O13 -73.54(15) . . . 7_556 ?
O9 Zn1 Na3 O7 124.6(2) 4 . . 4_545 ?
O4 Zn1 Na3 O7 -95.60(12) . . . 4_545 ?
O1 Zn1 Na3 O7 45.05(14) . . . 4_545 ?
F2 Zn1 Na3 O7 -3.96(12) . . . 4_545 ?
O15 Zn1 Na3 O7 156.59(19) 7_556 . . 4_545 ?
O14 Zn1 Na3 O7 -175.0(2) . . . 4_545 ?
Na5 Zn1 Na3 O7 -148.83(9) . . . 4_545 ?
Na2 Zn1 Na3 O7 46.32(11) . . . 4_545 ?
Na1 Zn1 Na3 O7 -12.54(9) . . . 4_545 ?
Na4 Zn1 Na3 O7 115.65(10) . . . 4_545 ?
O9 Zn1 Na3 O14 -60.3(3) 4 . . . ?
O4 Zn1 Na3 O14 79.4(2) . . . . ?
O1 Zn1 Na3 O14 -139.9(2) . . . . ?
F2 Zn1 Na3 O14 171.1(2) . . . . ?
O15 Zn1 Na3 O14 -28.4(3) 7_556 . . . ?
Na5 Zn1 Na3 O14 26.2(2) . . . . ?
Na2 Zn1 Na3 O14 -138.7(2) . . . . ?
Na1 Zn1 Na3 O14 162.5(2) . . . . ?
Na4 Zn1 Na3 O14 -69.3(2) . . . . ?
O9 Zn1 Na3 O6 -173.4(2) 4 . . . ?
O4 Zn1 Na3 O6 -33.66(12) . . . . ?
O1 Zn1 Na3 O6 107.00(15) . . . . ?
F2 Zn1 Na3 O6 57.98(11) . . . . ?
O15 Zn1 Na3 O6 -141.46(18) 7_556 . . . ?
O14 Zn1 Na3 O6 -113.1(2) . . . . ?
Na5 Zn1 Na3 O6 -86.89(8) . . . . ?
Na2 Zn1 Na3 O6 108.27(9) . . . . ?
Na1 Zn1 Na3 O6 49.40(8) . . . . ?
Na4 Zn1 Na3 O6 177.60(8) . . . . ?
O9 Zn1 Na3 C5 -37.18(19) 4 . . . ?
O4 Zn1 Na3 C5 102.58(9) . . . . ?
O1 Zn1 Na3 C5 -116.77(13) . . . . ?
F2 Zn1 Na3 C5 -165.78(8) . . . . ?
O15 Zn1 Na3 C5 -5.23(16) 7_556 . . . ?
O14 Zn1 Na3 C5 23.2(2) . . . . ?
Na5 Zn1 Na3 C5 49.34(4) . . . . ?
Na2 Zn1 Na3 C5 -115.50(4) . . . . ?
Na1 Zn1 Na3 C5 -174.37(5) . . . . ?
Na4 Zn1 Na3 C5 -46.17(4) . . . . ?
O9 Zn1 Na3 O15 -40.8(2) 4 . . . ?
O4 Zn1 Na3 O15 98.91(15) . . . . ?
O1 Zn1 Na3 O15 -120.44(17) . . . . ?
F2 Zn1 Na3 O15 -169.45(14) . . . . ?
O15 Zn1 Na3 O15 -8.9(3) 7_556 . . . ?
O14 Zn1 Na3 O15 19.5(2) . . . . ?
Na5 Zn1 Na3 O15 45.67(12) . . . . ?
Na2 Zn1 Na3 O15 -119.17(12) . . . . ?
Na1 Zn1 Na3 O15 -178.04(13) . . . . ?
Na4 Zn1 Na3 O15 -49.84(13) . . . . ?
O9 Zn1 Na3 Zn2 -170.17(18) 4 . . 4_545 ?
O4 Zn1 Na3 Zn2 -30.41(10) . . . 4_545 ?
O1 Zn1 Na3 Zn2 110.25(13) . . . 4_545 ?
F2 Zn1 Na3 Zn2 61.23(9) . . . 4_545 ?
O15 Zn1 Na3 Zn2 -138.21(17) 7_556 . . 4_545 ?
O14 Zn1 Na3 Zn2 -109.8(2) . . . 4_545 ?
Na5 Zn1 Na3 Zn2 -83.64(5) . . . 4_545 ?
Na2 Zn1 Na3 Zn2 111.52(5) . . . 4_545 ?
Na1 Zn1 Na3 Zn2 52.65(5) . . . 4_545 ?
Na4 Zn1 Na3 Zn2 -179.15(4) . . . 4_545 ?
O9 Zn1 Na3 Zn3 92.48(19) 4 . . . ?
O4 Zn1 Na3 Zn3 -127.77(9) . . . . ?
O1 Zn1 Na3 Zn3 12.89(12) . . . . ?
F2 Zn1 Na3 Zn3 -36.13(9) . . . . ?
O15 Zn1 Na3 Zn3 124.43(17) 7_556 . . . ?
O14 Zn1 Na3 Zn3 152.8(2) . . . . ?
Na5 Zn1 Na3 Zn3 179.00(4) . . . . ?
Na2 Zn1 Na3 Zn3 14.16(7) . . . . ?
Na1 Zn1 Na3 Zn3 -44.71(4) . . . . ?
Na4 Zn1 Na3 Zn3 83.49(5) . . . . ?
O7 Zn3 Na3 O1 119.53(17) 4_545 . . . ?
O2 Zn3 Na3 O1 -31.56(12) . . . . ?
O5 Zn3 Na3 O1 176.9(2) 3_445 . . . ?
F1 Zn3 Na3 O1 47.28(13) . . . . ?
O10 Zn3 Na3 O1 -124.47(13) 1_545 . . . ?
Na5 Zn3 Na3 O1 -73.28(10) 3_445 . . . ?
Na1 Zn3 Na3 O1 -2.05(10) 2 . . . ?
Na4 Zn3 Na3 O1 -166.19(9) 1_545 . . . ?
Na1 Zn3 Na3 O1 53.89(9) . . . . ?
Na2 Zn3 Na3 O1 129.04(9) 1_545 . . . ?
O7 Zn3 Na3 O12 -20.04(16) 4_545 . . 7_556 ?
O2 Zn3 Na3 O12 -171.12(14) . . . 7_556 ?
O5 Zn3 Na3 O12 37.3(2) 3_445 . . 7_556 ?
F1 Zn3 Na3 O12 -92.29(14) . . . 7_556 ?
O10 Zn3 Na3 O12 95.96(14) 1_545 . . 7_556 ?
Na5 Zn3 Na3 O12 147.15(12) 3_445 . . 7_556 ?
Na1 Zn3 Na3 O12 -141.62(11) 2 . . 7_556 ?
Na4 Zn3 Na3 O12 54.25(12) 1_545 . . 7_556 ?
Na1 Zn3 Na3 O12 -85.68(12) . . . 7_556 ?
Na2 Zn3 Na3 O12 -10.52(13) 1_545 . . 7_556 ?
O7 Zn3 Na3 O11 -135.51(17) 4_545 . . 1_545 ?
O2 Zn3 Na3 O11 73.41(12) . . . 1_545 ?
O5 Zn3 Na3 O11 -78.2(2) 3_445 . . 1_545 ?
F1 Zn3 Na3 O11 152.24(13) . . . 1_545 ?
O10 Zn3 Na3 O11 -19.51(13) 1_545 . . 1_545 ?
Na5 Zn3 Na3 O11 31.68(10) 3_445 . . 1_545 ?
Na1 Zn3 Na3 O11 102.91(10) 2 . . 1_545 ?
Na4 Zn3 Na3 O11 -61.23(10) 1_545 . . 1_545 ?
Na1 Zn3 Na3 O11 158.85(10) . . . 1_545 ?
Na2 Zn3 Na3 O11 -126.00(10) 1_545 . . 1_545 ?
O7 Zn3 Na3 O13 157.1(3) 4_545 . . 7_556 ?
O2 Zn3 Na3 O13 6.0(3) . . . 7_556 ?
O5 Zn3 Na3 O13 -145.5(3) 3_445 . . 7_556 ?
F1 Zn3 Na3 O13 84.9(3) . . . 7_556 ?
O10 Zn3 Na3 O13 -86.9(3) 1_545 . . 7_556 ?
Na5 Zn3 Na3 O13 -35.7(3) 3_445 . . 7_556 ?
Na1 Zn3 Na3 O13 35.5(3) 2 . . 7_556 ?
Na4 Zn3 Na3 O13 -128.6(3) 1_545 . . 7_556 ?
Na1 Zn3 Na3 O13 91.5(3) . . . 7_556 ?
Na2 Zn3 Na3 O13 166.6(3) 1_545 . . 7_556 ?
O2 Zn3 Na3 O7 -151.09(16) . . . 4_545 ?
O5 Zn3 Na3 O7 57.4(2) 3_445 . . 4_545 ?
F1 Zn3 Na3 O7 -72.25(16) . . . 4_545 ?
O10 Zn3 Na3 O7 116.00(16) 1_545 . . 4_545 ?
Na5 Zn3 Na3 O7 167.19(14) 3_445 . . 4_545 ?
Na1 Zn3 Na3 O7 -121.59(14) 2 . . 4_545 ?
Na4 Zn3 Na3 O7 74.28(14) 1_545 . . 4_545 ?
Na1 Zn3 Na3 O7 -65.64(14) . . . 4_545 ?
Na2 Zn3 Na3 O7 9.51(14) 1_545 . . 4_545 ?
O7 Zn3 Na3 O14 132.5(2) 4_545 . . . ?
O2 Zn3 Na3 O14 -18.55(19) . . . . ?
O5 Zn3 Na3 O14 -170.1(2) 3_445 . . . ?
F1 Zn3 Na3 O14 60.29(19) . . . . ?
O10 Zn3 Na3 O14 -111.46(19) 1_545 . . . ?
Na5 Zn3 Na3 O14 -60.28(18) 3_445 . . . ?
Na1 Zn3 Na3 O14 10.95(18) 2 . . . ?
Na4 Zn3 Na3 O14 -153.18(17) 1_545 . . . ?
Na1 Zn3 Na3 O14 66.90(17) . . . . ?
Na2 Zn3 Na3 O14 142.05(17) 1_545 . . . ?
O7 Zn3 Na3 O6 50.62(15) 4_545 . . . ?
O2 Zn3 Na3 O6 -100.47(12) . . . . ?
O5 Zn3 Na3 O6 108.0(2) 3_445 . . . ?
F1 Zn3 Na3 O6 -21.63(12) . . . . ?
O10 Zn3 Na3 O6 166.62(12) 1_545 . . . ?
Na5 Zn3 Na3 O6 -142.19(8) 3_445 . . . ?
Na1 Zn3 Na3 O6 -70.97(10) 2 . . . ?
Na4 Zn3 Na3 O6 124.90(8) 1_545 . . . ?
Na1 Zn3 Na3 O6 -15.02(8) . . . . ?
Na2 Zn3 Na3 O6 60.13(9) 1_545 . . . ?
O7 Zn3 Na3 C5 163.33(16) 4_545 . . . ?
O2 Zn3 Na3 C5 12.24(10) . . . . ?
O5 Zn3 Na3 C5 -139.32(19) 3_445 . . . ?
F1 Zn3 Na3 C5 91.08(11) . . . . ?
O10 Zn3 Na3 C5 -80.67(11) 1_545 . . . ?
Na5 Zn3 Na3 C5 -29.48(8) 3_445 . . . ?
Na1 Zn3 Na3 C5 41.74(9) 2 . . . ?
Na4 Zn3 Na3 C5 -122.39(7) 1_545 . . . ?
Na1 Zn3 Na3 C5 97.69(7) . . . . ?
Na2 Zn3 Na3 C5 172.84(5) 1_545 . . . ?
O7 Zn3 Na3 O15 -164.0(2) 4_545 . . . ?
O2 Zn3 Na3 O15 44.88(19) . . . . ?
O5 Zn3 Na3 O15 -106.7(3) 3_445 . . . ?
F1 Zn3 Na3 O15 123.72(19) . . . . ?
O10 Zn3 Na3 O15 -48.0(2) 1_545 . . . ?
Na5 Zn3 Na3 O15 3.15(19) 3_445 . . . ?
Na1 Zn3 Na3 O15 74.38(19) 2 . . . ?
Na4 Zn3 Na3 O15 -89.75(18) 1_545 . . . ?
Na1 Zn3 Na3 O15 130.33(19) . . . . ?
Na2 Zn3 Na3 O15 -154.52(18) 1_545 . . . ?
O7 Zn3 Na3 Zn2 10.04(13) 4_545 . . 4_545 ?
O2 Zn3 Na3 Zn2 -141.04(9) . . . 4_545 ?
O5 Zn3 Na3 Zn2 67.4(2) 3_445 . . 4_545 ?
F1 Zn3 Na3 Zn2 -62.21(10) . . . 4_545 ?
O10 Zn3 Na3 Zn2 126.04(10) 1_545 . . 4_545 ?
Na5 Zn3 Na3 Zn2 177.23(4) 3_445 . . 4_545 ?
Na1 Zn3 Na3 Zn2 -111.54(5) 2 . . 4_545 ?
Na4 Zn3 Na3 Zn2 84.32(5) 1_545 . . 4_545 ?
Na1 Zn3 Na3 Zn2 -55.60(5) . . . 4_545 ?
Na2 Zn3 Na3 Zn2 19.55(6) 1_545 . . 4_545 ?
O7 Zn3 Na3 Zn1 110.37(14) 4_545 . . . ?
O2 Zn3 Na3 Zn1 -40.71(9) . . . . ?
O5 Zn3 Na3 Zn1 167.73(18) 3_445 . . . ?
F1 Zn3 Na3 Zn1 38.12(10) . . . . ?
O10 Zn3 Na3 Zn1 -133.63(9) 1_545 . . . ?
Na5 Zn3 Na3 Zn1 -82.44(5) 3_445 . . . ?
Na1 Zn3 Na3 Zn1 -11.21(7) 2 . . . ?
Na4 Zn3 Na3 Zn1 -175.34(4) 1_545 . . . ?
Na1 Zn3 Na3 Zn1 44.73(4) . . . . ?
Na2 Zn3 Na3 Zn1 119.89(4) 1_545 . . . ?
O9 Zn1 Na5 O14 118.5(2) 4 . . . ?
O4 Zn1 Na5 O14 -114.0(2) . . . . ?
O1 Zn1 Na5 O14 -15.8(2) . . . . ?
F2 Zn1 Na5 O14 -153.6(3) . . . . ?
O15 Zn1 Na5 O14 46.3(3) 7_556 . . . ?
Na2 Zn1 Na5 O14 134.6(2) . . . . ?
Na3 Zn1 Na5 O14 -28.3(2) . . . . ?
Na1 Zn1 Na5 O14 -86.3(2) . . . . ?
Na4 Zn1 Na5 O14 68.2(2) . . . . ?
O9 Zn1 Na5 O11 33.12(15) 4 . . 7_566 ?
O4 Zn1 Na5 O11 160.62(16) . . . 7_566 ?
O1 Zn1 Na5 O11 -101.19(15) . . . 7_566 ?
F2 Zn1 Na5 O11 121.02(15) . . . 7_566 ?
O15 Zn1 Na5 O11 -39.1(2) 7_556 . . 7_566 ?
O14 Zn1 Na5 O11 -85.4(2) . . . 7_566 ?
Na2 Zn1 Na5 O11 49.22(13) . . . 7_566 ?
Na3 Zn1 Na5 O11 -113.73(11) . . . 7_566 ?
Na1 Zn1 Na5 O11 -171.68(10) . . . 7_566 ?
Na4 Zn1 Na5 O11 -17.21(12) . . . 7_566 ?
O9 Zn1 Na5 O2 -89.11(15) 4 . . 3 ?
O4 Zn1 Na5 O2 38.39(14) . . . 3 ?
O1 Zn1 Na5 O2 136.58(14) . . . 3 ?
F2 Zn1 Na5 O2 -1.21(17) . . . 3 ?
O15 Zn1 Na5 O2 -161.3(2) 7_556 . . 3 ?
O14 Zn1 Na5 O2 152.4(2) . . . 3 ?
Na2 Zn1 Na5 O2 -73.01(11) . . . 3 ?
Na3 Zn1 Na5 O2 124.04(10) . . . 3 ?
Na1 Zn1 Na5 O2 66.10(12) . . . 3 ?
Na4 Zn1 Na5 O2 -139.44(10) . . . 3 ?
O9 Zn1 Na5 O4 -127.49(15) 4 . . . ?
O1 Zn1 Na5 O4 98.19(16) . . . . ?
F2 Zn1 Na5 O4 -39.60(17) . . . . ?
O15 Zn1 Na5 O4 160.3(2) 7_556 . . . ?
O14 Zn1 Na5 O4 114.0(2) . . . . ?
Na2 Zn1 Na5 O4 -111.40(12) . . . . ?
Na3 Zn1 Na5 O4 85.66(11) . . . . ?
Na1 Zn1 Na5 O4 27.71(12) . . . . ?
Na4 Zn1 Na5 O4 -177.83(11) . . . . ?
O9 Zn1 Na5 O8 -30.21(13) 4 . . 4 ?
O4 Zn1 Na5 O8 97.28(13) . . . 4 ?
O1 Zn1 Na5 O8 -164.52(14) . . . 4 ?
F2 Zn1 Na5 O8 57.68(14) . . . 4 ?
O15 Zn1 Na5 O8 -102.4(2) 7_556 . . 4 ?
O14 Zn1 Na5 O8 -148.7(2) . . . 4 ?
Na2 Zn1 Na5 O8 -14.11(9) . . . 4 ?
Na3 Zn1 Na5 O8 -177.06(8) . . . 4 ?
Na1 Zn1 Na5 O8 124.99(9) . . . 4 ?
Na4 Zn1 Na5 O8 -80.54(8) . . . 4 ?
O9 Zn1 Na5 O15 72.2(2) 4 . . 7_556 ?
O4 Zn1 Na5 O15 -160.3(2) . . . 7_556 ?
O1 Zn1 Na5 O15 -62.1(2) . . . 7_556 ?
F2 Zn1 Na5 O15 160.1(2) . . . 7_556 ?
O14 Zn1 Na5 O15 -46.3(3) . . . 7_556 ?
Na2 Zn1 Na5 O15 88.3(2) . . . 7_556 ?
Na3 Zn1 Na5 O15 -74.7(2) . . . 7_556 ?
Na1 Zn1 Na5 O15 -132.6(2) . . . 7_556 ?
Na4 Zn1 Na5 O15 21.9(2) . . . 7_556 ?
O9 Zn1 Na5 O10 -171.13(14) 4 . . 3_545 ?
O4 Zn1 Na5 O10 -43.63(13) . . . 3_545 ?
O1 Zn1 Na5 O10 54.56(15) . . . 3_545 ?
F2 Zn1 Na5 O10 -83.23(15) . . . 3_545 ?
O15 Zn1 Na5 O10 116.7(2) 7_556 . . 3_545 ?
O14 Zn1 Na5 O10 70.4(2) . . . 3_545 ?
Na2 Zn1 Na5 O10 -155.03(8) . . . 3_545 ?
Na3 Zn1 Na5 O10 42.02(10) . . . 3_545 ?
Na1 Zn1 Na5 O10 -15.92(12) . . . 3_545 ?
Na4 Zn1 Na5 O10 138.54(9) . . . 3_545 ?
O9 Zn1 Na5 O13 127.17(17) 4 . . 7_556 ?
O4 Zn1 Na5 O13 -105.34(17) . . . 7_556 ?
O1 Zn1 Na5 O13 -7.15(17) . . . 7_556 ?
F2 Zn1 Na5 O13 -144.94(17) . . . 7_556 ?
O15 Zn1 Na5 O13 55.0(2) 7_556 . . 7_556 ?
O14 Zn1 Na5 O13 8.7(3) . . . 7_556 ?
Na2 Zn1 Na5 O13 143.26(13) . . . 7_556 ?
Na3 Zn1 Na5 O13 -19.68(14) . . . 7_556 ?
Na1 Zn1 Na5 O13 -77.63(14) . . . 7_556 ?
Na4 Zn1 Na5 O13 76.83(14) . . . 7_556 ?
O9 Zn1 Na5 C5 99.00(11) 4 . . . ?
O4 Zn1 Na5 C5 -133.51(12) . . . . ?
O1 Zn1 Na5 C5 -35.32(12) . . . . ?
F2 Zn1 Na5 C5 -173.11(12) . . . . ?
O15 Zn1 Na5 C5 26.8(2) 7_556 . . . ?
O14 Zn1 Na5 C5 -19.5(2) . . . . ?
Na2 Zn1 Na5 C5 115.10(4) . . . . ?
Na3 Zn1 Na5 C5 -47.85(4) . . . . ?
Na1 Zn1 Na5 C5 -105.80(5) . . . . ?
Na4 Zn1 Na5 C5 48.66(5) . . . . ?
O9 Zn1 Na5 Zn3 -129.66(11) 4 . . 3 ?
O4 Zn1 Na5 Zn3 -2.17(11) . . . 3 ?
O1 Zn1 Na5 Zn3 96.03(12) . . . 3 ?
F2 Zn1 Na5 Zn3 -41.76(14) . . . 3 ?
O15 Zn1 Na5 Zn3 158.1(2) 7_556 . . 3 ?
O14 Zn1 Na5 Zn3 111.8(2) . . . 3 ?
Na2 Zn1 Na5 Zn3 -113.56(5) . . . 3 ?
Na3 Zn1 Na5 Zn3 83.49(5) . . . 3 ?
Na1 Zn1 Na5 Zn3 25.54(8) . . . 3 ?
Na4 Zn1 Na5 Zn3 -179.99(5) . . . 3 ?
O9 Zn1 Na5 Zn2 -32.94(11) 4 . . 4 ?
O4 Zn1 Na5 Zn2 94.55(11) . . . 4 ?
O1 Zn1 Na5 Zn2 -167.26(11) . . . 4 ?
F2 Zn1 Na5 Zn2 54.95(13) . . . 4 ?
O15 Zn1 Na5 Zn2 -105.1(2) 7_556 . . 4 ?
O14 Zn1 Na5 Zn2 -151.5(2) . . . 4 ?
Na2 Zn1 Na5 Zn2 -16.85(7) . . . 4 ?
Na3 Zn1 Na5 Zn2 -179.79(4) . . . 4 ?
Na1 Zn1 Na5 Zn2 122.26(5) . . . 4 ?
Na4 Zn1 Na5 Zn2 -83.28(5) . . . 4 ?
O7 Zn3 F1 Zn3 84.62(9) 4_545 . . 2 ?
O2 Zn3 F1 Zn3 -158.52(8) . . . 2 ?
O5 Zn3 F1 Zn3 -35.18(8) 3_445 . . 2 ?
O10 Zn3 F1 Zn3 -99.2(6) 1_545 . . 2 ?
Na5 Zn3 F1 Zn3 -123.48(5) 3_445 . . 2 ?
Na1 Zn3 F1 Zn3 -116.42(10) 2 . . 2 ?
Na4 Zn3 F1 Zn3 2.22(5) 1_545 . . 2 ?
Na1 Zn3 F1 Zn3 115.52(10) . . . 2 ?
Na3 Zn3 F1 Zn3 124.01(4) . . . 2 ?
Na2 Zn3 F1 Zn3 0.0 1_545 . . 2 ?
O7 Zn3 F1 Na1 -30.89(14) 4_545 . . . ?
O2 Zn3 F1 Na1 85.97(13) . . . . ?
O5 Zn3 F1 Na1 -150.70(13) 3_445 . . . ?
O10 Zn3 F1 Na1 145.3(6) 1_545 . . . ?
Na5 Zn3 F1 Na1 121.01(8) 3_445 . . . ?
Na1 Zn3 F1 Na1 128.06(19) 2 . . . ?
Na4 Zn3 F1 Na1 -113.30(12) 1_545 . . . ?
Na3 Zn3 F1 Na1 8.49(13) . . . . ?
Na2 Zn3 F1 Na1 -115.52(10) 1_545 . . . ?
O7 Zn3 F1 Na1 -158.96(13) 4_545 . . 2 ?
O2 Zn3 F1 Na1 -42.10(12) . . . 2 ?
O5 Zn3 F1 Na1 81.24(13) 3_445 . . 2 ?
O10 Zn3 F1 Na1 17.2(7) 1_545 . . 2 ?
Na5 Zn3 F1 Na1 -7.06(13) 3_445 . . 2 ?
Na4 Zn3 F1 Na1 118.64(11) 1_545 . . 2 ?
Na1 Zn3 F1 Na1 -128.06(19) . . . 2 ?
Na3 Zn3 F1 Na1 -119.57(8) . . . 2 ?
Na2 Zn3 F1 Na1 116.42(9) 1_545 . . 2 ?
F2 Na1 F1 Zn3 104.02(12) . . . 2 ?
O6 Na1 F1 Zn3 -141.92(15) . . . 2 ?
O4 Na1 F1 Zn3 -38.30(12) 4_545 . . 2 ?
O2 Na1 F1 Zn3 35.17(10) 2 . . 2 ?
O1 Na1 F1 Zn3 163.91(13) . . . 2 ?
O8 Na1 F1 Zn3 24.8(2) . . . 2 ?
O7 Na1 F1 Zn3 -128.49(14) 4_545 . . 2 ?
Zn1 Na1 F1 Zn3 144.96(9) . . . 2 ?
Zn2 Na1 F1 Zn3 64.14(13) . . . 2 ?
Zn3 Na1 F1 Zn3 -151.9(2) . . . 2 ?
F2 Na1 F1 Zn3 -104.05(13) . . . . ?
O6 Na1 F1 Zn3 10.0(2) . . . . ?
O4 Na1 F1 Zn3 113.63(13) 4_545 . . . ?
O2 Na1 F1 Zn3 -172.90(15) 2 . . . ?
O1 Na1 F1 Zn3 -44.16(12) . . . . ?
O8 Na1 F1 Zn3 176.70(13) . . . . ?
O7 Na1 F1 Zn3 23.44(11) 4_545 . . . ?
Zn3 Na1 F1 Zn3 151.9(2) 2 . . . ?
Zn1 Na1 F1 Zn3 -63.10(14) . . . . ?
Zn2 Na1 F1 Zn3 -143.92(9) . . . . ?
F2 Na1 F1 Na1 -0.89(6) . . . 2 ?
O6 Na1 F1 Na1 113.17(17) . . . 2 ?
O4 Na1 F1 Na1 -143.21(8) 4_545 . . 2 ?
O2 Na1 F1 Na1 -69.74(8) 2 . . 2 ?
O1 Na1 F1 Na1 59.00(7) . . . 2 ?
O8 Na1 F1 Na1 -80.15(15) . . . 2 ?
O7 Na1 F1 Na1 126.59(8) 4_545 . . 2 ?
Zn3 Na1 F1 Na1 -104.91(10) 2 . . 2 ?
Zn1 Na1 F1 Na1 40.05(5) . . . 2 ?
Zn2 Na1 F1 Na1 -40.77(5) . . . 2 ?
Zn3 Na1 F1 Na1 103.15(11) . . . 2 ?
O1 Na3 C5 O14 109.4(3) . . . 7_556 ?
O12 Na3 C5 O14 -104.5(3) 7_556 . . 7_556 ?
O11 Na3 C5 O14 20.7(3) 1_545 . . 7_556 ?
O13 Na3 C5 O14 -114.3(4) 7_556 . . 7_556 ?
O7 Na3 C5 O14 95.3(4) 4_545 . . 7_556 ?
O14 Na3 C5 O14 180.000(2) . . . 7_556 ?
O6 Na3 C5 O14 -179.2(3) . . . 7_556 ?
O15 Na3 C5 O14 -45.6(4) . . . 7_556 ?
Zn2 Na3 C5 O14 -143.7(3) 4_545 . . 7_556 ?
Zn1 Na3 C5 O14 142.7(3) . . . 7_556 ?
Zn3 Na3 C5 O14 72.7(3) . . . 7_556 ?
O1 Na3 C5 O14 -70.6(3) . . . . ?
O12 Na3 C5 O14 75.5(3) 7_556 . . . ?
O11 Na3 C5 O14 -159.3(3) 1_545 . . . ?
O13 Na3 C5 O14 65.7(4) 7_556 . . . ?
O7 Na3 C5 O14 -84.7(4) 4_545 . . . ?
O6 Na3 C5 O14 0.8(3) . . . . ?
O15 Na3 C5 O14 134.4(4) . . . . ?
Zn2 Na3 C5 O14 36.3(3) 4_545 . . . ?
Zn1 Na3 C5 O14 -37.3(3) . . . . ?
Zn3 Na3 C5 O14 -107.3(3) . . . . ?
O1 Na3 C5 O13 -136.3(3) . . . 7_556 ?
O12 Na3 C5 O13 9.8(3) 7_556 . . 7_556 ?
O11 Na3 C5 O13 135.0(3) 1_545 . . 7_556 ?
O7 Na3 C5 O13 -150.4(4) 4_545 . . 7_556 ?
O14 Na3 C5 O13 -65.7(4) . . . 7_556 ?
O6 Na3 C5 O13 -64.9(3) . . . 7_556 ?
O15 Na3 C5 O13 68.8(4) . . . 7_556 ?
Zn2 Na3 C5 O13 -29.4(3) 4_545 . . 7_556 ?
Zn1 Na3 C5 O13 -103.0(3) . . . 7_556 ?
Zn3 Na3 C5 O13 -173.0(3) . . . 7_556 ?
O1 Na3 C5 O13 43.7(3) . . . . ?
O12 Na3 C5 O13 -170.2(3) 7_556 . . . ?
O11 Na3 C5 O13 -45.0(3) 1_545 . . . ?
O13 Na3 C5 O13 180.000(1) 7_556 . . . ?
O7 Na3 C5 O13 29.6(4) 4_545 . . . ?
O14 Na3 C5 O13 114.3(4) . . . . ?
O6 Na3 C5 O13 115.1(3) . . . . ?
O15 Na3 C5 O13 -111.2(4) . . . . ?
Zn2 Na3 C5 O13 150.6(3) 4_545 . . . ?
Zn1 Na3 C5 O13 77.0(3) . . . . ?
Zn3 Na3 C5 O13 7.0(3) . . . . ?
O1 Na3 C5 O15 154.9(3) . . . . ?
O12 Na3 C5 O15 -59.0(3) 7_556 . . . ?
O11 Na3 C5 O15 66.2(3) 1_545 . . . ?
O13 Na3 C5 O15 -68.8(4) 7_556 . . . ?
O7 Na3 C5 O15 140.9(4) 4_545 . . . ?
O14 Na3 C5 O15 -134.4(4) . . . . ?
O6 Na3 C5 O15 -133.6(3) . . . . ?
Zn2 Na3 C5 O15 -98.2(3) 4_545 . . . ?
Zn1 Na3 C5 O15 -171.8(3) . . . . ?
Zn3 Na3 C5 O15 118.3(3) . . . . ?
O1 Na3 C5 O15 -25.1(3) . . . 7_556 ?
O12 Na3 C5 O15 121.0(3) 7_556 . . 7_556 ?
O11 Na3 C5 O15 -113.8(3) 1_545 . . 7_556 ?
O13 Na3 C5 O15 111.2(4) 7_556 . . 7_556 ?
O7 Na3 C5 O15 -39.1(4) 4_545 . . 7_556 ?
O14 Na3 C5 O15 45.6(4) . . . 7_556 ?
O6 Na3 C5 O15 46.4(3) . . . 7_556 ?
O15 Na3 C5 O15 180.000(2) . . . 7_556 ?
Zn2 Na3 C5 O15 81.8(3) 4_545 . . 7_556 ?
Zn1 Na3 C5 O15 8.2(3) . . . 7_556 ?
Zn3 Na3 C5 O15 -61.7(3) . . . 7_556 ?
O1 Na3 C5 Na3 38(100) . . . 7_556 ?
O12 Na3 C5 Na3 -176(100) 7_556 . . 7_556 ?
O11 Na3 C5 Na3 -51(100) 1_545 . . 7_556 ?
O13 Na3 C5 Na3 174(100) 7_556 . . 7_556 ?
O7 Na3 C5 Na3 24(100) 4_545 . . 7_556 ?
O14 Na3 C5 Na3 109(100) . . . 7_556 ?
O6 Na3 C5 Na3 110(100) . . . 7_556 ?
O15 Na3 C5 Na3 -117(100) . . . 7_556 ?
Zn2 Na3 C5 Na3 145(100) 4_545 . . 7_556 ?
Zn1 Na3 C5 Na3 71(100) . . . 7_556 ?
Zn3 Na3 C5 Na3 1(100) . . . 7_556 ?
O1 Na3 C5 Na5 91.90(9) . . . 7_556 ?
O12 Na3 C5 Na5 -121.99(10) 7_556 . . 7_556 ?
O11 Na3 C5 Na5 3.18(9) 1_545 . . 7_556 ?
O13 Na3 C5 Na5 -131.8(3) 7_556 . . 7_556 ?
O7 Na3 C5 Na5 77.9(2) 4_545 . . 7_556 ?
O14 Na3 C5 Na5 162.5(3) . . . 7_556 ?
O6 Na3 C5 Na5 163.34(9) . . . 7_556 ?
O15 Na3 C5 Na5 -63.0(3) . . . 7_556 ?
Zn2 Na3 C5 Na5 -161.19(9) 4_545 . . 7_556 ?
Zn1 Na3 C5 Na5 125.21(4) . . . 7_556 ?
Zn3 Na3 C5 Na5 55.27(6) . . . 7_556 ?
O1 Na3 C5 Na5 -88.10(9) . . . . ?
O12 Na3 C5 Na5 58.01(10) 7_556 . . . ?
O11 Na3 C5 Na5 -176.82(9) 1_545 . . . ?
O13 Na3 C5 Na5 48.2(3) 7_556 . . . ?
O7 Na3 C5 Na5 -102.1(2) 4_545 . . . ?
O14 Na3 C5 Na5 -17.5(3) . . . . ?
O6 Na3 C5 Na5 -16.66(9) . . . . ?
O15 Na3 C5 Na5 117.0(3) . . . . ?
Zn2 Na3 C5 Na5 18.81(9) 4_545 . . . ?
Zn1 Na3 C5 Na5 -54.79(4) . . . . ?
Zn3 Na3 C5 Na5 -124.73(6) . . . . ?
O14 Na5 C5 O14 180.0 . . . 7_556 ?
O11 Na5 C5 O14 -18.4(4) 7_566 . . 7_556 ?
O2 Na5 C5 O14 172.4(7) 3 . . 7_556 ?
O4 Na5 C5 O14 -171.9(4) . . . 7_556 ?
O8 Na5 C5 O14 -98.6(4) 4 . . 7_556 ?
O15 Na5 C5 O14 -102.5(5) 7_556 . . 7_556 ?
O10 Na5 C5 O14 103.7(4) 3_545 . . 7_556 ?
O13 Na5 C5 O14 116.9(5) 7_556 . . 7_556 ?
Zn1 Na5 C5 O14 -144.0(4) . . . 7_556 ?
Zn3 Na5 C5 O14 137.6(4) 3 . . 7_556 ?
Zn2 Na5 C5 O14 -71.8(4) 4 . . 7_556 ?
O11 Na5 C5 O14 161.6(4) 7_566 . . . ?
O2 Na5 C5 O14 -7.6(7) 3 . . . ?
O4 Na5 C5 O14 8.1(4) . . . . ?
O8 Na5 C5 O14 81.4(4) 4 . . . ?
O15 Na5 C5 O14 77.5(5) 7_556 . . . ?
O10 Na5 C5 O14 -76.3(4) 3_545 . . . ?
O13 Na5 C5 O14 -63.1(5) 7_556 . . . ?
Zn1 Na5 C5 O14 36.0(4) . . . . ?
Zn3 Na5 C5 O14 -42.4(4) 3 . . . ?
Zn2 Na5 C5 O14 108.2(4) 4 . . . ?
O14 Na5 C5 O13 63.1(5) . . . 7_556 ?
O11 Na5 C5 O13 -135.3(3) 7_566 . . 7_556 ?
O2 Na5 C5 O13 55.5(6) 3 . . 7_556 ?
O4 Na5 C5 O13 71.2(3) . . . 7_556 ?
O8 Na5 C5 O13 144.6(3) 4 . . 7_556 ?
O15 Na5 C5 O13 140.7(4) 7_556 . . 7_556 ?
O10 Na5 C5 O13 -13.2(3) 3_545 . . 7_556 ?
Zn1 Na5 C5 O13 99.1(3) . . . 7_556 ?
Zn3 Na5 C5 O13 20.7(3) 3 . . 7_556 ?
Zn2 Na5 C5 O13 171.4(3) 4 . . 7_556 ?
O14 Na5 C5 O13 -116.9(5) . . . . ?
O11 Na5 C5 O13 44.7(3) 7_566 . . . ?
O2 Na5 C5 O13 -124.5(6) 3 . . . ?
O4 Na5 C5 O13 -108.8(3) . . . . ?
O8 Na5 C5 O13 -35.4(3) 4 . . . ?
O15 Na5 C5 O13 -39.3(4) 7_556 . . . ?
O10 Na5 C5 O13 166.8(3) 3_545 . . . ?
O13 Na5 C5 O13 180.000(1) 7_556 . . . ?
Zn1 Na5 C5 O13 -80.9(3) . . . . ?
Zn3 Na5 C5 O13 -159.3(3) 3 . . . ?
Zn2 Na5 C5 O13 -8.6(3) 4 . . . ?
O14 Na5 C5 O15 102.5(5) . . . . ?
O11 Na5 C5 O15 -96.0(3) 7_566 . . . ?
O2 Na5 C5 O15 94.9(6) 3 . . . ?
O4 Na5 C5 O15 110.5(3) . . . . ?
O8 Na5 C5 O15 -176.1(3) 4 . . . ?
O15 Na5 C5 O15 180.000(2) 7_556 . . . ?
O10 Na5 C5 O15 26.2(3) 3_545 . . . ?
O13 Na5 C5 O15 39.3(4) 7_556 . . . ?
Zn1 Na5 C5 O15 138.4(3) . . . . ?
Zn3 Na5 C5 O15 60.0(3) 3 . . . ?
Zn2 Na5 C5 O15 -149.3(3) 4 . . . ?
O14 Na5 C5 O15 -77.5(5) . . . 7_556 ?
O11 Na5 C5 O15 84.0(3) 7_566 . . 7_556 ?
O2 Na5 C5 O15 -85.1(6) 3 . . 7_556 ?
O4 Na5 C5 O15 -69.5(3) . . . 7_556 ?
O8 Na5 C5 O15 3.9(3) 4 . . 7_556 ?
O10 Na5 C5 O15 -153.8(3) 3_545 . . 7_556 ?
O13 Na5 C5 O15 -140.7(4) 7_556 . . 7_556 ?
Zn1 Na5 C5 O15 -41.6(3) . . . 7_556 ?
Zn3 Na5 C5 O15 -120.0(3) 3 . . 7_556 ?
Zn2 Na5 C5 O15 30.7(3) 4 . . 7_556 ?
O14 Na5 C5 Na3 21.6(4) . . . . ?
O11 Na5 C5 Na3 -176.76(9) 7_566 . . . ?
O2 Na5 C5 Na3 14.1(6) 3 . . . ?
O4 Na5 C5 Na3 29.71(9) . . . . ?
O8 Na5 C5 Na3 103.08(9) 4 . . . ?
O15 Na5 C5 Na3 99.2(3) 7_556 . . . ?
O10 Na5 C5 Na3 -54.65(9) 3_545 . . . ?
O13 Na5 C5 Na3 -41.5(3) 7_556 . . . ?
Zn1 Na5 C5 Na3 57.63(4) . . . . ?
Zn3 Na5 C5 Na3 -20.77(9) 3 . . . ?
Zn2 Na5 C5 Na3 129.86(7) 4 . . . ?
O14 Na5 C5 Na3 -158.4(4) . . . 7_556 ?
O11 Na5 C5 Na3 3.24(9) 7_566 . . 7_556 ?
O2 Na5 C5 Na3 -165.9(6) 3 . . 7_556 ?
O4 Na5 C5 Na3 -150.29(9) . . . 7_556 ?
O8 Na5 C5 Na3 -76.92(9) 4 . . 7_556 ?
O15 Na5 C5 Na3 -80.8(3) 7_556 . . 7_556 ?
O10 Na5 C5 Na3 125.35(9) 3_545 . . 7_556 ?
O13 Na5 C5 Na3 138.5(3) 7_556 . . 7_556 ?
Zn1 Na5 C5 Na3 -122.37(4) . . . 7_556 ?
Zn3 Na5 C5 Na3 159.23(9) 3 . . 7_556 ?
Zn2 Na5 C5 Na3 -50.14(7) 4 . . 7_556 ?
O14 Na5 C5 Na5 -48(100) . . . 7_556 ?
O11 Na5 C5 Na5 113(100) 7_566 . . 7_556 ?
O2 Na5 C5 Na5 -56(100) 3 . . 7_556 ?
O4 Na5 C5 Na5 -40(100) . . . 7_556 ?
O8 Na5 C5 Na5 33(100) 4 . . 7_556 ?
O15 Na5 C5 Na5 29(100) 7_556 . . 7_556 ?
O10 Na5 C5 Na5 -125(100) 3_545 . . 7_556 ?
O13 Na5 C5 Na5 -112(100) 7_556 . . 7_556 ?
Zn1 Na5 C5 Na5 -12(100) . . . 7_556 ?
Zn3 Na5 C5 Na5 -91(100) 3 . . 7_556 ?
Zn2 Na5 C5 Na5 60(100) 4 . . 7_556 ?
O13 Na4 C4 O11 85.6(6) . . . . ?
O3 Na4 C4 O11 -63.3(8) . . . . ?
O10 Na4 C4 O11 -90.9(6) . . . . ?
O15 Na4 C4 O11 50.6(6) 7_556 . . . ?
O12 Na4 C4 O11 -147.5(6) 5_566 . . . ?
O9 Na4 C4 O11 -7.5(6) 4 . . . ?
O12 Na4 C4 O11 123.0(7) . . . . ?
O10 Na4 C4 O11 164.7(6) 5_566 . . . ?
O5 Na4 C4 O11 -71.9(6) 3_455 . . . ?
C4 Na4 C4 O11 -174.0(6) 5_566 . . . ?
Na4 Na4 C4 O11 -174.0(6) 5_566 . . . ?
O13 Na4 C4 O10 176.6(3) . . . . ?
O3 Na4 C4 O10 27.7(5) . . . . ?
O15 Na4 C4 O10 141.6(3) 7_556 . . . ?
O12 Na4 C4 O10 -56.6(3) 5_566 . . . ?
O9 Na4 C4 O10 83.4(2) 4 . . . ?
O12 Na4 C4 O10 -146.1(4) . . . . ?
O10 Na4 C4 O10 -104.4(2) 5_566 . . . ?
O5 Na4 C4 O10 19.1(2) 3_455 . . . ?
C4 Na4 C4 O10 -83.1(2) 5_566 . . . ?
Na4 Na4 C4 O10 -83.1(2) 5_566 . . . ?
O13 Na4 C4 O12 -37.4(3) . . . . ?
O3 Na4 C4 O12 173.7(3) . . . . ?
O10 Na4 C4 O12 146.1(4) . . . . ?
O15 Na4 C4 O12 -72.4(3) 7_556 . . . ?
O12 Na4 C4 O12 89.5(2) 5_566 . . . ?
O9 Na4 C4 O12 -130.5(2) 4 . . . ?
O10 Na4 C4 O12 41.7(2) 5_566 . . . ?
O5 Na4 C4 O12 165.1(2) 3_455 . . . ?
C4 Na4 C4 O12 62.9(2) 5_566 . . . ?
Na4 Na4 C4 O12 62.9(2) 5_566 . . . ?
O13 Na4 C4 Na4 -100.32(17) . . . 5_566 ?
O3 Na4 C4 Na4 110.8(4) . . . 5_566 ?
O10 Na4 C4 Na4 83.1(2) . . . 5_566 ?
O15 Na4 C4 Na4 -135.32(18) 7_556 . . 5_566 ?
O12 Na4 C4 Na4 26.54(10) 5_566 . . 5_566 ?
O9 Na4 C4 Na4 166.53(14) 4 . . 5_566 ?
O12 Na4 C4 Na4 -62.9(2) . . . 5_566 ?
O10 Na4 C4 Na4 -21.25(9) 5_566 . . 5_566 ?
O5 Na4 C4 Na4 102.18(10) 3_455 . . 5_566 ?
C4 Na4 C4 Na4 0.0 5_566 . . 5_566 ?
F1 Na1 O6 C2 -153.2(3) . . . . ?
F2 Na1 O6 C2 -32.4(3) . . . . ?
O4 Na1 O6 C2 108.4(3) 4_545 . . . ?
O2 Na1 O6 C2 33.7(5) 2 . . . ?
O1 Na1 O6 C2 -95.6(3) . . . . ?
O8 Na1 O6 C2 36.3(3) . . . . ?
O7 Na1 O6 C2 -166.5(3) 4_545 . . . ?
Zn3 Na1 O6 C2 141.8(3) 2 . . . ?
Zn1 Na1 O6 C2 -56.3(3) . . . . ?
Zn2 Na1 O6 C2 2.9(3) . . . . ?
Zn3 Na1 O6 C2 -147.2(3) . . . . ?
F1 Na1 O6 Zn2 61.0(2) . . . 4_545 ?
F2 Na1 O6 Zn2 -178.14(12) . . . 4_545 ?
O4 Na1 O6 Zn2 -37.35(15) 4_545 . . 4_545 ?
O2 Na1 O6 Zn2 -112.0(3) 2 . . 4_545 ?
O1 Na1 O6 Zn2 118.71(14) . . . 4_545 ?
O8 Na1 O6 Zn2 -109.44(14) . . . 4_545 ?
O7 Na1 O6 Zn2 47.80(12) 4_545 . . 4_545 ?
Zn3 Na1 O6 Zn2 -3.9(3) 2 . . 4_545 ?
Zn1 Na1 O6 Zn2 158.01(14) . . . 4_545 ?
Zn2 Na1 O6 Zn2 -142.86(10) . . . 4_545 ?
Zn3 Na1 O6 Zn2 67.12(12) . . . 4_545 ?
F1 Na1 O6 Na3 -26.0(2) . . . . ?
F2 Na1 O6 Na3 94.81(11) . . . . ?
O4 Na1 O6 Na3 -124.40(11) 4_545 . . . ?
O2 Na1 O6 Na3 161.0(3) 2 . . . ?
O1 Na1 O6 Na3 31.66(10) . . . . ?
O8 Na1 O6 Na3 163.51(12) . . . . ?
O7 Na1 O6 Na3 -39.25(10) 4_545 . . . ?
Zn3 Na1 O6 Na3 -91.0(2) 2 . . . ?
Zn1 Na1 O6 Na3 70.96(8) . . . . ?
Zn2 Na1 O6 Na3 130.09(8) . . . . ?
Zn3 Na1 O6 Na3 -19.93(11) . . . . ?
O1 Na3 O6 C2 95.7(3) . . . . ?
O12 Na3 O6 C2 -80.7(3) 7_556 . . . ?
O11 Na3 O6 C2 135.3(4) 1_545 . . . ?
O13 Na3 O6 C2 -1.5(3) 7_556 . . . ?
O7 Na3 O6 C2 176.5(3) 4_545 . . . ?
O14 Na3 O6 C2 22.0(3) . . . . ?
C5 Na3 O6 C2 21.7(3) . . . . ?
O15 Na3 O6 C2 -0.6(4) . . . . ?
Zn2 Na3 O6 C2 -116.0(3) 4_545 . . . ?
Zn1 Na3 O6 C2 59.1(3) . . . . ?
Zn3 Na3 O6 C2 150.3(3) . . . . ?
O1 Na3 O6 Zn2 -148.33(13) . . . 4_545 ?
O12 Na3 O6 Zn2 35.28(10) 7_556 . . 4_545 ?
O11 Na3 O6 Zn2 -108.7(3) 1_545 . . 4_545 ?
O13 Na3 O6 Zn2 114.52(16) 7_556 . . 4_545 ?
O7 Na3 O6 Zn2 -67.49(11) 4_545 . . 4_545 ?
O14 Na3 O6 Zn2 138.02(16) . . . 4_545 ?
C5 Na3 O6 Zn2 137.67(8) . . . 4_545 ?
O15 Na3 O6 Zn2 115.40(17) . . . 4_545 ?
Zn1 Na3 O6 Zn2 175.05(11) . . . 4_545 ?
Zn3 Na3 O6 Zn2 -93.68(8) . . . 4_545 ?
O1 Na3 O6 Na1 -35.68(12) . . . . ?
O12 Na3 O6 Na1 147.93(14) 7_556 . . . ?
O11 Na3 O6 Na1 3.9(4) 1_545 . . . ?
O13 Na3 O6 Na1 -132.83(16) 7_556 . . . ?
O7 Na3 O6 Na1 45.16(12) 4_545 . . . ?
O14 Na3 O6 Na1 -109.33(17) . . . . ?
C5 Na3 O6 Na1 -109.68(9) . . . . ?
O15 Na3 O6 Na1 -131.95(17) . . . . ?
Zn2 Na3 O6 Na1 112.65(13) 4_545 . . . ?
Zn1 Na3 O6 Na1 -72.30(9) . . . . ?
Zn3 Na3 O6 Na1 18.97(10) . . . . ?
O7 Zn3 O2 C1 6.8(3) 4_545 . . . ?
O5 Zn3 O2 C1 -167.2(3) 3_445 . . . ?
F1 Zn3 O2 C1 -81.8(3) . . . . ?
O10 Zn3 O2 C1 108.4(3) 1_545 . . . ?
Na5 Zn3 O2 C1 144.3(3) 3_445 . . . ?
Na1 Zn3 O2 C1 -120.4(3) 2 . . . ?
Na4 Zn3 O2 C1 115.7(3) 1_545 . . . ?
Na1 Zn3 O2 C1 -36.9(3) . . . . ?
Na3 Zn3 O2 C1 28.0(3) . . . . ?
Na2 Zn3 O2 C1 -122.4(3) 1_545 . . . ?
O7 Zn3 O2 Na5 -137.46(12) 4_545 . . 3_445 ?
O5 Zn3 O2 Na5 48.52(16) 3_445 . . 3_445 ?
F1 Zn3 O2 Na5 133.87(10) . . . 3_445 ?
O10 Zn3 O2 Na5 -35.88(12) 1_545 . . 3_445 ?
Na1 Zn3 O2 Na5 95.34(12) 2 . . 3_445 ?
Na4 Zn3 O2 Na5 -28.64(17) 1_545 . . 3_445 ?
Na1 Zn3 O2 Na5 178.82(10) . . . 3_445 ?
Na3 Zn3 O2 Na5 -116.30(10) . . . 3_445 ?
Na2 Zn3 O2 Na5 93.31(16) 1_545 . . 3_445 ?
O7 Zn3 O2 Na1 127.20(12) 4_545 . . 2 ?
O5 Zn3 O2 Na1 -46.83(15) 3_445 . . 2 ?
F1 Zn3 O2 Na1 38.53(8) . . . 2 ?
O10 Zn3 O2 Na1 -131.22(11) 1_545 . . 2 ?
Na5 Zn3 O2 Na1 -95.34(12) 3_445 . . 2 ?
Na4 Zn3 O2 Na1 -123.98(9) 1_545 . . 2 ?
Na1 Zn3 O2 Na1 83.47(8) . . . 2 ?
Na3 Zn3 O2 Na1 148.36(9) . . . 2 ?
Na2 Zn3 O2 Na1 -2.0(2) 1_545 . . 2 ?
O3 Zn2 O8 C3 164.9(3) 2 . . . ?
O6 Zn2 O8 C3 -20.9(3) 4 . . . ?
F2 Zn2 O8 C3 -113.3(3) . . . . ?
O12 Zn2 O8 C3 72.9(3) 6_565 . . . ?
Na3 Zn2 O8 C3 27.2(3) 4 . . . ?
Na2 Zn2 O8 C3 -125.5(3) . . . . ?
Na4 Zn2 O8 C3 116.9(3) 2 . . . ?
Na1 Zn2 O8 C3 -139.6(3) . . . . ?
Na5 Zn2 O8 C3 132.0(3) 4_545 . . . ?
O3 Zn2 O8 Na5 32.89(16) 2 . . 4_545 ?
O6 Zn2 O8 Na5 -152.94(11) 4 . . 4_545 ?
F2 Zn2 O8 Na5 114.64(11) . . . 4_545 ?
O12 Zn2 O8 Na5 -59.16(13) 6_565 . . 4_545 ?
Na3 Zn2 O8 Na5 -104.87(9) 4 . . 4_545 ?
Na2 Zn2 O8 Na5 102.46(11) . . . 4_545 ?
Na4 Zn2 O8 Na5 -15.11(19) 2 . . 4_545 ?
Na1 Zn2 O8 Na5 88.33(11) . . . 4_545 ?
O3 Zn2 O8 Na1 -55.44(15) 2 . . . ?
O6 Zn2 O8 Na1 118.73(11) 4 . . . ?
F2 Zn2 O8 Na1 26.31(10) . . . . ?
O12 Zn2 O8 Na1 -147.49(11) 6_565 . . . ?
Na3 Zn2 O8 Na1 166.80(8) 4 . . . ?
Na2 Zn2 O8 Na1 14.13(15) . . . . ?
Na4 Zn2 O8 Na1 -103.44(13) 2 . . . ?
Na5 Zn2 O8 Na1 -88.33(11) 4_545 . . . ?
F1 Na1 O8 C3 -153.5(3) . . . . ?
F2 Na1 O8 C3 109.0(4) . . . . ?
O6 Na1 O8 C3 17.5(4) . . . . ?
O4 Na1 O8 C3 -84.7(4) 4_545 . . . ?
O2 Na1 O8 C3 -163.6(4) 2 . . . ?
O1 Na1 O8 C3 82.7(4) . . . . ?
O7 Na1 O8 C3 -26.9(5) 4_545 . . . ?
Zn3 Na1 O8 C3 -138.3(3) 2 . . . ?
Zn1 Na1 O8 C3 77.6(4) . . . . ?
Zn2 Na1 O8 C3 132.9(4) . . . . ?
Zn3 Na1 O8 C3 -141.3(5) . . . . ?
F1 Na1 O8 Zn2 73.57(19) . . . . ?
F2 Na1 O8 Zn2 -23.92(9) . . . . ?
O6 Na1 O8 Zn2 -115.46(12) . . . . ?
O4 Na1 O8 Zn2 142.37(12) 4_545 . . . ?
O2 Na1 O8 Zn2 63.50(11) 2 . . . ?
O1 Na1 O8 Zn2 -50.22(16) . . . . ?
O7 Na1 O8 Zn2 -159.87(18) 4_545 . . . ?
Zn3 Na1 O8 Zn2 88.77(10) 2 . . . ?
Zn1 Na1 O8 Zn2 -55.32(9) . . . . ?
Zn3 Na1 O8 Zn2 85.8(6) . . . . ?
F1 Na1 O8 Na5 -27.41(19) . . . 4_545 ?
F2 Na1 O8 Na5 -124.90(11) . . . 4_545 ?
O6 Na1 O8 Na5 143.56(12) . . . 4_545 ?
O4 Na1 O8 Na5 41.38(10) 4_545 . . 4_545 ?
O2 Na1 O8 Na5 -37.48(9) 2 . . 4_545 ?
O1 Na1 O8 Na5 -151.20(12) . . . 4_545 ?
O7 Na1 O8 Na5 99.2(2) 4_545 . . 4_545 ?
Zn3 Na1 O8 Na5 -12.22(9) 2 . . 4_545 ?
Zn1 Na1 O8 Na5 -156.31(8) . . . 4_545 ?
Zn2 Na1 O8 Na5 -100.98(12) . . . 4_545 ?
Zn3 Na1 O8 Na5 -15.2(6) . . . 4_545 ?
O13 Na4 O3 C1 3.2(4) . . . . ?
O10 Na4 O3 C1 168.2(3) . . . . ?
O15 Na4 O3 C1 35.2(4) 7_556 . . . ?
O12 Na4 O3 C1 -115.9(4) 5_566 . . . ?
O9 Na4 O3 C1 92.6(4) 4 . . . ?
O12 Na4 O3 C1 -55.3(13) . . . . ?
O10 Na4 O3 C1 -75.1(4) 5_566 . . . ?
O5 Na4 O3 C1 160.6(4) 3_455 . . . ?
C4 Na4 O3 C1 151.6(4) . . . . ?
C4 Na4 O3 C1 -89.8(4) 5_566 . . . ?
Na4 Na4 O3 C1 -110.1(4) 5_566 . . . ?
O13 Na4 O3 Zn2 148.34(18) . . . 2 ?
O10 Na4 O3 Zn2 -46.7(2) . . . 2 ?
O15 Na4 O3 Zn2 -179.70(18) 7_556 . . 2 ?
O12 Na4 O3 Zn2 29.23(12) 5_566 . . 2 ?
O9 Na4 O3 Zn2 -122.30(15) 4 . . 2 ?
O12 Na4 O3 Zn2 89.7(12) . . . 2 ?
O10 Na4 O3 Zn2 69.98(14) 5_566 . . 2 ?
O5 Na4 O3 Zn2 -54.32(12) 3_455 . . 2 ?
C4 Na4 O3 Zn2 -63.3(4) . . . 2 ?
C4 Na4 O3 Zn2 55.31(13) 5_566 . . 2 ?
Na4 Na4 O3 Zn2 34.9(2) 5_566 . . 2 ?
O13 Na4 O3 Na2 -124.08(17) . . . . ?
O10 Na4 O3 Na2 40.9(2) . . . . ?
O15 Na4 O3 Na2 -92.11(17) 7_556 . . . ?
O12 Na4 O3 Na2 116.81(12) 5_566 . . . ?
O9 Na4 O3 Na2 -34.71(11) 4 . . . ?
O12 Na4 O3 Na2 177.3(11) . . . . ?
O10 Na4 O3 Na2 157.56(10) 5_566 . . . ?
O5 Na4 O3 Na2 33.27(9) 3_455 . . . ?
C4 Na4 O3 Na2 24.3(4) . . . . ?
C4 Na4 O3 Na2 142.89(13) 5_566 . . . ?
Na4 Na4 O3 Na2 122.52(14) 5_566 . . . ?
F2 Na2 O3 C1 80.8(3) 2 . . . ?
F2 Na2 O3 C1 -30.1(3) . . . . ?
O5 Na2 O3 C1 177.9(3) 3_455 . . . ?
O5 Na2 O3 C1 -92.3(4) 4 . . . ?
O9 Na2 O3 C1 -102.9(3) 4 . . . ?
O9 Na2 O3 C1 105.9(3) 3_455 . . . ?
O3 Na2 O3 C1 21.1(2) 2 . . . ?
Zn1 Na2 O3 C1 78.8(3) 2 . . . ?
Zn1 Na2 O3 C1 -63.0(3) . . . . ?
Zn2 Na2 O3 C1 -21.1(3) . . . . ?
Zn2 Na2 O3 C1 118.2(3) 2 . . . ?
F2 Na2 O3 Zn2 -37.40(10) 2 . . 2 ?
F2 Na2 O3 Zn2 -148.23(11) . . . 2 ?
O5 Na2 O3 Zn2 59.74(11) 3_455 . . 2 ?
O5 Na2 O3 Zn2 149.6(3) 4 . . 2 ?
O9 Na2 O3 Zn2 138.87(13) 4 . . 2 ?
O9 Na2 O3 Zn2 -12.3(2) 3_455 . . 2 ?
O3 Na2 O3 Zn2 -97.12(10) 2 . . 2 ?
Zn1 Na2 O3 Zn2 -39.42(10) 2 . . 2 ?
Zn1 Na2 O3 Zn2 178.86(13) . . . 2 ?
Zn2 Na2 O3 Zn2 -139.32(8) . . . 2 ?
F2 Na2 O3 Na4 -138.06(14) 2 . . . ?
F2 Na2 O3 Na4 111.11(13) . . . . ?
O5 Na2 O3 Na4 -40.92(11) 3_455 . . . ?
O5 Na2 O3 Na4 48.9(4) 4 . . . ?
O9 Na2 O3 Na4 38.21(12) 4 . . . ?
O9 Na2 O3 Na4 -112.97(17) 3_455 . . . ?
O3 Na2 O3 Na4 162.22(13) 2 . . . ?
Zn1 Na2 O3 Na4 -140.09(10) 2 . . . ?
Zn1 Na2 O3 Na4 78.19(10) . . . . ?
Zn2 Na2 O3 Na4 120.01(10) . . . . ?
Zn2 Na2 O3 Na4 -100.67(14) 2 . . . ?
O9 Zn1 F2 Zn2 83.2(2) 4 . . . ?
O4 Zn1 F2 Zn2 -35.3(2) . . . . ?
O1 Zn1 F2 Zn2 -153.7(2) . . . . ?
O15 Zn1 F2 Zn2 123.5(5) 7_556 . . . ?
O14 Zn1 F2 Zn2 -100.2(6) . . . . ?
Na5 Zn1 F2 Zn2 -4.6(3) . . . . ?
Na2 Zn1 F2 Zn2 112.1(2) . . . . ?
Na3 Zn1 F2 Zn2 -122.2(2) . . . . ?
Na1 Zn1 F2 Zn2 -111.2(2) . . . . ?
Na4 Zn1 F2 Zn2 128.9(2) . . . . ?
O9 Zn1 F2 Na2 -28.92(12) 4 . . . ?
O4 Zn1 F2 Na2 -147.40(11) . . . . ?
O1 Zn1 F2 Na2 94.27(11) . . . . ?
O15 Zn1 F2 Na2 11.4(5) 7_556 . . . ?
O14 Zn1 F2 Na2 147.7(5) . . . . ?
Na5 Zn1 F2 Na2 -116.64(11) . . . . ?
Na3 Zn1 F2 Na2 125.74(8) . . . . ?
Na1 Zn1 F2 Na2 136.70(14) . . . . ?
Na4 Zn1 F2 Na2 16.80(11) . . . . ?
O9 Zn1 F2 Na1 -165.61(12) 4 . . . ?
O4 Zn1 F2 Na1 75.90(12) . . . . ?
O1 Zn1 F2 Na1 -42.43(11) . . . . ?
O15 Zn1 F2 Na1 -125.3(5) 7_556 . . . ?
O14 Zn1 F2 Na1 11.0(5) . . . . ?
Na5 Zn1 F2 Na1 106.66(11) . . . . ?
Na2 Zn1 F2 Na1 -136.70(14) . . . . ?
Na3 Zn1 F2 Na1 -10.96(11) . . . . ?
Na4 Zn1 F2 Na1 -119.90(8) . . . . ?
O8 Zn2 F2 Zn1 81.3(2) . . . . ?
O3 Zn2 F2 Zn1 -159.7(2) 2 . . . ?
O6 Zn2 F2 Zn1 -34.5(2) 4 . . . ?
O12 Zn2 F2 Zn1 -123.6(4) 6_565 . . . ?
Na3 Zn2 F2 Zn1 -4.6(3) 4 . . . ?
Na2 Zn2 F2 Zn1 -111.5(2) . . . . ?
Na4 Zn2 F2 Zn1 -129.2(2) 2 . . . ?
Na1 Zn2 F2 Zn1 110.5(3) . . . . ?
Na5 Zn2 F2 Zn1 123.7(2) 4_545 . . . ?
O8 Zn2 F2 Na2 -167.16(12) . . . . ?
O3 Zn2 F2 Na2 -48.19(12) 2 . . . ?
O6 Zn2 F2 Na2 77.01(12) 4 . . . ?
O12 Zn2 F2 Na2 -12.1(5) 6_565 . . . ?
Na3 Zn2 F2 Na2 106.93(12) 4 . . . ?
Na4 Zn2 F2 Na2 -17.70(11) 2 . . . ?
Na1 Zn2 F2 Na2 -137.98(15) . . . . ?
Na5 Zn2 F2 Na2 -124.80(8) 4_545 . . . ?
O8 Zn2 F2 Na1 -29.18(11) . . . . ?
O3 Zn2 F2 Na1 89.78(12) 2 . . . ?
O6 Zn2 F2 Na1 -145.01(11) 4 . . . ?
O12 Zn2 F2 Na1 125.9(4) 6_565 . . . ?
Na3 Zn2 F2 Na1 -115.09(11) 4 . . . ?
Na2 Zn2 F2 Na1 137.98(15) . . . . ?
Na4 Zn2 F2 Na1 120.28(8) 2 . . . ?
Na5 Zn2 F2 Na1 13.18(10) 4_545 . . . ?
F2 Na2 F2 Zn1 -105.63(10) 2 . . . ?
O5 Na2 F2 Zn1 -1.3(2) 3_455 . . . ?
O5 Na2 F2 Zn1 111.70(11) 4 . . . ?
O9 Na2 F2 Zn1 23.61(11) 4 . . . ?
O9 Na2 F2 Zn1 178.61(14) 3_455 . . . ?
O3 Na2 F2 Zn1 -176.79(13) 2 . . . ?
O3 Na2 F2 Zn1 -47.08(10) . . . . ?
Zn1 Na2 F2 Zn1 -145.07(7) 2 . . . ?
Zn2 Na2 F2 Zn1 146.06(15) . . . . ?
Zn2 Na2 F2 Zn1 -67.15(10) 2 . . . ?
F2 Na2 F2 Zn2 108.31(10) 2 . . . ?
O5 Na2 F2 Zn2 -147.40(17) 3_455 . . . ?
O5 Na2 F2 Zn2 -34.36(11) 4 . . . ?
O9 Na2 F2 Zn2 -122.45(13) 4 . . . ?
O9 Na2 F2 Zn2 32.54(19) 3_455 . . . ?
O3 Na2 F2 Zn2 37.15(10) 2 . . . ?
O3 Na2 F2 Zn2 166.85(11) . . . . ?
Zn1 Na2 F2 Zn2 68.87(10) 2 . . . ?
Zn1 Na2 F2 Zn2 -146.06(15) . . . . ?
Zn2 Na2 F2 Zn2 146.78(7) 2 . . . ?
F2 Na2 F2 Na1 -1.38(10) 2 . . . ?
O5 Na2 F2 Na1 102.9(2) 3_455 . . . ?
O5 Na2 F2 Na1 -144.05(16) 4 . . . ?
O9 Na2 F2 Na1 127.86(18) 4 . . . ?
O9 Na2 F2 Na1 -77.1(2) 3_455 . . . ?
O3 Na2 F2 Na1 -72.54(15) 2 . . . ?
O3 Na2 F2 Na1 57.16(15) . . . . ?
Zn1 Na2 F2 Na1 -40.82(16) 2 . . . ?
Zn1 Na2 F2 Na1 104.25(17) . . . . ?
Zn2 Na2 F2 Na1 -109.69(18) . . . . ?
Zn2 Na2 F2 Na1 37.10(16) 2 . . . ?
F1 Na1 F2 Zn1 106.82(9) . . . . ?
O6 Na1 F2 Zn1 -34.70(11) . . . . ?
O4 Na1 F2 Zn1 -142.63(15) 4_545 . . . ?
O2 Na1 F2 Zn1 165.98(11) 2 . . . ?
O1 Na1 F2 Zn1 35.20(9) . . . . ?
O8 Na1 F2 Zn1 -122.31(11) . . . . ?
O7 Na1 F2 Zn1 29.02(17) 4_545 . . . ?
Zn3 Na1 F2 Zn1 147.96(7) 2 . . . ?
Zn2 Na1 F2 Zn1 -145.84(15) . . . . ?
Zn3 Na1 F2 Zn1 67.37(10) . . . . ?
F1 Na1 F2 Zn2 -107.33(9) . . . . ?
O6 Na1 F2 Zn2 111.14(11) . . . . ?
O4 Na1 F2 Zn2 3.2(2) 4_545 . . . ?
O2 Na1 F2 Zn2 -48.17(10) 2 . . . ?
O1 Na1 F2 Zn2 -178.96(13) . . . . ?
O8 Na1 F2 Zn2 23.54(9) . . . . ?
O7 Na1 F2 Zn2 174.86(12) 4_545 . . . ?
Zn3 Na1 F2 Zn2 -66.20(10) 2 . . . ?
Zn1 Na1 F2 Zn2 145.84(15) . . . . ?
Zn3 Na1 F2 Zn2 -146.78(7) . . . . ?
F1 Na1 F2 Na2 2.37(17) . . . . ?
O6 Na1 F2 Na2 -139.16(15) . . . . ?
O4 Na1 F2 Na2 112.91(19) 4_545 . . . ?
O2 Na1 F2 Na2 61.53(15) 2 . . . ?
O1 Na1 F2 Na2 -69.26(15) . . . . ?
O8 Na1 F2 Na2 133.24(16) . . . . ?
O7 Na1 F2 Na2 -75.4(2) 4_545 . . . ?
Zn3 Na1 F2 Na2 43.50(16) 2 . . . ?
Zn1 Na1 F2 Na2 -104.46(17) . . . . ?
Zn2 Na1 F2 Na2 109.70(18) . . . . ?
Zn3 Na1 F2 Na2 -37.08(17) . . . . ?
O11 C4 O12 Zn2 45.2(5) . . . 6_566 ?
O10 C4 O12 Zn2 -134.5(3) . . . 6_566 ?
Na4 C4 O12 Zn2 -163.5(2) . . . 6_566 ?
Na4 C4 O12 Zn2 -93.6(2) 5_566 . . 6_566 ?
O11 C4 O12 Na3 -64.4(5) . . . 7_556 ?
O10 C4 O12 Na3 115.9(3) . . . 7_556 ?
Na4 C4 O12 Na3 86.9(2) . . . 7_556 ?
Na4 C4 O12 Na3 156.8(3) 5_566 . . 7_556 ?
O11 C4 O12 Na4 138.7(3) . . . 5_566 ?
O10 C4 O12 Na4 -40.9(3) . . . 5_566 ?
Na4 C4 O12 Na4 -69.94(11) . . . 5_566 ?
O11 C4 O12 Na4 -151.3(4) . . . . ?
O10 C4 O12 Na4 29.0(3) . . . . ?
Na4 C4 O12 Na4 69.94(11) 5_566 . . . ?
O13 Na4 O12 C4 141.3(3) . . . . ?
O3 Na4 O12 C4 -158.8(11) . . . . ?
O10 Na4 O12 C4 -18.6(2) . . . . ?
O15 Na4 O12 C4 110.9(3) 7_556 . . . ?
O12 Na4 O12 C4 -100.3(2) 5_566 . . . ?
O9 Na4 O12 C4 54.3(3) 4 . . . ?
O10 Na4 O12 C4 -138.9(2) 5_566 . . . ?
O5 Na4 O12 C4 -16.1(2) 3_455 . . . ?
C4 Na4 O12 C4 -125.36(19) 5_566 . . . ?
Na4 Na4 O12 C4 -100.3(2) 5_566 . . . ?
O13 Na4 O12 Zn2 -68.4(3) . . . 6_566 ?
O3 Na4 O12 Zn2 -8.5(14) . . . 6_566 ?
O10 Na4 O12 Zn2 131.7(3) . . . 6_566 ?
O15 Na4 O12 Zn2 -98.7(3) 7_556 . . 6_566 ?
O12 Na4 O12 Zn2 50.0(3) 5_566 . . 6_566 ?
O9 Na4 O12 Zn2 -155.3(3) 4 . . 6_566 ?
O10 Na4 O12 Zn2 11.4(3) 5_566 . . 6_566 ?
O5 Na4 O12 Zn2 134.2(3) 3_455 . . 6_566 ?
C4 Na4 O12 Zn2 150.3(4) . . . 6_566 ?
C4 Na4 O12 Zn2 25.0(3) 5_566 . . 6_566 ?
Na4 Na4 O12 Zn2 50.0(3) 5_566 . . 6_566 ?
O13 Na4 O12 Na3 22.82(17) . . . 7_556 ?
O3 Na4 O12 Na3 82.7(12) . . . 7_556 ?
O10 Na4 O12 Na3 -137.13(16) . . . 7_556 ?
O15 Na4 O12 Na3 -7.56(15) 7_556 . . 7_556 ?
O12 Na4 O12 Na3 141.22(14) 5_566 . . 7_556 ?
O9 Na4 O12 Na3 -64.16(14) 4 . . 7_556 ?
O10 Na4 O12 Na3 102.64(11) 5_566 . . 7_556 ?
O5 Na4 O12 Na3 -134.61(11) 3_455 . . 7_556 ?
C4 Na4 O12 Na3 -118.5(2) . . . 7_556 ?
C4 Na4 O12 Na3 116.16(12) 5_566 . . 7_556 ?
Na4 Na4 O12 Na3 141.22(14) 5_566 . . 7_556 ?
O13 Na4 O12 Na4 -118.40(18) . . . 5_566 ?
O3 Na4 O12 Na4 -58.5(12) . . . 5_566 ?
O10 Na4 O12 Na4 81.65(13) . . . 5_566 ?
O15 Na4 O12 Na4 -148.78(19) 7_556 . . 5_566 ?
O12 Na4 O12 Na4 0.0 5_566 . . 5_566 ?
O9 Na4 O12 Na4 154.62(15) 4 . . 5_566 ?
O10 Na4 O12 Na4 -38.58(8) 5_566 . . 5_566 ?
O5 Na4 O12 Na4 84.17(11) 3_455 . . 5_566 ?
C4 Na4 O12 Na4 100.3(2) . . . 5_566 ?
C4 Na4 O12 Na4 -25.06(10) 5_566 . . 5_566 ?
O9 Zn1 O4 C2 -176.8(3) 4 . . . ?
O1 Zn1 O4 C2 -2.7(3) . . . . ?
F2 Zn1 O4 C2 -85.8(3) . . . . ?
O15 Zn1 O4 C2 101.9(3) 7_556 . . . ?
O14 Zn1 O4 C2 77.2(3) . . . . ?
Na5 Zn1 O4 C2 118.7(3) . . . . ?
Na2 Zn1 O4 C2 -115.8(3) . . . . ?
Na3 Zn1 O4 C2 26.9(3) . . . . ?
Na1 Zn1 O4 C2 -40.6(3) . . . . ?
Na4 Zn1 O4 C2 122.9(3) . . . . ?
O9 Zn1 O4 Na5 64.49(16) 4 . . . ?
O1 Zn1 O4 Na5 -121.41(12) . . . . ?
F2 Zn1 O4 Na5 155.51(10) . . . . ?
O15 Zn1 O4 Na5 -16.8(2) 7_556 . . . ?
O14 Zn1 O4 Na5 -41.57(17) . . . . ?
Na2 Zn1 O4 Na5 125.46(10) . . . . ?
Na3 Zn1 O4 Na5 -91.78(8) . . . . ?
Na1 Zn1 O4 Na5 -159.33(9) . . . . ?
Na4 Zn1 O4 Na5 4.2(2) . . . . ?
O9 Zn1 O4 Na1 -26.0(2) 4 . . 4 ?
O1 Zn1 O4 Na1 148.11(13) . . . 4 ?
F2 Zn1 O4 Na1 65.02(13) . . . 4 ?
O15 Zn1 O4 Na1 -107.3(2) 7_556 . . 4 ?
O14 Zn1 O4 Na1 -132.1(2) . . . 4 ?
Na5 Zn1 O4 Na1 -90.49(13) . . . 4 ?
Na2 Zn1 O4 Na1 34.97(18) . . . 4 ?
Na3 Zn1 O4 Na1 177.74(12) . . . 4 ?
Na1 Zn1 O4 Na1 110.18(11) . . . 4 ?
Na4 Zn1 O4 Na1 -86.3(2) . . . 4 ?
O14 Na5 O4 C2 -77.3(3) . . . . ?
O11 Na5 O4 C2 -160.3(3) 7_566 . . . ?
O2 Na5 O4 C2 96.4(3) 3 . . . ?
O8 Na5 O4 C2 173.9(3) 4 . . . ?
O15 Na5 O4 C2 -106.3(3) 7_556 . . . ?
O10 Na5 O4 C2 21.6(3) 3_545 . . . ?
O13 Na5 O4 C2 -55.7(3) 7_556 . . . ?
C5 Na5 O4 C2 -80.6(3) . . . . ?
Zn1 Na5 O4 C2 -119.6(3) . . . . ?
Zn3 Na5 O4 C2 58.0(3) 3 . . . ?
Zn2 Na5 O4 C2 149.8(3) 4 . . . ?
O14 Na5 O4 Zn1 42.32(18) . . . . ?
O11 Na5 O4 Zn1 -40.7(3) 7_566 . . . ?
O2 Na5 O4 Zn1 -144.04(13) 3 . . . ?
O8 Na5 O4 Zn1 -66.55(10) 4 . . . ?
O15 Na5 O4 Zn1 13.26(16) 7_556 . . . ?
O10 Na5 O4 Zn1 141.17(12) 3_545 . . . ?
O13 Na5 O4 Zn1 63.87(14) 7_556 . . . ?
C5 Na5 O4 Zn1 38.95(9) . . . . ?
Zn3 Na5 O4 Zn1 177.58(12) 3 . . . ?
Zn2 Na5 O4 Zn1 -90.58(9) 4 . . . ?
O14 Na5 O4 Na1 152.3(2) . . . 4 ?
O11 Na5 O4 Na1 69.2(3) 7_566 . . 4 ?
O2 Na5 O4 Na1 -34.08(11) 3 . . 4 ?
O8 Na5 O4 Na1 43.42(10) 4 . . 4 ?
O15 Na5 O4 Na1 123.23(17) 7_556 . . 4 ?
O10 Na5 O4 Na1 -108.87(11) 3_545 . . 4 ?
O13 Na5 O4 Na1 173.84(15) 7_556 . . 4 ?
C5 Na5 O4 Na1 148.92(9) . . . 4 ?
Zn1 Na5 O4 Na1 109.97(13) . . . 4 ?
Zn3 Na5 O4 Na1 -72.45(8) 3 . . 4 ?
Zn2 Na5 O4 Na1 19.38(9) 4 . . 4 ?
O9 Zn1 O1 C1 4.0(3) 4 . . . ?
O4 Zn1 O1 C1 -169.8(3) . . . . ?
F2 Zn1 O1 C1 -80.4(3) . . . . ?
O15 Zn1 O1 C1 78.9(3) 7_556 . . . ?
O14 Zn1 O1 C1 114.5(3) . . . . ?
Na5 Zn1 O1 C1 125.7(3) . . . . ?
Na2 Zn1 O1 C1 -34.9(3) . . . . ?
Na3 Zn1 O1 C1 144.2(3) . . . . ?
Na1 Zn1 O1 C1 -118.9(3) . . . . ?
Na4 Zn1 O1 C1 35.4(3) . . . . ?
O9 Zn1 O1 Na3 -140.16(15) 4 . . . ?
O4 Zn1 O1 Na3 46.01(17) . . . . ?
F2 Zn1 O1 Na3 135.44(12) . . . . ?
O15 Zn1 O1 Na3 -65.3(2) 7_556 . . . ?
O14 Zn1 O1 Na3 -29.69(18) . . . . ?
Na5 Zn1 O1 Na3 -18.46(16) . . . . ?
Na2 Zn1 O1 Na3 -179.04(10) . . . . ?
Na1 Zn1 O1 Na3 96.92(12) . . . . ?
Na4 Zn1 O1 Na3 -108.79(11) . . . . ?
O9 Zn1 O1 Na1 122.93(15) 4 . . . ?
O4 Zn1 O1 Na1 -50.91(15) . . . . ?
F2 Zn1 O1 Na1 38.52(10) . . . . ?
O15 Zn1 O1 Na1 -162.22(18) 7_556 . . . ?
O14 Zn1 O1 Na1 -126.60(17) . . . . ?
Na5 Zn1 O1 Na1 -115.37(9) . . . . ?
Na2 Zn1 O1 Na1 84.04(8) . . . . ?
Na3 Zn1 O1 Na1 -96.92(12) . . . . ?
Na4 Zn1 O1 Na1 154.29(9) . . . . ?
O12 Na3 O1 C1 171.3(3) 7_556 . . . ?
O11 Na3 O1 C1 -1.4(4) 1_545 . . . ?
O13 Na3 O1 C1 -103.7(4) 7_556 . . . ?
O7 Na3 O1 C1 88.1(4) 4_545 . . . ?
O14 Na3 O1 C1 -110.6(4) . . . . ?
O6 Na3 O1 C1 165.0(4) . . . . ?
C5 Na3 O1 C1 -86.1(4) . . . . ?
O15 Na3 O1 C1 -74.9(4) . . . . ?
Zn2 Na3 O1 C1 143.8(3) 4_545 . . . ?
Zn1 Na3 O1 C1 -136.6(4) . . . . ?
Zn3 Na3 O1 C1 58.7(3) . . . . ?
O12 Na3 O1 Zn1 -52.2(3) 7_556 . . . ?
O11 Na3 O1 Zn1 135.18(13) 1_545 . . . ?
O13 Na3 O1 Zn1 32.89(17) 7_556 . . . ?
O7 Na3 O1 Zn1 -135.39(13) 4_545 . . . ?
O14 Na3 O1 Zn1 25.91(15) . . . . ?
O6 Na3 O1 Zn1 -58.42(12) . . . . ?
C5 Na3 O1 Zn1 50.47(9) . . . . ?
O15 Na3 O1 Zn1 61.62(16) . . . . ?
Zn2 Na3 O1 Zn1 -79.63(12) 4_545 . . . ?
Zn3 Na3 O1 Zn1 -164.75(14) . . . . ?
O12 Na3 O1 Na1 39.6(3) 7_556 . . . ?
O11 Na3 O1 Na1 -133.01(12) 1_545 . . . ?
O13 Na3 O1 Na1 124.70(16) 7_556 . . . ?
O7 Na3 O1 Na1 -43.58(11) 4_545 . . . ?
O14 Na3 O1 Na1 117.72(16) . . . . ?
O6 Na3 O1 Na1 33.39(10) . . . . ?
C5 Na3 O1 Na1 142.28(10) . . . . ?
O15 Na3 O1 Na1 153.42(14) . . . . ?
Zn2 Na3 O1 Na1 12.18(12) 4_545 . . . ?
Zn1 Na3 O1 Na1 91.81(12) . . . . ?
Zn3 Na3 O1 Na1 -72.94(9) . . . . ?
F1 Na1 O1 C1 -32.0(3) . . . . ?
F2 Na1 O1 C1 84.0(3) . . . . ?
O6 Na1 O1 C1 -176.5(3) . . . . ?
O4 Na1 O1 C1 -99.5(4) 4_545 . . . ?
O2 Na1 O1 C1 23.6(3) 2 . . . ?
O8 Na1 O1 C1 111.1(3) . . . . ?
O7 Na1 O1 C1 -101.1(3) 4_545 . . . ?
Zn3 Na1 O1 C1 -20.6(3) 2 . . . ?
Zn1 Na1 O1 C1 119.5(3) . . . . ?
Zn2 Na1 O1 C1 83.3(3) . . . . ?
Zn3 Na1 O1 C1 -61.2(3) . . . . ?
F1 Na1 O1 Zn1 -151.44(12) . . . . ?
F2 Na1 O1 Zn1 -35.52(9) . . . . ?
O6 Na1 O1 Zn1 64.02(11) . . . . ?
O4 Na1 O1 Zn1 141.0(3) 4_545 . . . ?
O2 Na1 O1 Zn1 -95.91(13) 2 . . . ?
O8 Na1 O1 Zn1 -8.37(16) . . . . ?
O7 Na1 O1 Zn1 139.41(13) 4_545 . . . ?
Zn3 Na1 O1 Zn1 -140.07(9) 2 . . . ?
Zn2 Na1 O1 Zn1 -36.17(10) . . . . ?
Zn3 Na1 O1 Zn1 179.28(12) . . . . ?
F1 Na1 O1 Na3 108.82(12) . . . . ?
F2 Na1 O1 Na3 -135.27(13) . . . . ?
O6 Na1 O1 Na3 -35.72(11) . . . . ?
O4 Na1 O1 Na3 41.3(3) 4_545 . . . ?
O2 Na1 O1 Na3 164.35(12) 2 . . . ?
O8 Na1 O1 Na3 -108.11(15) . . . . ?
O7 Na1 O1 Na3 39.66(11) 4_545 . . . ?
Zn3 Na1 O1 Na3 120.19(10) 2 . . . ?
Zn1 Na1 O1 Na3 -99.74(13) . . . . ?
Zn2 Na1 O1 Na3 -135.91(9) . . . . ?
Zn3 Na1 O1 Na3 79.54(10) . . . . ?
O10 C4 O11 Na5 112.5(4) . . . 7_566 ?
O12 C4 O11 Na5 -67.1(5) . . . 7_566 ?
Na4 C4 O11 Na5 -177.2(4) . . . 7_566 ?
Na4 C4 O11 Na5 12.1(7) 5_566 . . 7_566 ?
O10 C4 O11 Na3 -77.4(4) . . . 1_565 ?
O12 C4 O11 Na3 103.0(4) . . . 1_565 ?
Na4 C4 O11 Na3 -7.2(7) . . . 1_565 ?
Na4 C4 O11 Na3 -177.8(3) 5_566 . . 1_565 ?
O11 C4 O10 Zn3 38.8(5) . . . 1_565 ?
O12 C4 O10 Zn3 -141.5(3) . . . 1_565 ?
Na4 C4 O10 Zn3 -106.1(3) . . . 1_565 ?
Na4 C4 O10 Zn3 -178.0(3) 5_566 . . 1_565 ?
O11 C4 O10 Na4 145.0(3) . . . . ?
O12 C4 O10 Na4 -35.4(4) . . . . ?
Na4 C4 O10 Na4 -71.85(13) 5_566 . . . ?
O11 C4 O10 Na5 -55.3(4) . . . 3_455 ?
O12 C4 O10 Na5 124.3(3) . . . 3_455 ?
Na4 C4 O10 Na5 159.7(2) . . . 3_455 ?
Na4 C4 O10 Na5 87.85(16) 5_566 . . 3_455 ?
O11 C4 O10 Na4 -143.2(4) . . . 5_566 ?
O12 C4 O10 Na4 36.5(3) . . . 5_566 ?
Na4 C4 O10 Na4 71.85(13) . . . 5_566 ?
O13 Na4 O10 C4 -4.0(3) . . . . ?
O3 Na4 O10 C4 -166.6(2) . . . . ?
O15 Na4 O10 C4 -45.4(3) 7_556 . . . ?
O12 Na4 O10 C4 128.6(2) 5_566 . . . ?
O9 Na4 O10 C4 -98.0(2) 4 . . . ?
O12 Na4 O10 C4 18.9(2) . . . . ?
O10 Na4 O10 C4 82.3(2) 5_566 . . . ?
O5 Na4 O10 C4 -158.5(3) 3_455 . . . ?
C4 Na4 O10 C4 108.3(2) 5_566 . . . ?
Na4 Na4 O10 C4 82.3(2) 5_566 . . . ?
O13 Na4 O10 Zn3 117.9(2) . . . 1_565 ?
O3 Na4 O10 Zn3 -44.7(2) . . . 1_565 ?
O15 Na4 O10 Zn3 76.5(2) 7_556 . . 1_565 ?
O12 Na4 O10 Zn3 -109.51(12) 5_566 . . 1_565 ?
O9 Na4 O10 Zn3 23.94(13) 4 . . 1_565 ?
O12 Na4 O10 Zn3 140.82(16) . . . 1_565 ?
O10 Na4 O10 Zn3 -155.82(14) 5_566 . . 1_565 ?
O5 Na4 O10 Zn3 -36.57(9) 3_455 . . 1_565 ?
C4 Na4 O10 Zn3 121.9(3) . . . 1_565 ?
C4 Na4 O10 Zn3 -129.77(12) 5_566 . . 1_565 ?
Na4 Na4 O10 Zn3 -155.82(14) 5_566 . . 1_565 ?
O13 Na4 O10 Na5 -152.6(2) . . . 3_455 ?
O3 Na4 O10 Na5 44.8(3) . . . 3_455 ?
O15 Na4 O10 Na5 166.0(2) 7_556 . . 3_455 ?
O12 Na4 O10 Na5 -20.0(2) 5_566 . . 3_455 ?
O9 Na4 O10 Na5 113.5(2) 4 . . 3_455 ?
O12 Na4 O10 Na5 -129.7(3) . . . 3_455 ?
O10 Na4 O10 Na5 -66.3(2) 5_566 . . 3_455 ?
O5 Na4 O10 Na5 53.0(2) 3_455 . . 3_455 ?
C4 Na4 O10 Na5 -148.6(4) . . . 3_455 ?
C4 Na4 O10 Na5 -40.2(3) 5_566 . . 3_455 ?
Na4 Na4 O10 Na5 -66.3(2) 5_566 . . 3_455 ?
O13 Na4 O10 Na4 -86.3(2) . . . 5_566 ?
O3 Na4 O10 Na4 111.08(18) . . . 5_566 ?
O15 Na4 O10 Na4 -127.7(2) 7_556 . . 5_566 ?
O12 Na4 O10 Na4 46.30(9) 5_566 . . 5_566 ?
O9 Na4 O10 Na4 179.76(13) 4 . . 5_566 ?
O12 Na4 O10 Na4 -63.36(11) . . . 5_566 ?
O10 Na4 O10 Na4 0.0 5_566 . . 5_566 ?
O5 Na4 O10 Na4 119.25(11) 3_455 . . 5_566 ?
C4 Na4 O10 Na4 -82.3(2) . . . 5_566 ?
C4 Na4 O10 Na4 26.05(10) 5_566 . . 5_566 ?
Zn1 O1 C1 O3 -12.2(5) . . . . ?
Na3 O1 C1 O3 118.8(4) . . . . ?
Na1 O1 C1 O3 -116.5(4) . . . . ?
Zn1 O1 C1 O2 167.6(3) . . . . ?
Na3 O1 C1 O2 -61.5(5) . . . . ?
Na1 O1 C1 O2 63.3(4) . . . . ?
Zn2 O3 C1 O1 165.3(3) 2 . . . ?
Na4 O3 C1 O1 -54.1(6) . . . . ?
Na2 O3 C1 O1 68.9(4) . . . . ?
Zn2 O3 C1 O2 -14.5(5) 2 . . . ?
Na4 O3 C1 O2 126.1(4) . . . . ?
Na2 O3 C1 O2 -110.9(4) . . . . ?
Zn3 O2 C1 O1 -1.7(5) . . . . ?
Na5 O2 C1 O1 125.8(4) 3_445 . . . ?
Na1 O2 C1 O1 -108.3(4) 2 . . . ?
Zn3 O2 C1 O3 178.1(3) . . . . ?
Na5 O2 C1 O3 -54.4(5) 3_445 . . . ?
Na1 O2 C1 O3 71.5(4) 2 . . . ?
Zn3 O7 C3 O9 -6.2(5) 4 . . . ?
Na3 O7 C3 O9 134.4(4) 4 . . . ?
Na1 O7 C3 O9 -112.0(4) 4 . . . ?
Zn3 O7 C3 O8 174.5(3) 4 . . . ?
Na3 O7 C3 O8 -44.9(5) 4 . . . ?
Na1 O7 C3 O8 68.7(4) 4 . . . ?
Zn1 O9 C3 O7 -169.3(3) 4_545 . . . ?
Na2 O9 C3 O7 67.8(5) 3_545 . . . ?
Na4 O9 C3 O7 -56.7(5) 4_545 . . . ?
Zn1 O9 C3 O8 10.0(6) 4_545 . . . ?
Na2 O9 C3 O8 -112.9(4) 3_545 . . . ?
Na4 O9 C3 O8 122.6(3) 4_545 . . . ?
Zn2 O8 C3 O7 -1.3(5) . . . . ?
Na5 O8 C3 O7 122.7(3) 4_545 . . . ?
Na1 O8 C3 O7 -123.9(4) . . . . ?
Zn2 O8 C3 O9 179.5(3) . . . . ?
Na5 O8 C3 O9 -56.5(5) 4_545 . . . ?
Na1 O8 C3 O9 56.8(5) . . . . ?
Zn3 O5 C2 O6 -163.9(3) 3 . . . ?
Na2 O5 C2 O6 49.8(5) 3_545 . . . ?
Na4 O5 C2 O6 -66.5(4) 3_545 . . . ?
Zn3 O5 C2 O4 15.6(5) 3 . . . ?
Na2 O5 C2 O4 -130.6(3) 3_545 . . . ?
Na4 O5 C2 O4 113.1(4) 3_545 . . . ?
Zn2 O6 C2 O5 14.3(5) 4_545 . . . ?
Na1 O6 C2 O5 -130.8(3) . . . . ?
Na3 O6 C2 O5 112.7(4) . . . . ?
Zn2 O6 C2 O4 -165.3(3) 4_545 . . . ?
Na1 O6 C2 O4 49.6(5) . . . . ?
Na3 O6 C2 O4 -66.9(4) . . . . ?
Zn1 O4 C2 O5 -167.5(3) . . . . ?
Na5 O4 C2 O5 -66.5(4) . . . . ?
Na1 O4 C2 O5 46.3(5) 4 . . . ?
Zn1 O4 C2 O6 12.1(5) . . . . ?
Na5 O4 C2 O6 113.1(4) . . . . ?
Na1 O4 C2 O6 -134.2(3) 4 . . . ?
O14 C5 O13 Na4 -160.8(8) 7_556 . . . ?
O14 C5 O13 Na4 19.2(8) . . . . ?
O13 C5 O13 Na4 23(100) 7_556 . . . ?
O15 C5 O13 Na4 -148.2(5) . . . . ?
O15 C5 O13 Na4 31.8(5) 7_556 . . . ?
Na3 C5 O13 Na4 -56.1(6) . . . . ?
Na3 C5 O13 Na4 123.9(6) 7_556 . . . ?
Na5 C5 O13 Na4 -110.4(5) 7_556 . . . ?
Na5 C5 O13 Na4 69.6(5) . . . . ?
O14 C5 O13 Na3 75.3(4) 7_556 . . 7_556 ?
O14 C5 O13 Na3 -104.7(4) . . . 7_556 ?
O13 C5 O13 Na3 -100(100) 7_556 . . 7_556 ?
O15 C5 O13 Na3 87.9(4) . . . 7_556 ?
O15 C5 O13 Na3 -92.1(4) 7_556 . . 7_556 ?
Na3 C5 O13 Na3 180.0 . . . 7_556 ?
Na5 C5 O13 Na3 125.7(3) 7_556 . . 7_556 ?
Na5 C5 O13 Na3 -54.3(3) . . . 7_556 ?
O14 C5 O13 Na5 -50.4(4) 7_556 . . 7_556 ?
O14 C5 O13 Na5 129.6(4) . . . 7_556 ?
O13 C5 O13 Na5 134(100) 7_556 . . 7_556 ?
O15 C5 O13 Na5 -37.8(3) . . . 7_556 ?
O15 C5 O13 Na5 142.2(3) 7_556 . . 7_556 ?
Na3 C5 O13 Na5 54.3(3) . . . 7_556 ?
Na3 C5 O13 Na5 -125.7(3) 7_556 . . 7_556 ?
Na5 C5 O13 Na5 180.0 . . . 7_556 ?
O3 Na4 O13 C5 40.0(6) . . . . ?
O10 Na4 O13 C5 -127.5(5) . . . . ?
O15 Na4 O13 C5 -27.1(4) 7_556 . . . ?
O12 Na4 O13 C5 111.4(5) 5_566 . . . ?
O9 Na4 O13 C5 -34.3(5) 4 . . . ?
O12 Na4 O13 C5 -145.5(6) . . . . ?
O10 Na4 O13 C5 129.9(6) 5_566 . . . ?
O5 Na4 O13 C5 -32.5(9) 3_455 . . . ?
C4 Na4 O13 C5 -129.3(5) . . . . ?
C4 Na4 O13 C5 112.9(5) 5_566 . . . ?
Na4 Na4 O13 C5 169.1(5) 5_566 . . . ?
O3 Na4 O13 Na3 162.74(17) . . . 7_556 ?
O10 Na4 O13 Na3 -4.7(3) . . . 7_556 ?
O15 Na4 O13 Na3 95.7(4) 7_556 . . 7_556 ?
O12 Na4 O13 Na3 -125.83(18) 5_566 . . 7_556 ?
O9 Na4 O13 Na3 88.47(19) 4 . . 7_556 ?
O12 Na4 O13 Na3 -22.72(16) . . . 7_556 ?
O10 Na4 O13 Na3 -107.37(19) 5_566 . . 7_556 ?
O5 Na4 O13 Na3 90.3(5) 3_455 . . 7_556 ?
C4 Na4 O13 Na3 -6.5(2) . . . 7_556 ?
C4 Na4 O13 Na3 -124.36(18) 5_566 . . 7_556 ?
Na4 Na4 O13 Na3 -68.1(2) 5_566 . . 7_556 ?
O3 Na4 O13 Na5 -64.4(2) . . . 7_556 ?
O10 Na4 O13 Na5 128.19(18) . . . 7_556 ?
O15 Na4 O13 Na5 -131.4(4) 7_556 . . 7_556 ?
O12 Na4 O13 Na5 7.1(3) 5_566 . . 7_556 ?
O9 Na4 O13 Na5 -138.63(18) 4 . . 7_556 ?
O12 Na4 O13 Na5 110.17(19) . . . 7_556 ?
O10 Na4 O13 Na5 25.52(16) 5_566 . . 7_556 ?
O5 Na4 O13 Na5 -136.8(4) 3_455 . . 7_556 ?
C4 Na4 O13 Na5 126.41(18) . . . 7_556 ?
C4 Na4 O13 Na5 8.5(2) 5_566 . . 7_556 ?
Na4 Na4 O13 Na5 64.8(2) 5_566 . . 7_556 ?
O14 C5 O15 Zn1 -31.2(4) 7_556 . . 7_556 ?
O14 C5 O15 Zn1 148.8(4) . . . 7_556 ?
O13 C5 O15 Zn1 137.3(5) 7_556 . . 7_556 ?
O13 C5 O15 Zn1 -42.7(5) . . . 7_556 ?
O15 C5 O15 Zn1 -164(100) 7_556 . . 7_556 ?
Na3 C5 O15 Zn1 -167.2(4) . . . 7_556 ?
Na3 C5 O15 Zn1 12.8(4) 7_556 . . 7_556 ?
Na5 C5 O15 Zn1 -81.7(4) 7_556 . . 7_556 ?
Na5 C5 O15 Zn1 98.3(4) . . . 7_556 ?
O14 C5 O15 Na4 -147.4(5) 7_556 . . 7_556 ?
O14 C5 O15 Na4 32.6(5) . . . 7_556 ?
O13 C5 O15 Na4 21.1(3) 7_556 . . 7_556 ?
O13 C5 O15 Na4 -158.9(3) . . . 7_556 ?
O15 C5 O15 Na4 80(100) 7_556 . . 7_556 ?
Na3 C5 O15 Na4 76.5(3) . . . 7_556 ?
Na3 C5 O15 Na4 -103.5(3) 7_556 . . 7_556 ?
Na5 C5 O15 Na4 162.0(4) 7_556 . . 7_556 ?
Na5 C5 O15 Na4 -18.0(4) . . . 7_556 ?
O14 C5 O15 Na5 50.6(3) 7_556 . . 7_556 ?
O14 C5 O15 Na5 -129.4(3) . . . 7_556 ?
O13 C5 O15 Na5 -140.9(4) 7_556 . . 7_556 ?
O13 C5 O15 Na5 39.1(4) . . . 7_556 ?
O15 C5 O15 Na5 -82(100) 7_556 . . 7_556 ?
Na3 C5 O15 Na5 -85.50(15) . . . 7_556 ?
Na3 C5 O15 Na5 94.50(15) 7_556 . . 7_556 ?
Na5 C5 O15 Na5 180.0 . . . 7_556 ?
O14 C5 O15 Na3 136.1(4) 7_556 . . . ?
O14 C5 O15 Na3 -43.9(4) . . . . ?
O13 C5 O15 Na3 -55.5(3) 7_556 . . . ?
O13 C5 O15 Na3 124.5(3) . . . . ?
O15 C5 O15 Na3 4(100) 7_556 . . . ?
Na3 C5 O15 Na3 180.0 7_556 . . . ?
Na5 C5 O15 Na3 85.50(15) 7_556 . . . ?
Na5 C5 O15 Na3 -94.50(15) . . . . ?
O1 Na3 O15 C5 -25.3(3) . . . . ?
O12 Na3 O15 C5 124.6(3) 7_556 . . . ?
O11 Na3 O15 C5 -109.1(3) 1_545 . . . ?
O13 Na3 O15 C5 57.2(4) 7_556 . . . ?
O7 Na3 O15 C5 -114.8(5) 4_545 . . . ?
O14 Na3 O15 C5 24.2(2) . . . . ?
O6 Na3 O15 C5 55.4(3) . . . . ?
Zn2 Na3 O15 C5 104.9(2) 4_545 . . . ?
Zn1 Na3 O15 C5 7.0(2) . . . . ?
Zn3 Na3 O15 C5 -82.8(3) . . . . ?
O1 Na3 O15 Zn1 122.9(8) . . . 7_556 ?
O12 Na3 O15 Zn1 -87.3(8) 7_556 . . 7_556 ?
O11 Na3 O15 Zn1 39.0(8) 1_545 . . 7_556 ?
O13 Na3 O15 Zn1 -154.6(10) 7_556 . . 7_556 ?
O7 Na3 O15 Zn1 33.3(12) 4_545 . . 7_556 ?
O14 Na3 O15 Zn1 172.3(9) . . . 7_556 ?
O6 Na3 O15 Zn1 -156.5(7) . . . 7_556 ?
C5 Na3 O15 Zn1 148.1(10) . . . 7_556 ?
Zn2 Na3 O15 Zn1 -107.0(8) 4_545 . . 7_556 ?
Zn1 Na3 O15 Zn1 155.1(8) . . . 7_556 ?
Zn3 Na3 O15 Zn1 65.3(8) . . . 7_556 ?
O1 Na3 O15 Na4 -142.69(15) . . . 7_556 ?
O12 Na3 O15 Na4 7.15(14) 7_556 . . 7_556 ?
O11 Na3 O15 Na4 133.43(19) 1_545 . . 7_556 ?
O13 Na3 O15 Na4 -60.2(3) 7_556 . . 7_556 ?
O7 Na3 O15 Na4 127.8(5) 4_545 . . 7_556 ?
O14 Na3 O15 Na4 -93.3(2) . . . 7_556 ?
O6 Na3 O15 Na4 -62.0(2) . . . 7_556 ?
C5 Na3 O15 Na4 -117.4(3) . . . 7_556 ?
Zn2 Na3 O15 Na4 -12.6(2) 4_545 . . 7_556 ?
Zn1 Na3 O15 Na4 -110.42(14) . . . 7_556 ?
Zn3 Na3 O15 Na4 159.79(11) . . . 7_556 ?
O1 Na3 O15 Na5 66.86(17) . . . 7_556 ?
O12 Na3 O15 Na5 -143.30(17) 7_556 . . 7_556 ?
O11 Na3 O15 Na5 -17.03(13) 1_545 . . 7_556 ?
O13 Na3 O15 Na5 149.4(4) 7_556 . . 7_556 ?
O7 Na3 O15 Na5 -22.7(6) 4_545 . . 7_556 ?
O14 Na3 O15 Na5 116.3(3) . . . 7_556 ?
O6 Na3 O15 Na5 147.53(14) . . . 7_556 ?
C5 Na3 O15 Na5 92.1(3) . . . 7_556 ?
Zn2 Na3 O15 Na5 -163.00(10) 4_545 . . 7_556 ?
Zn1 Na3 O15 Na5 99.12(14) . . . 7_556 ?
Zn3 Na3 O15 Na5 9.3(3) . . . 7_556 ?
O14 C5 O14 Zn1 -21(100) 7_556 . . . ?
O13 C5 O14 Zn1 159.5(7) 7_556 . . . ?
O13 C5 O14 Zn1 -20.5(7) . . . . ?
O15 C5 O14 Zn1 146.5(4) . . . . ?
O15 C5 O14 Zn1 -33.5(4) 7_556 . . . ?
Na3 C5 O14 Zn1 94.3(4) . . . . ?
Na3 C5 O14 Zn1 -85.7(4) 7_556 . . . ?
Na5 C5 O14 Zn1 69.2(6) 7_556 . . . ?
Na5 C5 O14 Zn1 -110.8(6) . . . . ?
O14 C5 O14 Na5 90(100) 7_556 . . . ?
O13 C5 O14 Na5 -89.7(5) 7_556 . . . ?
O13 C5 O14 Na5 90.3(5) . . . . ?
O15 C5 O14 Na5 -102.7(4) . . . . ?
O15 C5 O14 Na5 77.3(4) 7_556 . . . ?
Na3 C5 O14 Na5 -154.9(4) . . . . ?
Na3 C5 O14 Na5 25.1(4) 7_556 . . . ?
Na5 C5 O14 Na5 180.0 7_556 . . . ?
O14 C5 O14 Na3 -115(100) 7_556 . . . ?
O13 C5 O14 Na3 65.2(4) 7_556 . . . ?
O13 C5 O14 Na3 -114.8(4) . . . . ?
O15 C5 O14 Na3 52.2(4) . . . . ?
O15 C5 O14 Na3 -127.8(4) 7_556 . . . ?
Na3 C5 O14 Na3 180.0 7_556 . . . ?
Na5 C5 O14 Na3 -25.1(4) 7_556 . . . ?
Na5 C5 O14 Na3 154.9(4) . . . . ?
O9 Zn1 O14 C5 52.1(5) 4 . . . ?
O4 Zn1 O14 C5 168.7(5) . . . . ?
O1 Zn1 O14 C5 -71.4(5) . . . . ?
F2 Zn1 O14 C5 -124.3(5) . . . . ?
O15 Zn1 O14 C5 31.3(4) 7_556 . . . ?
Na5 Zn1 O14 C5 120.6(5) . . . . ?
Na2 Zn1 O14 C5 8.2(7) . . . . ?
Na3 Zn1 O14 C5 -97.6(5) . . . . ?
Na1 Zn1 O14 C5 -115.5(4) . . . . ?
Na4 Zn1 O14 C5 11.0(4) . . . . ?
O9 Zn1 O14 Na5 -68.4(2) 4 . . . ?
O4 Zn1 O14 Na5 48.17(16) . . . . ?
O1 Zn1 O14 Na5 168.06(18) . . . . ?
F2 Zn1 O14 Na5 115.1(5) . . . . ?
O15 Zn1 O14 Na5 -89.3(4) 7_556 . . . ?
Na2 Zn1 O14 Na5 -112.4(3) . . . . ?
Na3 Zn1 O14 Na5 141.8(3) . . . . ?
Na1 Zn1 O14 Na5 123.93(14) . . . . ?
Na4 Zn1 O14 Na5 -109.59(17) . . . . ?
O9 Zn1 O14 Na3 149.75(13) 4 . . . ?
O4 Zn1 O14 Na3 -93.65(16) . . . . ?
O1 Zn1 O14 Na3 26.24(15) . . . . ?
F2 Zn1 O14 Na3 -26.7(6) . . . . ?
O15 Zn1 O14 Na3 128.9(4) 7_556 . . . ?
Na5 Zn1 O14 Na3 -141.8(3) . . . . ?
Na2 Zn1 O14 Na3 105.8(3) . . . . ?
Na1 Zn1 O14 Na3 -17.9(2) . . . . ?
Na4 Zn1 O14 Na3 108.59(15) . . . . ?
O11 Na5 O14 C5 -19.2(4) 7_566 . . . ?
O2 Na5 O14 C5 177.4(2) 3 . . . ?
O4 Na5 O14 C5 -171.3(4) . . . . ?
O8 Na5 O14 C5 -103.7(4) 4 . . . ?
O15 Na5 O14 C5 -60.4(4) 7_556 . . . ?
O10 Na5 O14 C5 107.3(4) 3_545 . . . ?
O13 Na5 O14 C5 67.3(5) 7_556 . . . ?
Zn1 Na5 O14 C5 -131.7(5) . . . . ?
Zn3 Na5 O14 C5 146.6(3) 3 . . . ?
Zn2 Na5 O14 C5 -91.6(4) 4 . . . ?
O11 Na5 O14 Zn1 112.49(18) 7_566 . . . ?
O2 Na5 O14 Zn1 -50.9(4) 3 . . . ?
O4 Na5 O14 Zn1 -39.61(14) . . . . ?
O8 Na5 O14 Zn1 28.0(2) 4 . . . ?
O15 Na5 O14 Zn1 71.3(4) 7_556 . . . ?
O10 Na5 O14 Zn1 -121.07(17) 3_545 . . . ?
O13 Na5 O14 Zn1 -161.0(6) 7_556 . . . ?
C5 Na5 O14 Zn1 131.7(5) . . . . ?
Zn3 Na5 O14 Zn1 -81.78(19) 3 . . . ?
Zn2 Na5 O14 Zn1 40.1(3) 4 . . . ?
O11 Na5 O14 Na3 -156.2(4) 7_566 . . . ?
O2 Na5 O14 Na3 40.4(7) 3 . . . ?
O4 Na5 O14 Na3 51.7(4) . . . . ?
O8 Na5 O14 Na3 119.3(4) 4 . . . ?
O15 Na5 O14 Na3 162.6(7) 7_556 . . . ?
O10 Na5 O14 Na3 -29.7(4) 3_545 . . . ?
O13 Na5 O14 Na3 -69.7(5) 7_556 . . . ?
C5 Na5 O14 Na3 -137.0(7) . . . . ?
Zn1 Na5 O14 Na3 91.3(4) . . . . ?
Zn3 Na5 O14 Na3 9.5(5) 3 . . . ?
Zn2 Na5 O14 Na3 131.4(3) 4 . . . ?
O1 Na3 O14 C5 103.1(3) . . . . ?
O12 Na3 O14 C5 -109.8(3) 7_556 . . . ?
O11 Na3 O14 C5 21.6(3) 1_545 . . . ?
O13 Na3 O14 C5 -61.4(4) 7_556 . . . ?
O7 Na3 O14 C5 135.5(3) 4_545 . . . ?
O6 Na3 O14 C5 -179.2(3) . . . . ?
O15 Na3 O14 C5 -25.8(2) . . . . ?
Zn2 Na3 O14 C5 -151.7(3) 4_545 . . . ?
Zn1 Na3 O14 C5 127.2(4) . . . . ?
Zn3 Na3 O14 C5 91.5(3) . . . . ?
O1 Na3 O14 Zn1 -24.13(14) . . . . ?
O12 Na3 O14 Zn1 122.96(17) 7_556 . . . ?
O11 Na3 O14 Zn1 -105.61(17) 1_545 . . . ?
O13 Na3 O14 Zn1 171.4(5) 7_556 . . . ?
O7 Na3 O14 Zn1 8.3(4) 4_545 . . . ?
O6 Na3 O14 Zn1 53.59(15) . . . . ?
C5 Na3 O14 Zn1 -127.2(4) . . . . ?
O15 Na3 O14 Zn1 -153.0(3) . . . . ?
Zn2 Na3 O14 Zn1 81.08(17) 4_545 . . . ?
Zn3 Na3 O14 Zn1 -35.7(2) . . . . ?
O1 Na3 O14 Na5 -116.1(4) . . . . ?
O12 Na3 O14 Na5 31.0(5) 7_556 . . . ?
O11 Na3 O14 Na5 162.4(4) 1_545 . . . ?
O13 Na3 O14 Na5 79.4(6) 7_556 . . . ?
O7 Na3 O14 Na5 -83.7(5) 4_545 . . . ?
O6 Na3 O14 Na5 -38.4(4) . . . . ?
C5 Na3 O14 Na5 140.8(7) . . . . ?
O15 Na3 O14 Na5 115.1(5) . . . . ?
Zn2 Na3 O14 Na5 -10.9(5) 4_545 . . . ?
Zn1 Na3 O14 Na5 -92.0(4) . . . . ?
Zn3 Na3 O14 Na5 -127.7(4) . . . . ?

_diffrn_measured_fraction_theta_max 0.998
_diffrn_reflns_theta_full        25.99
_diffrn_measured_fraction_theta_full 0.998
_refine_diff_density_max         0.873
_refine_diff_density_min         -2.200
_refine_diff_density_rms         0.329
